Manipulating elastic wave propagation

in non-linear flexible materials

via external stimuli

Pavel I. Galich

Manipulating elastic wave propagation

in non-linear flexible materials

via external stimuli

Research thesis In Partial Fulfillment of the Requirements for the Degree of Doctor of Philosophy

Pavel I. Galich

Submitted to the Senate of the Technion - Israel Institute of Technology

Elul 5778, August 2018, Haifa

The Research Thesis Was Done Under the Supervision of Stephan Rudykh in the Faculty of Aerospace Engineering

Acknowledgements

The generous financial help of Technion – Israel Institute of Technology and The Irwin and Joan Jacobs Scholarship is gratefully acknowledged.

I am deeply thankful to Stephan Rudykh for his professional guidance, for sharing his knowledge and experience with me, and for his dedicated support through my Doctorate studies.

I thank Viacheslav (Slava) Slesarenko, Jian Li and Artemii Goshkoderia for useful discussions of my PhD research.

I wish to express my gratitude to the Israel Science Foundation for the financial support of my research.

Contents

Abstract1

List of abbreviations3

1 Preamble4

1.1 Wave propagation in non-linear elastic materials...... 5

1.1.1 Finitely deformed isotropic materials ...... 5

1.1.2 Finitely deformed laminates...... 5

1.1.3 Finitely deformed ﬁber-reinforced composites...... 7

1.2 Wave propagation in non-linear electroelastic materials ...... 9

2 Research methods 11

2.1 Non-linear elasticity ...... 11

2.1.1 Small amplitude motions superimposed on large deformations 13

2.2 Bloch-Floquet approach for periodic composites ...... 15

2.2.1 Static ﬁnite deformation ...... 15

2.2.2 Small-amplitude motions superimposed on a deformed state 16

2.3 Non-linear electroelasticity ...... 16 2.3.1 Electrostatics ...... 17

2.3.2 Mechanical balance laws...... 17

2.3.3 Constitutive equations...... 18

2.3.4 Incremental equations...... 18

2.3.5 Incremental motions superimposed on ﬁnite deformation in

the presence of an electric ﬁeld...... 19

2.3.6 Plane waves in incompressible DEs subjected to electrome-

chanical loading ...... 20

3 Findings 22

4 Conclusions and discussion 84

4.1 Inﬂuence of stiffening on elastic wave propagation in extremely de-

formed soft matter: from nearly incompressible to auxetic materials . 85

4.2 Manipulating pressure and shear waves in dielectric elastomers via

external electric stimuli...... 86

4.3 Elastic wave propagation in ﬁnitely deformed layered materials . . . 87

4.4 Shear wave propagation and band gaps in ﬁnitely deformed dielec-

tric elastomer laminates: long wave estimates and exact solution . . . 88

4.5 Shear wave propagation in ﬁnitely deformed 3D ﬁber-reinforced

composites ...... 89

Bibliography 91 Abstract

Understanding of wave propagation phenomena in solids is pivotal for numerous engineering applications in healthcare, petroleum, military, and aerospace indus- tries. Among them nondestructive material testing, vibration protection of sensi- tive electronics, unwanted noise mitigation, earthquake forecasting, and medical ultrasound diagnostics. The ability of ﬂexible materials to sustain large deforma- tions opens rich prospects for manipulating elastic wave characteristics by defor- mation. Moreover, elastic waves can be tuned through designing micro- or macro- structures, which can be further actively controlled by external stimuli, such as me- chanical loading, electric or magnetic ﬁelds. Understanding of how large deforma- tions affect relatively simple isotropic and more complex anisotropic materials is essential for this task. Therefore, in my thesis, I investigated the acoustic properties of the relatively simple initially isotropic non-linear materials and then proceeded with the periodic layered and ﬁber composites made of these materials. Firstly,

I studied the inﬂuence of the deformation induced stiffening (intrinsic feature of most soft materials) on the propagation of small-amplitude elastic plane waves.

Secondly, I showed that electroelastic isotropic materials (i.e. dielectric elastomers) can be utilized to achieve acoustic functionalities such as decoupling of pressure and shear waves by application of an electric ﬁeld. Thirdly, I analyzed wave prop- agation in non-linear elastic and electroelastic laminates. In particular, I derived the long wave estimates of the phase and group velocities for the waves propagat- ing in the laminates subject to external mechanical or electrical stimuli. Moreover, I found the material compositions and loading conditions producing wide complete

1 band gaps (frequency ranges where neither pressure nor shear waves can propa- gate) at desired low frequency ranges. Finally, I investigated the anisotropy of elastic wave propagation in ﬁnitely deformed ﬁber composites (FCs). Speciﬁcally, by employing rigorous analytical methods of non-linear mechanics, I derived long wave estimates for phase and group velocities of shear waves propagating in non- linear FCs. Next, by utilizing Bloch-Floquet approach in a ﬁnite element code,

I calculated dispersion relations for shear waves propagating along the ﬁbers in

FCs with square arrays of ﬁbers.

2 List of abbreviations

FC – Fiber composite

P-wave – Pressure (longitudinal) wave

S-wave – Shear (transversal) wave

BG – Band gap

SBG – Shear wave band gap

PBG – Pressure wave band gap

DE – Dielectric elastomer

RVE – Representative Volume Element

3 Chapter 1

Preamble

Lightweight composite materials with excellent mechanical properties are of im- mense importance for aerospace engineering [8]; however, in aerospace structures, undesirable vibrations and noise propagate from the source, e.g., an engine, to other parts; this phenomenon requires control, reduction, or even elimination.

Therefore, new lightweight materials allowing tunable noise and vibration reduc- tion need to be developed, while maintaining mechanical properties such as stiff- ness, toughness, and damage tolerance. Moreover, better understanding of wave propagation phenomena in ﬂexible materials can beneﬁt nondestructive material testing in composite aerospace structures. Motivated by these requirements for aerospace structural materials, in my PhD research I explored the general ﬁeld of elastic wave propagation in non-linear isotropic elastic [21] and electroelastic [22] materials and then in layered [19, 23] and ﬁbrous [25] composites made of these materials.

4 1.1 Wave propagation in non-linear elastic materials

1.1.1 Finitely deformed isotropic materials

Small amplitude elastic wave propagation in ﬁnitely deformed homogeneous isotropic materials was pioneered by Biot [5]. Boulanger and Hayes [6] considered wave propagation in ﬁnitely deformed incompressible Mooney-Rivlin materials and de- rived explicit relations for wave velocities. Boulanger et al. [7] extended this work to a broader class of ﬁnitely deformed compressible Hadamard materials and ﬁrst obtained the explicit expressions for the phase velocities of longitudinal (pressure) and transversal (shear) waves. Recently, Destrade and Ogden [15] have revised and generalized the problem of an inﬁnitesimal wave propagation in the ﬁnitely deformed hyperelastic materials by application of the invariant theory. More re- cently, I have investigated inﬁnitesimal (linear) wave propagation in ﬁnitely de- formed compressible Gent materials, exhibiting pronounced stiffening effects, and obtained closed form expressions for the phase velocities of longitudinal and transver- sal waves [21]. It is worth mentioning that deformation can be utilized not only for the changing of phase and group velocities of elastic waves but also for decou- pling of P- and S-waves in these relatively simple originally isotropic non-linear materials [9, 20].

1.1.2 Finitely deformed laminates

Small amplitude (linear) elastic wave propagation in linear bi-laminates made of isotropic materials was pioneered by by Rytov [43]. He derived explicit disper-

5 sion relations for steady-state P- and S-waves propagating perpendicular and par- allel to the layers. Recently, problem of wave propagation in periodic laminates has been revived in a framework of elastic metamaterials [53, 59]. Hence, I ex- tended classical result of Rytov [43] for non-linear bi-laminates made of hypere- lastic isotropic materials, namely neo-Hookean and Gent materials [19]. This al- lowed me to investigate inﬂuence of ﬁnite deformations on S- and P-wave band gaps in these laminates. In particular, I found that S-wave band gaps (SBGs) in laminates with compressible neo-Hookean layers are not inﬂuenced by defor- mation, because deformation-induced changes in geometry and effective material properties fully compensate each other. Thus, I corrected a misconception that had prevailed in the literature [47], namely that SBGs could be tuned by applica- tion of elastic deformation in compressible neo-Hookean laminates – I rigorously showed, through exact analytical solution, that they could not [19]. However, con- traction or extension of the laminate with Gent layers (exhibiting strong stiffening effects) widens and shifts up SBGs towards higher frequencies due to the stronger effect of deformation-induced change in the layer properties as compared to the change in the layer thicknesses. Moreover, I derived closed-form expressions for the phase and group velocities of long S-waves propagating in any direction in the

ﬁnitely deformed laminates with incompressible neo-Hookean layers. For the case of wave propagation perpendicular to the layers, I also obtained long wave esti- mates for the velocities of P- and S-waves propagating in laminates with compress- ible neo-Hookean or Gent layers [19]. More recently, Li et al. [32] studied oblique

S-wave propagation in ﬁnitely deformed laminates and showed that SBGs closes immediately when the wave inclines from the normal (i.e., perpendicular to the

6 layers) direction of propagation. Additionally, Li et al. [33] investigated inﬂuence of compressibility on BGs in buckled bi-laminates. Slesarenko et al. [50] found that shear waves of lowest frequencies in marginally stable bi-laminates (i.e., deformed close to the instability point) have negative (anti-parallel to the phase velocity) group velocities for certain wavenumbers, which foreshadow onset of elastic in- stability. Very recently, Demcenko et al. [13, 14] extended my analysis [19] and investigated propagation of ﬁnite amplitude elastic waves in hyperelastic lami- nates.

1.1.3 Finitely deformed ﬁber-reinforced composites

By employing the nonlinear elastic theory [57] and a phenomenological approach,

Scott and Hayes [46] considered small amplitude plane waves superimposed on a homogeneous deformation in the so-called idealized ﬁber-reinforced materials

(with an incompressible matrix and inextensible ﬁbers). The inﬁnitesimal elastic wave propagation in nearly incompressible and nearly inextensible ﬁber-reinforced materials with unidirectional ﬁbers was examined by Rogerson and Scott [38].

Later, Ogden and Singh [37] revisited the problem of inﬁnitesimal wave propa- gation in an incompressible transversely isotropic elastic solid in the presence of an initial stress. In particular, they exploited the phenomenological theory of in- variants and presented a more general and transparent formulation of the theory for small amplitude waves propagating in a deformed transversely isotropic hy- perelastic solid.

In my work [25], I employed a micromechanics based approach [11] accounting

7 for the phase properties and their spatial distribution to analyze the wave propa- gation in ﬁnitely deformed 3D FCs, as opposite to previous works that employed phenomenological approach [46, 44, 45, 38, 37], or numerically modeled the com- posites in 2D settings [3], or did not consider ﬁnite deformations [1, 30]. I derived explicit closed-form expressions for phase and group velocities of the S-waves for any direction of propagation in ﬁnitely deformed 3D FCs with neo-Hookean phases. These explicit expressions provide essential information on the S-wave propagation in the long wave limit. To account for the interaction of the S-waves with the composite microstructure, I implemented the Bloch-Floquet analysis [1,3] in the ﬁnite element code (COMSOL), allowing me to analyze small amplitude mo- tions superimposed on ﬁnite macroscopically applied homogeneous deformation.

Moreover, I compared the micromechanics-based homogenization approach and the numerical Bloch-Floquet analysis and showed the equivalence of these dis- tinct approaches for the large wavelengths [25]. More recently, I studied inﬂuence of ﬁber arrangement on shear waves and elastic instabilities in ﬁnitely deformed

FCs [24]. In particular, I showed that elastic instabilities and S-waves propagating along the ﬁbers in uniaxially deformed FCs can be tuned through the choice of the periodicity (or periodic unit cell aspect ratio b/a) of FCs. It worth mentioning that my numerical results on elastic instabilities in FCs with rectangular arrays of ﬁbers were validated by Li et al. [31] on 3D-printed FCs.

8 1.2 Wave propagation in non-linear electroelastic ma-

terials

Another part of my PhD research deals with problems of elastic wave propagation in dielectric elastomers (DEs) materials that can signiﬁcantly deform when sub- ject to an electric ﬁeld (Pelrine et al., 1998). Investigation of this problem opens new possibilities for improving small length-scale devices, e.g., micro-electromechanical systems in aerospace structures, where electric ﬁeld is the preferred control pa- rameter. Remarkably, even isotropic DEs allow to tune elastic wave propagation by an electric ﬁeld, e.g. one can decouple P- and S-waves propagating in DE via application of a speciﬁc electric ﬁeld [22]. However, for achieving more sophis- ticated wave phenomena, such as band gaps, structured materials must be intro- duced [61, 28].

Following the work of Toupin [56], the theory of nonlinear electroelasticity for homogeneous isotropic hyperelastic media has been revised recently by Dorfmann and Ogden [16], McMeeking and Landis [36], and Suo et al. [54]. More recently,

Cohen et al. [10] proposed a model based on considerations of polymer networks under electromechanical loadings. Motivated by potential enhancement of elec- tromechanical coupling, which is typically rather weak in DEs, microstructured

DEs have been explored [12, 55, 42] showing signiﬁcant potential of this approach.

However, one needs to account for electromechanical instabilities [40,4, 27] when dealing with composite DEs.

The analysis of small amplitude wave propagation in ﬁnitely deformed non- linear electroelastic materials in the presence of an electric ﬁeld in the frame of the

9 quasi-electrostatic approximation was presented by Dorfmann and Ogden [17].

This paper has been followed by a number of works on elastic wave propagation in ﬁnitely deformed homogenous and composite DEs [26, 48, 22, 60]. Note that layered DEs are of speciﬁc importance since they may be realized through various layer-by-layer material fabrication techniques which already allow manufacturing of deformable layered materials [39, 29].

During my PhD I revisited the problem of S-wave propagation perpendicularly to the layers in the laminates made of ideal (neo-Hookean) dielectric elastomers and corrected a misconception that had prevailed in the literature [48, 49], namely that SBGs could be shifted via application of an electric ﬁeld I rigorously demon- strated, through exact analytical solution, that they could not [23]. My results were recently conﬁrmed by Jandron and Henann [28].

10 Chapter 2

Research methods

2.1 Non-linear elasticity

Consider a continuum body and identify each point in the reference conﬁguration

with vector X. In the current conﬁguration, the new location of the corresponding points is deﬁned by vector x = x(X, t). Then, the deformation gradient is F =

∂x/∂X, and J ≡ det F > 0. For a hyperelastic compressible material with a strain

energy function ψ(F), the ﬁrst Piola-Kirchhoff stress tensor can be calculated as

follows ∂ψ(F) P = . (2.1) ∂F For an incompressible material, J = 1 and Eq. (2.1) modiﬁes as

∂ψ(F) P = − pF−T, (2.2) ∂F

where p represents an unknown Lagrange multiplier. The corresponding Cauchy stress tensor is related to the ﬁrst Piola-Kirchhoff stress tensor via the relation σ =

J−1P · FT.

11 In the absence of body forces the equations of motion can be written in the

undeformed conﬁguration as

D2χ DivP = ρ , (2.3) 0 Dt2

2 2 where ρ0 is the initial density of the material and the operator D (•)/Dt repre-

sents the material time derivative. If the deformation is applied quasi-statically, the

right hand part of (2.3) can be assumed to be zero, and the equilibrium equation

reads as

DivP = 0. (2.4)

Consider next inﬁnitesimal motions superimposed on the equilibrium state.

The equations of the incremental motions are

D2u DivP˙ = ρ , (2.5) 0 Dt2

where P˙ is the incremental change in the ﬁrst Piola-Kirchhoff stress tensor and u is

the incremental displacement.

The linearized constitutive law can be written as

P˙ij = A0ijkl F˙kl, (2.6) where F˙ = Grad u is the incremental change in the deformation gradient, and the

2 tensor of elastic moduli is deﬁned as A0iαkβ = ∂ ψ/∂Fiα∂Fkβ. Under substitution of

(2.6) into (2.5) the incremental motion equation takes the form

D2u A u = ρ i . (2.7) 0ijkl k,lj 0 Dt2

12 2.1.1 Small amplitude motions superimposed on large deforma-

tions

To analyze small amplitude motions superimposed on a ﬁnite deformation, we present equation of motion (2.7) in the updated Lagrangian formulation

∂2u A u = ρ i , (2.8) ijkl k,lj ∂t2

−1 −1 where Aiqkp = J A0ijkl Fpl Fqj is the updated tensor of elastic moduli and ρ = J ρ0 is the density of the deformed material.

We seek a solution for equation (2.8) in the form of plane waves with constant polarization

u = gh(n · x − ct), (2.9) where h is a twice continuously differentiable function and unit vector g denotes the polarization; the unit vector n deﬁnes the direction of wave propagation, and

c is the phase velocity of the wave.

Substituting (2.9) into (2.8), we obtain

Q(n) · g = ρc2g, (2.10) where

Qik = Aijklnjnl (2.11) is the acoustic tensor deﬁning the condition of propagation of the inﬁnitesimal plane waves. Thus, for a real wave to exist acoustic tensor has to be positively deﬁned for any non-zero vectors n and g

2 g · Q(n) · g = Aijklnjnl gigk = ρc > 0. (2.12)

13 Recall that the inequality

Aijklnjnl gigk > 0 (2.13) is called the strong ellipticity condition [57]. This inequality also arises in the sta- bility theory of elastic and elasto-plastic solids. Thus, if the inequality (2.13) does not hold true in any point of the body for the applied boundary conditions, the body is unstable in this state. In a similar vein, the body becomes unstable if the velocity of at least one wave with any polarization and any propagation direction in the body becomes zero. It is worth noting that loss of strong ellipticity analy- sis is widely used for ﬁnding macroscopic instabilities in homogenizable compos- ites [34, 35,2, 41].

For incompressible materials Eq. (2.8) modiﬁes as

∂2v A u + p˙ = ρ i , (2.14) ijkl k,lj ,i ∂t2

together with the incompressibility constraint

ui,i = 0. (2.15)

0 Substitution of (2.9) and p˙ = p0h (n · x − ct), where p0 is a scalar, into (2.14) and

(2.15) yields

Qˆ (n) · g = ρc2g and g · n = 0, (2.16) where Qˆ = Iˆ · Q · Iˆ and Iˆ = I − n ⊗ n is the projection onto the plane normal to n. Thus, in the incompressible case, the strong ellipticity condition (2.13) subject to the restriction g · n = 0. The readers, who are not familiar with non-linear elasticity, are referred to the book by Volokh [58] for comprehensible discussion and derivations of the material presented above.

14 2.2 Bloch-Floquet approach for periodic composites

To analyze elastic wave propagation in ﬁnitely deformed periodic composites, I

superimpose small amplitude (linear) motions on a ﬁnitely deformed state [3]. Re-

call that in a periodic structure plane waves can be described by the Bloch func-

tion [30]. To perform the analysis, I utilize the ﬁnite element method with the help

of COMSOL.

2.2.1 Static ﬁnite deformation

Firstly, the solution for the ﬁnitely deformed periodic composite is obtained. The

¯ = R macroscopic deformation gradient F 1/Ω Ω FdV is applied through periodic boundary conditions imposed on the displacements of the representative volume element (RVE) faces such that

UB − UA = (F¯ − I) · (XB − XA) , (2.17) where A and B are the nodes on the opposite faces of the RVE boundary and

U = x (X) − X is the displacement ﬁeld; RVE occupies a domain Ω in the un- deformed conﬁguration. The macroscopic ﬁrst Piola-Kirchhoff stress tensor and

¯ = R the corresponding Cauchy stress tensor are calculated as P 1/Ω Ω PdV and = R σ¯ 1/Ω Ω σdV, respectively. Rigid body motions are prevented by ﬁxing the displacements of a single node, i.e. UA = 0.

15 2.2.2 Small-amplitude motions superimposed on a deformed state

Secondly, the Bloch-Floquet periodicity conditions are superimposed on the de-

formed state. The corresponding incremental change in the displacement and the

ﬁrst Piola-Kirchhoff stress tensor are

u (X, t) = U (X) e−iωt and P˙ (X, t) = P (X) e−iωt, (2.18) where ω is the angular frequency. Substitution of (2.18) in (2.5) yields

2 DivP + ρ0ω U = 0. (2.19)

Next, according to the Floquet theorem

U (X + R) = U (X) e−iK·R and P (X + R) = P (X) e−iK·R, (2.20) where R deﬁnes the distance between the nodes on the opposite faces of the RVE in the reference conﬁguration, and K is the wavevector in the reference conﬁgu- ration. The periodicity conditions (2.20) are imposed in the ﬁnite element code through the corresponding boundary conditions for the displacements of the op- posite faces [3, 51]. The dispersion relations are obtained by solving the eigenvalue problem stemming from Eq. (2.18), (2.19) and (2.20) for a range of the wavevectors

K. Recall that the corresponding wavevector in the deformed conﬁguration can be found via relation k = F−T · K.

2.3 Non-linear electroelasticity

In this section, a brief description of non-linear electroelastic theory is presented.

For a full story, the readers are referred to the book by Dorfmann and Ogden [18]

16 and references therein.

2.3.1 Electrostatics

Here, the so-called quasi-electrostatic approximation assuming the absence of mag-

netic ﬁelds and neglecting electromagnetic interactions is adopted. Thus, in the

absence of free body charges and currents, the equations of electrostatics in the

current conﬁguration read as

divD = 0 and curlE = 0, (2.21)

where D and E denote electric displacement and electric ﬁeld applied in the current conﬁguration, respectively. Here and thereafter, the differential operators with the ﬁrst low-case letter refer to the current conﬁguration, while the differential operators with the ﬁrst upper-case letter refer to the reference conﬁguration.

In the reference conﬁguration, the equations of electrostatics read as

DivDL = 0 and CurlEL = 0, (2.22) where

−1 T DL = JF · D and EL = F · E (2.23) are the Lagrangian counterparts of D and E, respectively.

2.3.2 Mechanical balance laws

In the absence of body forces, the linear and angular momentum balance for an electroelastic material are

T divτ = ρx,tt and τ = τ , (2.24)

17 where τ represents the total Cauchy stress tensor (current conﬁguration).

In Lagrangian description the balance equations (2.24) read as

T T DivP = ρ0x,tt and P · F = F · P , (2.25) where

P = Jτ · F−T (2.26) is the ﬁrst Piola-Kirchhoff total stress tensor (reference conﬁguration).

2.3.3 Constitutive equations

To model non-linear behavior of DEs, an energy potential ψ(F, DL), as introduced in Dorfmann and Ogden [16], is considered. The strain energy-density potential is a function of deformation gradient F and Lagrangian counterpart of electric dis- placement DL. Then, for an electroelastic material, the ﬁrst Piola-Kirchhoff total stress tensor and Lagrangian counterpart of electric ﬁeld are given by

∂ψ ∂ψ P = and EL = . (2.27) ∂F ∂DL

For an incompressible material, J = 1, and the constitutive equations (2.27) modify

as

∂ψ −T ∂ψ P = − pF and EL = . (2.28) ∂F ∂DL

2.3.4 Incremental equations

For an electroelastic material, the incremental constitutive equations for the ﬁrst

Piola-Kirchhoff stress and Lagrangian electric ﬁeld read as

P˙ = C0 : F˙ + M0 · D˙ L and E˙ L = F˙ : M0 + K0 · D˙ L, (2.29)

18 respectively. Here, the superposed dot represent incremental changes in the cor-

responding variables; C0, M0, and K0 are the tensors of electroelastic moduli de-

ﬁned as ∂2ψ ∂2ψ ∂2ψ C0 = , M0 = and K0 = . (2.30) ∂F∂F ∂F∂DL ∂DL∂DL For an incompressible material, the incremental equations (2.29) read as

−T T −T −T P˙ = C0 : F˙ + pF · F˙ · F − p˙F + M0 · D˙ L and E˙ L = F˙ : M0 + K0 · D˙ L.

(2.31)

2.3.5 Incremental motions superimposed on ﬁnite deformation in

the presence of an electric ﬁeld

In a framework of the updated Lagrangian formulation, the incremental forms of the governing Eqs. (2.22) and (2.25)1, describing small motions superimposed on

ﬁnite deformation, transform to

divD˙ L? = 0, curlE˙ L? = 0, and divP˙ ? = ρx˙ ,tt, (2.32) where

−1 −T −1 T D˙ L? = J F · D˙ L, E˙ L? = F · E˙ L, and P˙ ? = J P˙ · F (2.33) are the so-called push-forward versions of D˙ L, E˙ L, and P˙ , respectively. Identifying the ﬁeld of incremental displacements as u = x˙ and then displacement gradient as H = gradu = F˙ · F−1, the following updated incremental relations (2.29) are obtained

P˙ ? = C : H + M· D˙ L? and E˙ L? = H : M + K · D˙ L?, (2.34)

19 where

−1 −1 −T −1 Cirks = J C0ijkl FrjFsl, Mirk = M0ijmFrjFmk and K = JF · K0 · F (2.35) are the updated tensors of electroelastic moduli, enjoying the following symme- tries

T Cirks = Cksir, Mirk = Mrik, and K = K . (2.36)

For an incompressible material, the incremental equations (2.34) read as

T P˙ ? = C : H + pH − p˙I + M· D˙ L? and E˙ L? = H : M + K · D˙ L?; (2.37) moreover, the incompressibility assumption implies

trH ≡ divu = 0. (2.38)

2.3.6 Plane waves in incompressible DEs subjected to electrome-

chanical loading

The solution of Eqs. (2.32) is sought in the form of plane waves with constant po- larizations [17]

u = g f (n · x − ct), D˙ L? = dg(n · x − ct), and p˙ = Π(n · x − ct), (2.39) where f , g, and Π are arbitrary twice continuously differentiable, continuously differentiable, and continuous functions, respectively; as before, the unit vectors g and d represent polarization vectors of mechanical and electrical displacements, respectively; the unit vector n denotes the direction of wave propagation, and c is the phase velocity of the wave.

20 Substitution of (2.37) and (2.39) into (2.32) and (2.38) yields

Aˆ · g = ρc2g and g · n = 0, (2.40) where Aˆ is the so-called generalized acoustic tensor deﬁning the condition of prop- agation of plane elastic waves in an incompressible electroelastic solid. The gener- alized acoustic tensor for an electroelastic material with an arbitrary energy poten- tial ψ(F, DL) can be calculated as follows [52]

2 Aˆ = Qˆ − Rˆ · (trKˆ )Iˆ − Kˆ · Rˆ T, (2.41) (trKˆ )2 − trKˆ 2 where Kˆ = Iˆ · K · Iˆ, Qˆ = Iˆ · Q · Iˆ, Rˆ = Iˆ · R · Iˆ, and

Qik = Cijklnjnl and R = n ·M. (2.42)

The generalized acoustic tensor Aˆ is symmetric. Recall that an incompressible elec- troelastic material is strongly elliptic (stable), if its generalized acoustic tensor Aˆ is positively deﬁned, i.e. g · Aˆ · g > 0 for any unit vectors n and g satisfying the incompressibility constraint (J = 1) n · g = 0 along an electromechanical loading path deﬁned through a combination of DL and F.

21 Chapter 3

Findings

This chapter contains the ﬁndings of the research conducted to fulﬁll the require- ments of the Graduate School of the Technion – Israel Institute of Technology. The thesis submitted as a collection of papers, which were published in peer-reviewed scientiﬁc journals. The list of published papers is cited below.

List of published papers:

1. P. I. Galich and S. Rudykh, Inﬂuence of stiffening on elastic wave propagation

in extremely deformed soft matter: from nearly incompressible to auxetic

materials. Extreme Mech. Lett., 4, 156-161 (2015).

2. P. I. Galich and S. Rudykh, Manipulating pressure and shear waves in dielec-

tric elastomers via external electric stimuli. Int. J. Solids Struct., 91, 18-25

(2016).

3. P. I. Galich, N. X. Fang, M. C. Boyce, and S. Rudykh, Elastic wave propagation

in ﬁnitely deformed layered materials. J. Mech. Phys. Solids, 98, 390-410

22 (2017).

4. P. I. Galich and S. Rudykh, Shear wave propagation and band gaps in ﬁnitely

deformed dielectric elastomer laminates: long wave estimates and exact so-

lution. J. Appl. Mech., 84(9), 91002 (2017).

5. P. I. Galich, V. Slesarenko, and S. Rudykh, Shear wave propagation in ﬁnitely

deformed 3D ﬁber-reinforced composites. Int. J. Solids Struct., 110-111, 294-

304 (2017).

23 Extreme Mechanics Letters 4 (2015) 156–161

Contents lists available at ScienceDirect

Extreme Mechanics Letters

journal homepage: www.elsevier.com/locate/eml

Influence of stiffening on elastic wave propagation in extremely deformed soft matter: from nearly incompressible to auxetic materials Pavel I. Galich, Stephan Rudykh ∗ Department of Aerospace Engineering, Technion - Israel Institute of Technology, Haifa 32000, Israel article info a b s t r a c t

Article history: We analyse the propagation of elastic waves in soft materials subjected to finite defor- Received 5 April 2015 mations. We derive explicit phase velocity relations for matter with pronounced stiffen- Received in revised form 9 June 2015 ing effect, namely Gent model, and apply these results to study elastic wave propagation Accepted 10 June 2015 in (a) nearly incompressible materials such as biological tissues and polymers, (b) highly Available online 14 June 2015 compressible and (c) negative Poisson’s ratio or auxetic materials. We find, that for nearly incompressible materials transverse wave velocities exhibit strong dependence on the di- Keywords: rection of propagation and initial strain state, whereas the longitudinal wave velocity is Elastic waves Finite deformations not affected significantly until extreme levels of deformation are attained. For highly com- Soft materials pressible materials, we show that both longitudinal and transversal wave velocities depend Compressible materials strongly on deformation and direction of propagation. Moreover, the dependence becomes Stiffening stronger when stiffening effects increase. When compression is applied, the longitudinal Auxetics wave velocity decreases regardless the direction of wave propagation in highly compress- ible materials, and increases for most of the directions in materials with negative Poisson’s ratio behaviour. We demonstrate that finite deformations can influence elastic wave prop- agation through combinations of induced effective compressibility and stiffness. © 2015 Elsevier Ltd. All rights reserved.

1. Introduction sustain large deformations, open promising opportuni- ties of manipulating acoustic characteristics via deforma- The propagation of elastic waves has been investigated tion [21–23]. intensively [1–16] because the understanding of the phe- In this work, we derive explicit phase velocity rela- nomenon is vital for a large variety of applications from tions for finitely deformed materials, which stiffen when non-invasive material testing and medical imaging for stretched/compressed. Our analysis is based on the the- health care to petroleum exploration. Recently, the field ory first developed by Hadamard [2], which was recently of acoustic or phononic metamaterials has attracted con- revised by Destrade and Ogden [11]. We specify the the- siderable attention. The peculiarity of these metamateri- ory for the class of Gent materials, and obtain compact als originates in their microstructure [17,18], which can explicit expressions of phase velocities for any finite de- be tailored to give rise to various effects such as local formation and direction of propagation. The availability of resonances [19], band-gaps [12] and cloaking [20]. Fur- explicit relations for phase velocity is important for design- thermore, soft metamaterials, due to their capability to ing mechanotunable acoustic metamaterials. Moreover, the information may benefit non-invasive medical diagnos- tic techniques by providing important information on the ∗ Corresponding author. dependence of elastic wave propagation on pre-stress/ E-mail address: [email protected] (S. Rudykh). pre-strain conditions, which are common in biological http://dx.doi.org/10.1016/j.eml.2015.06.003 2352-4316/© 2015 Elsevier Ltd. All rights reserved. P.I. Galich, S. Rudykh / Extreme Mechanics Letters 4 (2015) 156–161 157 tissues. By application of the derived explicit expressions, we show the role of deformation and significant influence of stiffening effects on wave propagation in soft media undergoing finite deformations. Moreover, we extend the analysis to a class of exotic metamaterials characterized by negative Poisson’s ratio (NPR) behaviour. Examples of NPR materials, also known as auxetics, include living bone tis- sue [24], skin [25], blood vessels [26], certain rocks and minerals [25], and artificial materials [27]. As we shall show, elastic wave propagation in these materials is sig- nificantly affected by deformation. In our analysis, we Fig. 1. Direction of propagation n relating to principal directions in general case (a) and when n lies in one of the planes of orthotropy treat the materials as continuous media; their overall ho- (b). Here (e1, e2, e3) is orthonormal basis of eigenvectors of left mogenized behaviour is characterized by effective elastic Cauchy–Green tensor B. moduli. These material properties may originate in so- phisticatedly engineered microstructures that give rise to which is a compressible extension of the neo-Hookean remarkable overall properties (for example, negative Pois- strain–energy function [33]. son’s ratio or/and bulk modulus). The information on Recall the definition of an acoustic tensor [2,4] which elastic wave propagation in terms of the effective proper- defines the condition of propagation of plane waves ties can guide the design of new tunable metamaterials. Moreover, this information can shed light on the distinct Q(n) = A(1324) : n ⊗ n, (3) roles of geometrical changes and material non-linearities where the unit vector n defines the direction of propa- occurring in tunable metamaterials due to large deforma- (2134) tions [28]. Furthermore, even simple homogeneous mate- = −1 · (2134) · T gation of the wave; A J F A0 F and rials can behave like smart metamaterials when finitely 2 = ∂ ψ are tensors of elastic moduli in current and ref- deformed. For example, they can be used to disentangle A0 ∂F∂F shear and pressure waves [23,29]. erence configuration respectively; superscripts (1324) and (2134) denote isomers of the fourth-rank tensors [34,35], as detailed in Appendix A. 2. Analysis Strong stiffening. Acoustic tensor for finitely deformed Gent material (1) takes the form To analyse the finitely deformed state, we introduce the deformation gradient F(X, t) = ∇ ⊗ x(X, t), where µ K 2 2 2 X Q(n) = 1 + − − J n ⊗ n X and x are position vectors in the reference and current J µ 3 Jm configurations, respectively. To take into account the non- µJm linear effects of the finite deformation as well as material + ξ(n · B · n)I + 2n ⊗ n : B ⊗ B(1324) , (4) 2 non-linearity, we analyse the wave propagation in terms Jξ of infinitesimal plane waves superimposed on a finitely (1324) where ξ = 3+Jm −I1, I is the identity tensor, and B⊗B deformed state [2,4]. To account for the stiffening effects is the fourth-rank tensor isomer (see Appendices A andB). (due to, for example, finite extensibility of polymer chains, General case. One can conclude from (4) that in general or due to collective straightening of collagen fibres in case (when n does not lie in any plane of orthotropy biological tissues) in finitely deformed media, we make use (Fig. 1(a)) and deformations are different along each of the strain–energy density function corresponding to an principal axis, i.e. all eigenvalues of tensor B are different) approximation of the Arruda–Boyce model [30], namely the waves are neither purely longitudinal nor purely the Gent model [31,32] which is given in Eq. (1). transversal (for details see Appendix B). µJm I1 − 3 Case 1. If wave vector n lies in one of the planes of ψ(F) = − ln 1 − − µ ln J orthotropy (Fig. 1(b)) then we always have one purely 2 Jm transversal wave with the velocity K µ µ + − − (J − 1)2, (1) c = µ(n · B · n)J /(ρ ξ), (5) 2 3 Jm tr m 0 where µ is the initial shear modulus, K is the initial bulk where ρ0 is the density of the undeformed material. modulus, I1 = tr B is the first invariant of the left Cauchy– Any finite deformation F at a homogeneous state can be Green tensor B = F · FT , and J = det F. The model neatly represented as covers the stiffening of the material with the deformation; F = λ1e1 ⊗ e1 + λ2e2 ⊗ e2 + λ3e3 ⊗ e3, (6) as the first strain invariant approaches I1 = 3 + Jm, the en- ergy function becomes unbounded and a dramatic increase where λ1,2,3 are stretch ratios along principal directions. in stress occurs. Consequently, Jm is a locking parameter. Thus, expression (5) holds true for any combination of λ1, Clearly, when Jm → ∞, the strain–energy function (1) re- λ2 and λ3. duces to Case 2. When wave vector n lies in one of the planes of orthotropy (for example in e1 − e2) and stretch ratios µ 2 ψ(F) = (I1 − 3) − µ ln J + (K/2 − µ/3) (J − 1) , (2) in this plane are equal (λ = λ = λˆ) then we have 2 1 2 158 P.I. Galich, S. Rudykh / Extreme Mechanics Letters 4 (2015) 156–161 one longitudinal and two transversal polarizations with a b following velocities 2 −2 ˆ 2 ˆ 2 cl = µ 1 + ηJ + Jmξ ξ + 2λ λ /ρ0 (7) and ˆ ctr = λ µJm/(ρ0ξ) (8) respectively, with η = K/µ − 2/3 − 2/Jm. Case 3. For waves propagating along the principal direc- d tion (n = ei), the velocities of longitudinal and transversal c waves are = + 2 + −2 + 2 2 cl µ 1 ηJ Jmξ ξ 2λi λi /ρ0 (9) and ctr = λi µJm/(ρ0ξ). (10) Case 4. When materials undergo so-called uniform dilatation or compaction (λ1 = λ2 = λ3 or F = qI), then Fig. 2. Polar diagrams of the phase velocities in nearly incompressible we have only pure modes with the velocities given by materials: for the purely transversal (a), quasi-longitudinal (b), quasi- transversal (d) waves in Gent material with J = 3 and K/µ = 300; m = + 4 + −2 + 2 2 and for the purely transversal (c) wave in neo-Hookean material with cl µ 1 ηq Jmξ ξ 2q q /ρ0 (11) K/µ = 300. and where ν is Poisson’s ratio. Thus, −1/3 < K/µ < ∞ ctr = q µJm/(ρ0ξ). (12) with µ > 0. Note that for −1/3 < K/µ < 0 the Weak stiffening. In case of a weak stiffening effect, material is stable only if constrained [34,36,37]. It follows namely, J → ∞, the acoustic tensor (4) reduces to the m from (15) that matter exhibits auxetic behaviour when well-known expression [9] −1/3 < K/µ < 2/3. Q(n) = a1n ⊗ n + a2(I − n ⊗ n), (13) Nearly incompressible materials. For nearly incom- ˜ −1/2 where n⊗n is the projection on the direction n; (I−n⊗n) pressible materials (K/µ ≫ 1 and λ ≃ λ ) the depen- dence of the longitudinal wave velocity on the direction is the projection on the plane normal to n; a1 = (K − −1 −1 of propagation and initial stress state is relatively weak 2µ/3)J + µJ (1 + n · B · n) and a2 = µJ (n · B · n). Consequently, there always exist one longitudinal and two unless extreme levels of deformation are attained. Fig. 2 transverse waves for any direction of propagation n. Phase shows the polar diagrams of the phase velocities for the velocities√ of these waves√ can be calculated as [13] cl = nearly incompressible Gent and neo-Hookean materials a1J/ρ0 and ctr = a2J/ρ0. In the√ small deformation under extreme levels of deformation. Here and thereafter limit these√ formulae reduce to cl = (K + 4µ/3)/ρ0 and the velocities are normalized by their value in the unde- ctr = µ/ρ0. It is worth mentioning that Boulanger and formed state; c1 and c2 are phase velocities along prin- Hayes [13,16] presented explicit phase velocity expres- cipal directions e1 and e2, correspondingly; more details sions for wide classes of Hadamard and Mooney–Rivlin on phase velocity or slowness surfaces can be found in materials; however, the Gent material model, considered the textbooks of Auld [38] or Nayfeh [39]. At the extreme here, does not belong to these classes of hyperelastic ma- levels of deformations, the stiffening effect manifests in a terials. significant increase of the effective shear modulus, which becomes comparable with the bulk modulus (see Eq. (9)). 3. Examples Fig. 2(b) shows that velocity of longitudinal wave increases in both compressed and stretched materials. Moreover, To illustrate the dependence of wave propagation on stiffening of the material gives rise to the dramatic de- the deformation and direction of propagation, we consider pendence of transversal wave velocities on the direction the case of uniaxial tension of propagation and deformation as compared to the ma- ˜ F = λe1 ⊗ e1 + λ(I − e1 ⊗ e1), (14) terials with weak stiffening effect (compare Fig. 2(a) and (d) vs (c)). Besides, we observe that the dependence of the ˜ = ˜ where λ is the applied stretch ratio and λ λ(λ, K/µ) is phase velocities on deformation and propagation direction defined through and the compressibility of the material. λ increases when the locking parameter J decreases (which Remind that the compressibility of the material is defined m corresponds to an earlier stiffening of the material with de- by the ratio K/µ. In the linear elastic limit the elastic formation). Comparing the quasi-transversal wave veloc- moduli are related through ity profiles with the purely transversal ones on the Fig. 2, K 2(1 + ν) we observe that the velocity of quasi-transversal wave has = , (15) µ 3(1 − 2ν) maxima for the non-principal directions (Fig. 2(d)). Note P.I. Galich, S. Rudykh / Extreme Mechanics Letters 4 (2015) 156–161 159

ab

a 1.05

cd 1.00 λ

0.95

0.90 Fig. 3. Polar diagrams of the phase velocities in highly compressible materials: for the quasi-longitudinal (a) and purely transversal (c) waves in Gent material with Jm = 3 and K/µ = 1; for the purely longitudinal (b) and transversal (d) waves in neo-Hookean material with K = 1. /µ 0.85 0.4 0.6 0.8 1.0 λ that this phenomenon is not observed in Hadamard mate- b 0.50 rials [40,41]. Highly compressible materials. In contrast to nearly incompressible materials, for highly compressible matter, 0.25 the velocity of longitudinal wave depends strongly on the direction of propagation and initial deformation state 0.00 even for moderate levels of deformation. More specifically Fig. 3(a) and (b) show that the velocity of pressure wave –0.25 increases when material is stretched and decreases when it is compressed. Propagation of shear waves in highly compressible media differs significantly from the one –0.50 in nearly incompressible materials. In particular, under compression the velocities of shear waves decrease in any –0.75 direction if K/µ ≤ 1 (Fig. 3(c)), while it can either decrease or increase depending on the propagation direction in the –1.00 nearly incompressible case (Fig. 2(a) and (c)). It should 0.4 0.6 0.8 1.0 be noted that the deformation induced stiffening has a λ significant influence on both modes (compare Fig. 3(a), (c) vs (b), (d)), in particular when material is stretched. This is Fig. 4. Dependence of λ˜ (a) and Poisson’s ratio ν (b) on applied stretch λ due to an increase in the effective shear modulus (the term for Gent and neo-Hookean materials with different ratios K/µ. 2 µJm/ξ in Eq. (9) and µJm/ξ in Eq. (10)). The polar diagram of the phase velocity for the quasi-transversal wave in Gent example, λcr ≈ 0.66 for neo-Hookean material with = − ≈ material with J = 3 and K/µ = 1 is similar to one plotted K/µ 0.3, and λcr 0.76 for Gent material with m = − = in Fig. 3(c), and it is not presented here. K/µ 0.3 and Jm 3. Auxetic materials. Next, we consider auxetic materials An example of wave velocities for auxetic materials is characterized by NPR behaviour. Yet can such materials ex- shown in Fig. 5. We observe that the velocity of the lon- gitudinal wave increases in any direction of propagation ist? Would they be stable? How can they be constructed? n when the material undergoes compression (Fig. 5(b)). These questions have recently arisen in many papers This is in contrast to the case of highly compressible mat- [19,27,36,37,42–45] and still the topic is open for discus- ter (see Fig. 3(a) and (b)). Moreover, the velocity of the lon- sion. Wang and Lakes in their article [36] report that bulk gitudinal wave increases and reaches the maximum when modulus can be varied within the range − 4µ < K < ∞. 3 wave vector n lies in the plane of transverse isotropy. How- Based on this and the previous estimations (Eq. (15)), we ever, for materials with strong stiffening effect the veloc- − examine the material behaviour when 1/3 < K/µ < 0. ity of longitudinal wave decreases in some direction of To illustrate the auxetic materials behaviour, we present propagation (see Fig. 5(a)). Fig. 5(c) and (d) show that ve- ˜ the dependence of λ and Poisson’s ratio on the applied locities of transversal waves decrease considerably for all stretch λ for different ratios of K/µ. directions of propagations n in contrast to the effect of de- Fig. 4 show that NPR behaviour is more pronounced formation observed in the nearly incompressible materials in materials with negative bulk modulus. Note that the (Fig. 5(a), (c) and (d)). The influence of stiffening on elastic material becomes locally non-auxetic when certain level wave propagation is rather weak in the case of auxetics as of deformation is reached. Furthermore, this level depends compared to nearly incompressible and highly compress- on stiffening of the material. In particular, materials with ible materials; yet it can be observed. In particular, phase pronounced stiffening effect become locally non-auxetic velocity of transversal wave decreases more under com- faster than materials with weak stiffening effect. For pression when stiffening effect is pronounced (compare 160 P.I. Galich, S. Rudykh / Extreme Mechanics Letters 4 (2015) 156–161

a b The fact that the isomer is independent of the choice of the polyadic representation of the original tensor can be readily proved by using well-known isomorphism between tensors and multilinear forms of the same rank.

Appendix B. Proof of absence of pure modes in general case in deformed Gent material

For clarity sake let us write an expanded form of tensor n ⊗ n : B ⊗ B(1324) and its scalar product on n. First, let us write B and B ⊗ B: = · T = 2 ⊗ + 2 ⊗ + 2 ⊗ c d B F F λ1e1 e1 λ2e2 e2 λ3e3 e3 (B.1) ⊗ = 4 ⊗ ⊗ ⊗ + 4 ⊗ ⊗ ⊗ B B λ1e1 e1 e1 e1 λ2e2 e2 e2 e2 + 4 ⊗ ⊗ ⊗ λ3e3 e3 e3 e3 + 2 2 ⊗ ⊗ ⊗ + ⊗ ⊗ ⊗ λ1λ2 (e1 e1 e2 e2 e2 e2 e1 e1) + 2 2 ⊗ ⊗ ⊗ + ⊗ ⊗ ⊗ λ1λ3 (e1 e1 e3 e3 e3 e3 e1 e1) + 2 2 ⊗ ⊗ ⊗ + ⊗ ⊗ ⊗ λ2λ3 (e2 e2 e3 e3 e3 e3 e2 e2) . (B.2) Now we can write the isomer (1324) of fourth-rank ⊗ Fig. 5. Polar diagrams of the phase velocities in auxetics: for the quasi- tensor B B as longitudinal (a) and purely transversal (c) waves in Gent material with ⊗ (1324) = 4 ⊗ ⊗ ⊗ B B λ1e1 e1 e1 e1 Jm = 3 and K/µ = −0.3; for the purely longitudinal (b) and transversal (d) waves in neo-Hookean material with K/µ = −0.3. + 4 ⊗ ⊗ ⊗ + 4 ⊗ ⊗ ⊗ λ2e2 e2 e2 e2 λ3e3 e3 e3 e3 + λ2λ2 (e ⊗ e ⊗ e ⊗ e + e ⊗ e ⊗ e ⊗ e ) Fig. 5(c) vs (d)). The polar diagram of the phase velocity for 1 2 1 2 1 2 2 1 2 1 + 2 2 ⊗ ⊗ ⊗ + ⊗ ⊗ ⊗ the quasi-transversal wave in Gent material with Jm = 3 λ1λ3 (e1 e3 e1 e3 e3 e1 e3 e1) and K/µ = −0.3 is similar to one plotted in Fig. 5(c), and + 2 2 e ⊗ e ⊗ e ⊗ e + e ⊗ e ⊗ e ⊗ e (B.3) is not shown here. λ2λ3 ( 2 3 2 3 3 2 3 2) .

Resolving n on the orthonormal basis n = n1e1 +n2e2 + 4. Concluding remarks n3e3, we obtain n ⊗ n : B ⊗ B(1324) = 4n2e ⊗ e + 4n2e ⊗ e We derived explicit expressions for phase velocity for λ1 1 1 1 λ2 2 2 2 + 4 2 ⊗ + 2 2 ⊗ + ⊗ finitely deformed materials with pronounced stiffening ef- λ3n3e3 e3 λ1λ2n1n2 (e1 e2 e2 e1) fect and demonstrated the significant role of the deforma- + λ2λ2n n (e ⊗ e + e ⊗ e ) tion on elastic wave propagation on examples for nearly 1 3 1 3 1 3 3 1 incompressible, highly compressible and extreme auxetic + 2 2 ⊗ + ⊗ λ2λ3n2n3 (e2 e3 e3 e2) (B.4) materials. Furthermore, we demonstrated how direction of wave propagation influences on the phase velocities and ⊗ : ⊗ (1324) · = 2 2 + 2 2 + 2 2 of elastic waves. These findings may guide further design n n B B n λ1n1 λ2n2 λ3n3 of mechanotunable acoustic metamaterials and phononic × 2 + 2 + 2 crystals with a large range of constituent properties. The lo- λ1n1e1 λ2n2e2 λ3n3e3 . (B.5) cal strain field in these engineered materials could be used Now, let g be a polarization vector, hence if g ∥ n to induce regions with extremely varied phononic prop- we have longitudinal polarization and if g ⊥ n we have erties to give rise to various acoustic effects. This opens a transversal polarization. Firstly, assume that g ∥ n then very rich and broad research avenue for designing tunable expression (4) yields acoustic/phononic metamaterials. Q(n) · n = (α + βξ(n · B · n)) n Appendix A. Isomers of a fourth-rank tensor + 2β n ⊗ n : B ⊗ B(1324) · n, (B.6) Here we follow the notation of isomer firstly introduced where for convenience we denoted = µ 1 + K − α J µ by Ryzhak [34,35]. Let M be a fourth-rank tensor with the µJ following representation as the sum of a certain number of 2 − 2 J2 and β = m . Since in general case vector 3 Jm Jξ 2 tetrads: n ⊗ n : B ⊗ B(1324) · n is not collinear to n (see Eq. (B.5)),

M = a1 ⊗ a2 ⊗ a3 ⊗ a4 + b1 ⊗ b2 ⊗ b3 ⊗ b4 + · · · . (A.1) therefore vector g = n is not an eigenvector of acoustic tensor, i.e. longitudinal polarization is absent, q.e.d. Let (ijks) be some permutation of the numbers (1234). Then Now let us assume that g ⊥ n then (4) yields the isomer M(ijks) is defined to be the fourth-rank tensor determined by the relation Q(n) · g = βξ(n · B · n)g (1324) M = ai ⊗ aj ⊗ ak ⊗ as + bi ⊗ bj ⊗ bk ⊗ bs + · · · . (A.2) + 2β n ⊗ n : B ⊗ B · g, (B.7) P.I. Galich, S. Rudykh / Extreme Mechanics Letters 4 (2015) 156–161 161

Suppose that g is an eigenvector of acoustic tensor then [20] S. Zhang, C. Xia, N. Fang, Broadband acoustic cloak for ultrasound waves, Phys. Rev. Lett. 106 (2011) 024301. βξ(n · B · n)g + 2β n ⊗ n : B ⊗ B(1324) · g = θg. (B.8) [21] K. Bertoldi, M.C. Boyce, Wave propagation and instabilities in mono- lithic and periodically structured elastomeric materials undergoing Scalar multiplication of the last equation by n yields large deformations, Phys. Rev. B 78 (2008) 184107. [22] S. Rudykh, M. Boyce, Transforming wave propagation in layered n · n ⊗ n : B ⊗ B(1324) · g = 0 media via instability-induced interfacial wrinkling, Phys. Rev. Lett. 112 (2014) 034301. 2 + 2 + 2 · = [23] Z. Chang, H.-Y. Guo, B. Li, X.-Q. Feng, Disentangling longitudinal and or λ1n1e1 λ2n2e2 λ3n3e3 g 0. (B.9) shear elastic waves by neo-hookean soft devices, Appl. Phys. Lett. 106 (2015) 161903. Yet last expression does not hold true in the general case. [24] J.L. Williams, J.L. Lewis, Properties and an anisotropic model of Consequently, g ⊥ n is not an eigenvector of acoustic cancellous bone from the proximal tibial epiphysis, Trans. ASME, J. tensor, q.e.d. Biomech. Eng. 104 (1982) 5–56. [25] K.E. Evans, K.L. Alderson, Auxetic materials: the positive side of being negative, Eng. Sci. Educ. J. 9 (2000) 148–154. References [26] B.D. Caddock, K.E. Evans, Negative Poisson ratios and strain- dependent mechanical properties in arterial prostheses, Biomateri- als 16 (1995) 1109–1115. [1] M. Biot, The influence of initial stress on elastic waves, J. Appl. Phys. [27] S. Babaee, J. Shim, J. Weaver, E. Chen, N. Patel, K. Bertoldi, 3d soft 11 (1940) 522. metamaterials with negative Poisson ratio, Adv. Mater. 25 (2013) [2] C. Truesdell, W. Noll, in: S.S. Antman (Ed.), The Non-Linear Field 5044–5049. Theories of Mechanics, third ed., Springer, 1965. [28] P. Wang, J. Shim, K. Bertoldi, Effects of geometric and material non- [3] A. Norris, Propagation of plane waves in a pre-stressed elastic linearities on the tunable response of phononic crystals, Phys. Rev. B medium, J. Acoust. Soc. Am. 74 (1983) 1642. 88 (2013) 014304. [4] R. Ogden, Non-Linear Elastic Deformations, Dover Publications, [29] P.I. Galich, S. Rudykh, Comment on ‘‘Disentangling longitudinal and 1984. shear elastic waves by neo-hookean soft devices’’, 2015. [5] F. John, Plane elastic waves of finite amplitude. Hadamard materials [30] E. Arruda, M. Boyce, A three-dimensional constitutive model for and harmonic materials, Comm. Pure Appl. Math. 19 (1966) the large stretch behavior of rubber elastic materials, J. Mech. Phys. 309–341. [6] M.S. Kushwaha, P. Halevi, L. Dobrzynski, B. Djafari-Rouhani, Acoustic Solids 41 (1993) 389–412. band structure of periodic elastic composites, Phys. Rev. Lett. 71 [31] A.N. Gent, A new constitutive relation for rubber, Rubber Chem. (1993) 2022. Technol. 69 (1996) 59–61. [7] V.K. Ignatovich, L.T.N. Phan, Those wonderful elastic waves, Amer. J. [32] C. Horgan, The remarkable gent constitutive model for hyperelastic Phys. 77 (2009) 1162. materials, Int. J. Non-Linear Mech. 68 (2015) 9–16. [8] R. Ogden, B. Sighn, Propagation of waves in an incompressible [33] M. Boyce, E. Arruda, Constitutive models of rubber elasticity: A transversally isotripic elastic solid with initial stress: Biot revisited, review, Rubber Chem. Technol. 73 (2000) 504–523. J. Mech. Mater. Struct. 6 (2011) 453–477. [34] E. Ryzhak, On stable deformation of unstable materials in a rigid [9] M. Shams, M. Destrade, R. Ogden, Initial stresses in elastic solids: triaxial testing mashine, J. Mech. Phys. Solids 41 (1993) 1345–1356. Constitutive laws and acoustoelasticity, Wave Motion 48 (2011) [35] L. Nikitin, E. Ryzhak, On stability and instability of a compressed 552–567. block pressed to a smooth basement, Mech. Solids 43 (2008) [10] W. Parnell, A.N. Norris, T. Shearer, Employing pre-stress to generate 558–570. finite cloaks for antiplane elastic waves, Appl. Phys. Lett. 100 (2012) [36] Y. Wang, R. Lakes, Composites with inclusions of negative bulk 171907. modulus: Extreme damping and negative Poisson ratio, J. Compos. [11] M. Destrade, R.W. Ogden, On stress-dependent elastic moduli and Mater. 39 (2005) 1645–1657. wave speeds, J. of Appl. Math. 78 (2013) 965–997. [37] N. Gaspar, C.W. Smith, K.E. Evans, Effect of heterogeneity on the [12] M. Hussein, M. Leamy, M. Ruzzene, Dynamics of phononic materials elastic properties of auxetic materials, J. Appl. Phys. 94 (2003) 6143. and structures: Historical origins, recent progress and future [38] B. Auld, Acoustic Fields and Waves in Solids, Krieger publishing outlook, Appl. Mech. Rev. 66 (2014) 040802. company, 1990. [13] P. Boulanger, M. Hayes, C. Trimarco, Finite-amplitude plane waves [39] A. Nayfeh, Wave Propagation in Layered Anisotropic Media with in deformed hadamard elastic materials, Geophys. J. Int. 118 (1994) Applications to Composites, Elsevier Science, 1995. 447–458. [40] N. Scott, The slowness surfaces of incompressible and nearly [14] S. Shan, S.H. Kang, P. Wang, C. Qu, S. Shian, E.R. Chen, K. Bertoldi, incompressible elastic materials, J. Elasticity 16 (1986) 239–250. Harnessing multiple folding mechanisms in soft periodic structures [41] G. Rogerson, N. Scott, Wave propagation in singly-constrained and for tunable control of elastic waves, Adv. Funct. Mater. 24 (2014) nearly-constrained elastic materials, Q. J. Mech. Appl. Math. 45 4935–4942. (1992) 77–99. [15] A. Bergamini, T. Delpero, L.D. Simoni, L.D. Lillo, M. Ruzzene, P. [42] L. Chen, C. Liu, J. Wang, W. Zhang, C. Hu, S. Fan, Auxetic materials Ermanni, Phononic crystal with adaptive connectivity, Adv. Mater with large negative Poisson ratios based on highly oriented carbon 26 (2014) 1343–1347. nanotube structures, Appl. Phys. Lett. 94 (2009) 253111. [16] P. Boulanger, M. Hayes, Finite-amplitude waves in deformed [43] K. Bertoldi, P. Reis, S. Willshaw, T. Mullin, Negative Poisson ratio mooney-rivlin materials, Q. J. Mech. Appl. Math. 45 (1992) 575–593. behavior induced by an elastic instability, Adv. Mater. 22 (2010) [17] X. Zhuang, Y. Mai, D. Wu, F. Zhang, X. Feng, Two-dimensional soft 361–366. nanomaterials: A fascinating world of materials, Adv. Mater. 27 [44] T. Still, M. Oudich, G.K. Auerhammer, D. Vlassopoulos, B. Djafari- (2015) 403–427. Rouhani, G. Fytas, P. Sheng, Soft silicone rubber in phononic [18] Y. Li, N. Kaynia, S. Rudykh, M. Boyce, Wrinkling of interfacial layers structures: Correct elastic moduli, Phys. Rev. B 88 (2013) in stratified composites, Adv. Energy Mater. 15 (2013) 921–926. 094102. [19] P. Wang, F. Casadei, S. Shan, J.C. Weaver, K. Bertoldi, Harnessing [45] P.J. Beltramo, D. Schneider, G. Fytas, E.M. Furst, Anisotropic buckling to design tunable locally resonant acoustic metamaterials, hypersonic phonon propagation in films of aligned ellipsoids, Phys. Phys. Rev. Lett. 113 (2014) 014301. Rev. Lett. 113 (2014) 205503. International Journal of Solids and Structures 91 (2016) 18–25

Contents lists available at ScienceDirect

International Journal of Solids and Structures

journal homepage: www.elsevier.com/locate/ijsolstr

Manipulating pressure and shear waves in dielectric elastomers via external electric stimuli

∗ Pavel I. Galich, Stephan Rudykh

Department of Aerospace Engineering, Technion –Israel Institute of Technology, Haifa 320 0 0, Israel

a r t i c l e i n f o a b s t r a c t

Article history: We investigate elastic wave propagation in ﬁnitely deformed dielectric elastomers in the presence of an Received 31 December 2015 electrostatic ﬁeld. To analyze the propagation of both longitudinal (P-) and transverse (S-) waves, we uti-

Revised 19 April 2016 lize compressible material models. We derive explicit expressions for the generalized acoustic tensor and Available online 3 May 2016 phase velocities of elastic waves for ideal and enriched dielectric elastomer models. We analyze the slow-

Keywords: ness curves of elastic wave propagation, and ﬁnd the P-S-mode disentangling phenomenon. In particular, Elastic waves P-and S-waves can be separated by applying an electric ﬁeld. The divergence angle between P-and S- Non-linear electroelasticity waves strongly depends on the applied electrostatic excitation. The inﬂuence of an electric ﬁeld depends Dielectric elastomers on the choice of a material model. In the case of the ideal dielectric model, the in-plane shear wave Finite deformation velocity increases with an increase in electric ﬁeld, while for the enriched model the velocity may de- crease depending on material constants. The divergence angle also gradually increases with an increase in electric ﬁeld, while for the enriched model the angle variation may be limited. Material compressibility affects the P-wave velocity, and for relatively compressible materials the slowness curve of the P-wave evolves from circular to elliptical shape manifesting in an increase in the refraction angle of the P-wave. As a result, the divergence angle decreases with an increase in material compressibility. ©2016 Elsevier Ltd. All rights reserved.

1. Introduction Rudykh et al., 2014; Rudykh and Bertoldi, 2013; Gei et al., 2014; Siboni et al., 2014; Bortot et al., 2016 ). Potentially, the need for the Dielectric elastomers (DEs) are soft responsive materials that high voltage can be reduced through architectured microstructures can change their form and shape when subjected to an electric of DEs increasing the electromechanical coupling ( Huang et al., stimulus ( Pelrine et al., 20 0 0; Bar-Cohen, 20 02 ). DEs have at- 2004; Rudykh et al., 2013; Cao and Zhao, 2013; Galipeau et al., tracted considerable attention due to a large variety of possible 2014; Chatzigeorgiou et al., 2015 ). Moreover, synthesis of new applications ranging from artiﬁcial muscles and soft robotics to soft dielectric materials seems to be another promising approach energy conversion and noise canceling devices ( O’Halloran et al., ( Madsen et al., 2014 ). The effective electromechanical properties 2008; Brochu and Pei, 2010; Carpi et al., 2011; Rudykh et al., 2012; of DEs can be actively controlled by external electric stimuli. The Kornbluh et al., 2012; Rogers, 2013 ). The theoretical framework of dominant factor is the ﬁnite deformations induced by an electric the non-linear electroelasticity is based on a theory ﬁrst developed excitation. Since in purely elastic materials wave propagation by Toupin (1956 ; 1963 ), which was recently revisited by Dorfmann strongly depends on the mechanical properties of the media and and Ogden (2005 ; 2010 ) and Suo et al. (2008) ; Suo (2010) . This fol- deformation ﬁelds ( Rudykh and Boyce, 2014; Galich and Rudykh, lowed by a series of works on modeling DEs ( Volokh, 2012; Itskov 2015b; 2015a ), this opens an opportunity to manipulate wave and Khiêm, 2014; Keip et al., 2014; Cohen and deBotton, 2014; propagation in DEs by applying an electric ﬁeld. Jabareen, 2015; Miehe et al., 2015; Aboudi, 2015; Hossain et al., In this work, we focus on elastic wave propagation in ﬁnitely 2015; Cohen et al., 2016 ), to name a few recent contributions. deformed DEs in the presence of a uniform electric ﬁeld. To The electromechanical coupling in typical DEs is rather weak, explore the elastic wave propagation in DEs, we follow the widely and, therefore, DEs need to operate at the edge of instabilities and used approach for the analysis of small-amplitude motions super- breakthrough voltages to achieve meaningful actuation ( Zhao et al., imposed on the ﬁnite deformations ( Ogden, 1997 ) induced by an 2007; Zhao and Suo, 2008; 2010; Rudykh and deBotton, 2011 ; external stimulus ( Dorfmann and Ogden, 2010; Destrade and Og- den, 2011 ). To allow for the consideration of the longitudinal wave propagation (differently from the recent works ( Gei et al., 2011; ∗ Corresponding author. Tel.: +972 48292547. Shmuel et al., 2012; Chen and Dai, 2012 ), where incompressible E-mail address: [email protected] (S. Rudykh). http://dx.doi.org/10.1016/j.ijsolstr.2016.04.032 0020-7683/© 2016 Elsevier Ltd. All rights reserved. P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25 19

( ) C = C 3412 = T Note that 0 0 and K0 K0 ; here the superscript (3412) denotes an isomer of the fourth-rank tensor ( Galich and Rudykh, 2015b; Ryzhak, 1993; Nikitin and Ryzhak, 2008 ) as detailed in Appendix A . Next, we consider the small-amplitude motions superimposed on ﬁnite deformations; hence, we present the incremental consti- tutive Eqs. (3) in the frame of the updated reference conﬁguration

δP = C : δH + M · δD 01 and δE 01 = δH : M + K · δD 01 , (5) −1 T −1 −T Fig. 1. Schematics of the splitting of pressure (P-) and shear (S-) elastic waves in where δP = J δP 0 · F , δD 01 = J F · δD 0 , δE 01 = F · δE 0 , δH = a nearly incompressible neo-Hookean DE. P-wave does not refract from the initial δF · F −1 , direction of propagation, while S-wave refracts at a certain angle. ( ) − ( ) 2134 ( ) − C = 1 · C 2134 · T , M = · M 213 · 1 J F 0 F F 0 F and K materials were considered), we utilize compressible electroactive −T −1 = JF · K 0 · F . (6) material models, namely the ideal ( Zhao et al., 2007 ) and enriched C = C (3412) , M (213) = M = T DE models. By application of wave propagation analysis to the Note that and K K . The linearized compressible DE models, we derive explicit expressions for the equation of motion and Maxwell’s equations in Eulerian form are generalized acoustic tensor and phase velocities for both longitu- ∂ 2 u dinal and transverse waves. We ﬁnd that electrostatically induced ∇ x · δP = ρ , ∇ x × δE = 0 and ∇ x · δD = 0 , (7) ∂ 2 01 01 changes in the key characteristics of shear (S-) and pressure (P-) t waves lead to a disentangling phenomenon, where P-and S-waves where u is the incremental displacement; ρ = ρ0 /J is the den- ρ travel in different directions. Fig. 1 schematically illustrates the sity of the deformed material and 0 is the initial density of the P-and S-wave splitting phenomenon. The divergence angle strongly material. We assume the absence of free body charges and cur- depends on the external ﬁeld, the induced deformation, and mate- rents. Note that we use the so called quasi-electrostatic approxi- rial compressibility. P-and S-waves possess diverse properties and, mation ( Dorfmann and Ogden, 2010; Maugin, 1985 ); more speciﬁ- thus, can be used for different purposes. For example, the S-wave cally, the interactions between electric and magnetic ﬁelds are ne- serves as a virtual “ﬁnger” to probe elasticity of internal regions glected. This is the non-relativistic approximation corresponding to of the body in shear wave elasticity imaging ( Sarvazyan et al., the case where the mechanical velocity is signiﬁcantly smaller than 1998 ). Longitudinal and transversal elastic waves can be separated the light velocity ( Dorfmann and Ogden, 2010 ). at the interface between dissimilar materials; however, this may We seek for a solution for Eqs. (7) in the form of plane waves cause a loss of energy or/and a wave-mode conversion at the with constant polarizations interface (Achenbach, 1973). Alternatively, we can use dielectric u = m f ( n · x − ct ) and δD = d g( n · x − ct ) , (8) elastomers to split P-and S-elastic waves by applying a bias electric 01 ﬁeld. This feature can be employed, for example, in small-scale where f is a twice continuously differentiable function and g is a micro-electromechanical systems, where it is convenient to use an continuously differentiable function; unit vectors m and d are po- electric ﬁeld to control the performance. Moreover, due to mathe- larization vectors of mechanical and electrical displacements, re- matical similarities between electro- and magneto-active materials, spectively; the unit vector n deﬁnes the direction of wave propa- this splitting phenomenon can be utilized in magnetorheological gation, and c is the phase velocity of the wave. elastomers controlled by an external magnetic ﬁeld. Substituting (5) and (8) into (7) , we obtain

· = ρ 2 , 2. Analysis A m c m (9) where A is the so-called “generalized” acoustic tensor deﬁning the To analyze the ﬁnitely deformed state, we introduce the de- condition of propagation of elastic plane waves in non-linear elec- ( , ) = ∇ ( , ) , formation gradient F X t X x X t where X and x are po- troelastic materials. The generalized acoustic tensor of electroelas- sition vectors in the reference and current conﬁgurations, respec- tic materials with an arbitrary strain energy function ψ(F , D 0 ) , has tively. In order to model a non-linear electroelastic material be- the following form ( Destrade and Ogden, 2011; Spinelli and Lopez- ψ( , ) , havior, we consider an energy function F D0 which is a func- Pamies, 2015 ) tion of deformation gradient F and electric displacement vector D0 2 in the reference conﬁguration. The corresponding electric displace- A = Q − R · ( tr Kˆ )ˆ I − Kˆ · R T , (10) −1 ( ˆ ) 2 − ˆ 2 ment in the current conﬁguration is given by D = J F · D 0 , where trK trK ≡ > J det F 0. The ﬁrst Piola–Kirchhoff stress tensor and electric where ﬁeld in the reference conﬁguration are given by ˆ = − ∂ψ ∂ψ I I n n (11) P = and E = , (1) 0 ∂ 0 , ˆ = ˆ · · ˆ, F ∂ D 0 is the projection on the plane normal to n K I K I and ( ) the corresponding counterparts in the current conﬁguration are Q = C 1324 : n n and R = n · M . (12) − − = 1 · T = T · . T J P0 F and E F E0 (2) Note that the generalized acoustic tensor A and the purely elas- Linearized constitutive Eqs. (1) read as tic acoustic tensor Q are symmetric. Recall that for DE to be sta- ble, the generalized acoustic tensor A has to be positively deﬁned. δP 0 = C 0 : δF + M 0 · δD 0 and δE 0 = δF : M 0 + K 0 · δD 0 , (3) Note that an analogue of the generalized acoustic tensor (10) was δ C , M where denotes an incremental change; 0 0 and K0 are derived by Destrade and Ogden (2011) for incompressible magne- the so-called tensors of electroelastic moduli ( Dorfmann and toelastic materials. Ogden, 2010 ) deﬁned as A detailed description of the non-linear electroelastic theory for ∂ 2 ψ ∂ 2 ψ ∂ 2 ψ DEs can be found in publications of Dorfmann and Ogden (2005 ; C = , M = and K = . (4) 0 ∂ ∂ 0 0 2010 ), and Suo et al. (2008) , Suo (2010) . F F ∂ F ∂ D 0 ∂ D 0 ∂ D 0 20 P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25

It is well known that incompressible materials do not support part of the energy function (13) , here and thereafter, we utilize a longitudinal waves. Therefore, to analyze both transversal and lon- model of a compressible neo-Hookean material ( Ogden, 1997 ) ψ( , ) gitudinal waves, we consider the energy function F D0 for the μ μ K 2 compressible electroelastic material in the following form: ψ (F ) = (I − 3) − μ ln J + − (J − 1) , (20) elas 2 1 2 3

1 ψ(F , D ) = ψ (F ) + ( γ I + γ I + γ I ), (13) where I = tr C is the ﬁrst invariant of the right Cauchy-Green ten- 0 elas 2 J 0 4e 1 5e 2 6e 1 sor, μ is the shear modulus and K is the bulk modulus. ψ where elas (F) is a purely elastic energy function (for example, For the ideal DE, the generalized acoustic tensor takes the form neo-Hookean, Mooney–Rivlin, Gent, etc. ( Ogden, 1997 )), is the = γ ∗ ∗ material permittivity in the undeformed state ( F I) and i are = + ˆ, A a1 n n a2 I (21) dimensionless parameters, moreover γ0 + γ1 + γ2 = 1 , and

2 where n n is the projection on the direction n and ˆI is given in I = D · D , I = D · C · D and I = D · C · D (14) 4e 0 0 5e 0 0 6e 0 0 (11) , are invariants depending on the electric displacement D0 and right ∗ − = ( − μ/ ) + μ 1( + · · ) Cauchy-Green tensor C = F T · F . a1 K 2 3 J J 1 n B n (22) For the energy function (13) the relation between the electric ∗ − ﬁeld and displacement is and a = μJ 1( n · B · n ) . (23) 2 1 − = γ 1 + γ + γ · , E 0 B 1 I 2 B D (15) Consequently, there always exist one pressure and two shear waves for any direction of propagation n , ﬁnite deformation F and elec- = · T where B F F is the left Cauchy–Green tensor. The correspond- tric displacement D . The phase velocities of these waves can be ing tensors of electroelastic moduli are calculated as 1 ∗ ∗ C = C + γ C + γ C + γ C , = /ρ = /ρ . elas 0 4e 1 5e 2 6e cp a1 J 0 and cs a2 J 0 (24) 2 1 Remarkably, while the electroelastic moduli (16) explicitly depend M = γ M + γ M + γ M and 2 0 4e 1 5e 2 6e on the electric ﬁeld, the phase velocities of elastic waves do not ex- plicitly depend on the electric ﬁeld. The dependence of the veloc- 1 − = γ 1 + γ + γ , K 0 B 1 I 2 B (16) ities on an electric ﬁeld is introduced through the electrostatically √ = μ , C ψ induced deformation. Let us consider the case when D0 D e2 where elas is derived from the purely elastic part elas (F) of the DE can freely expand in plane e − e , and the deformation gradi- energy function in accordance to (4) and (6) ; and the explicit ex- 1 3 ent can be expressed as pressions for the other tensors are given in Appendix B . ˜ Finally, the corresponding generalized acoustic tensor takes the F = λ(D ) e 2 e 2 + λ(D )(I − e 2 e 2 ) . (25) following form For an incompressible ideal DE ( Zhao et al., 2007 ), the stretch ra- 1 4 2 −1 / 3 −1 / 2 = + γ + γ + γ − , tios can be expressed as λ = (1 + D ) and λ˜ = λ . It should A Q elas 0 Q 4 e 1 Q 5 e 2 Q 6 e η Ae (17) 2 be noted that these relations approximately hold even for very where Q elas is calculated by applying of Eqs. (4), (6) and (12) to compressible materials with K / μ ∼ 1 for the range of deforma- ψ the purely elastic part elas (F) of the energy function; the explicit tions and electric ﬁelds√ considered here. Recall that neo-Hookean η expressions for , and tensors Q4 e , Q5 e , Q6 e and Ae are given in DE is stable for D 3 ( Zhao et al., 2007 ) and it will thin down the Appendix B . Remarkably, in the particular case of F = λ1 e 1 without any limit when the electric ﬁeld is further increased. Note e + λ e e + λ e e , n = e and D = D e , the generalized 1 2 2 2 3 3 3 1 0 2 2 that in the absence of an electric√ ﬁeld, expressions (24) reduce to acoustic tensor (17) reduces to c p = (K + 4 μ/ 3) /ρ0 and c s = μ/ρ0 . γ 2 For the nearly incompressible DE, the phase velocities of P-and 2 D2 A = Q + e e , (18) elas 2 2 2 S-waves can be calculated as λ 3 here the set of ( e , e , e ) deﬁnes the orthonormal basis. μ + 2 2 ϕ 1 2 3 1 D cos c = (K + μ/ 3 + /ρ (26) Let us consider the inﬂuence of an electric ﬁeld on the P-and S- p 2 / 3 0 + 2 waves propagation. Important characteristics of elastic waves can 1 D be deduced from the consideration of slowness curves. Fig. 2 (a) and schematically shows the slowness curves for P-and S-waves propa- −2 / 3 gating in a DE subjected to an electric ﬁeld. P-and S-waves refract 2 2 2 c s = 1 + D cos ϕ 1 + D μ/ρ , (27) differently from the initial direction of propagation, thus, the P-and 0 S-waves can be split in such media. The normals to the slowness where the propagation direction is deﬁned as n = ( cosϕ , sinϕ , 0) . curves can be deﬁned by the corresponding angle θ (see Fig. 2 (a)) Hence, refraction angles of P-and S-waves are − / ϕ − ( / ϕ) ϕ 2 3 s p,s sin dsp,s d cos K + μ/ 3 + μ 1 + D 2 tan ϕ tan θp,s = , (19) , ϕ + ( , / ϕ) ϕ θ = sp s cos dsp s d sin tan p / (28) 1 3 + μ/ + μ + 2 ϕ (ϕ) = −1(ϕ) K 3 1 D where is the incident angle and sp,s cp,s are slownesses of P-and S-waves, respectively. Consequently, the divergence angle and θ = θ − θ between P-and S-wave can be calculated as p s . tan ϕ tan θs = . (29) + 2 3. Results 1 D Remarkably, relations (26), (27), (28) and (29) approximately hold 3.1. Ideal dielectric elastomer model even for very compressible materials with K / μ ∼ 1 for the range of deformations and electric ﬁelds considered here. By making use First, we consider an ideal dielectric elastomer model ( Zhao of relations (26) and (27) , the slowness curves of P-and S-waves et al., 2007 ), namely γ0 = γ2 = 0 and γ1 = 1 in (13) . For the elastic for the ideal DE can be constructed. Fig. 2 (b) shows an example P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25 21

Fig. 2. (a) Schematic illustration of slowness curves for P-and S-waves in the DE subjected to an electric ﬁeld. (b) Slowness curves of P-and S-waves for the ideal DE with /μ = = K √ 50 subjected to the electric excitation of D 1. Slowness curves are constructed by using (26) and (27). Scale is 0.2 per division, and slowness curves are normalized by μ/ρ0 .

Fig. 3. Divergence angle as function of non-dimensional electric displacement – (a), and incident angle –(b) for the nearly incompressible neo-Hookean DE with K/μ = 300 . of the slowness curves for an ideal DE with K/μ = 50 subjected to ﬁeld) the phase velocity of the longitudinal wave depends signiﬁ- the electric excitation of D = 1 . cantly on the direction of wave propagation and applied deforma- Fig. 3 (a) shows that the divergence angle θ signiﬁcantly de- tion ( Galich and Rudykh, 2015b ). Here, we also observe a strong pends on the value of an applied electric ﬁeld. In particular, the dependence of the P-wave velocity on the direction of wave prop- divergence angle increases monotonically with an increase in the agation and the deformation induced by an electric ﬁeld. An in- μ electric√ ﬁeld until the limiting value of the electric ﬁeld is reached crease in the material compressibility parameter /K results in a ( D = 3). Fig. 3 (b) shows the dependence of the divergence angle more pronounced inﬂuence of electrostatically induced deforma- θ on the incident angle ϕ. We observe that the divergence angle tion on elastic waves. In particular, the slowness curves of P-wave θ ϕ has a maximum for a certain incident angle 0 depending on evolve from circle to ellipse shape with an increase in electric ﬁeld. ϕ the applied electric ﬁeld. The incident angle 0 corresponding to Thus, refraction angle of P-wave differs from the incident angle, the maximal divergence angle is given by namely P-wave refracts along with S-wave. Fig. 4 schematically il- lustrates the phenomenon in compressible materials. The depen- α αμ3 ( α + ) + 2 α μ( α − μ) + ζ 27 3D 1 1 3 dence of the divergence angle on compressibility for different val- tan ϕ 0 = , (30) μ3 α2 + 27 + ζ ues of the electrostatic excitation is presented in Fig. 5 . Clearly, an increase in material compressibility weakens the disentangling / α = + 2, α = α2 3( + μ) ζ = α2 μ2 + where 1 D 1 3 K and 9 K 3K phenomenon. ( K + μ) . The maximal angle, ϕ , monotonically increases with 0 μ ϕ = 3.2. Enriched electroactive material model an increase in the electric ﬁeld. Note that for /K 1, 0 −1 / 2 arccos 2 + D 2 . Motivated by the experimental observations ( Wissler and Next we consider the inﬂuence of the material compressibility Mazza, 2007; Li et al., 2011 ), in this section we investigate elas- on the elastic wave propagation in DEs. It has been recently shown tic wave propagation in DEs described by an enriched electroactive that for highly compressible material (in the absence of an electric material model (13) . The model is similar to that considered by 22 P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25

Fig. 4. Schematics of the splitting of P-and S-waves in the compressible neo- Hookean DE. P-and S-waves unidirectionally refract from the initial direction of propagation, however, their refraction angles are different.

Fig. 6. Phase velocity of in-plane shear wave as functions of non-dimensional elec- tric displacement for ideal and enriched DE models, ϕ = 0 .

phase velocity of the in-plane shear wave as a function of the non- dimensional electrostatic excitation for the ideal and enriched DE

models. One can see that the consideration of the I4 e and I6 e invari- ants strongly inﬂuences the in-plane shear wave velocity. In par- ticular, the increase in phase velocity of the in-plane shear wave is less prominent (dashed blue curve in Fig. 6 ) as compared with the ideal DE model result; moreover, the velocity may even decrease with an increase in the electric ﬁeld (see the example for the par- ticular material denoted by the dot-dashed green curve in Fig. 6 ), while for the ideal DE model the velocity always increases. These

Fig. 5. Divergence angle as function of material compressibility for the ideal neo- differences indeed affect the splitting mechanism and, thus, differ- Hookean DE subjected to different levels of electrostatic excitation, ϕ = π/ 6 . ent results are produced by these material models. Fig. 7 illustrates

Table 1 the difference in the divergence angles for the ideal and enriched Material constants of DE model (13) . DE models. In particular, Fig. 7 (a) shows that the divergence angle θ is smaller than it is predicted by the ideal DE model. Moreover, Reference γ 0 γ 1 γ 2 for Li et al. experimental data, the divergence angle θ decreases Ideal DE ( Zhao et al., 2007 ) 0 1 0 with an increase in the electric ﬁeld after a certain level of the Wissler and Mazza (2007) 0.00104 1.14904 −0.15008 applied voltage is reached. Fig. 7 (b) shows that the divergence an- Li et al. (2011) 0.00458 1.3298 −0.33438 θ ϕ gle has a maximum for a certain incident angle 1 . Moreover, ϕ the incident angle 1 , producing the maximum divergence angle, Gei et al. (2014) . To allow for the investigation of pressure waves, varies for different materials. we extend the model to capture the compressibility effects. Table 1 Although in this work we perform a fully electromechanical summarizes the parameters of the material model (13) for differ- coupling analysis, it is possible to employ only a purely mechani- ent experimental data ( Wissler and Mazza, 2007; Li et al., 2011 ). cal analysis of wave propagation in non-linear electroelastic solids. γ = , γ = , In the case when 0 0 2 0 and the deformation gradient In that case the contribution of the electroelastic moduli tensors = , identical to (25), and n e1 the expressions for phase velocities M and K is neglected, and only terms of the tensor C contribute take the following form to the generalized acoustic tensor. Remarkably, this approximation

yields very close results for the phase velocity of pressure wave as = ( − μ/ ) λ2 λ˜ 4 + + λ˜ 2 μ /ρ ( = ), cp K 2 3 1 0 m e1 (31) the fully electromechanically coupled analysis; moreover, the re- sulting expressions for the phase velocities of the shear waves are identical in both analyzes. For example, for the deformation gradi- = γ 2 λ + λ˜ 2 μ/ρ ( = ) √ cs 2 D 0 m e2 (32) ent (25) , n = e 1 and D 0 = D μe 2 , the classic acoustic tensor takes and the form − − − = λ˜ μ/ρ ( = ). = + μ 2(γ 2 + γ λ˜ 4 + γ λ2λ˜ 4 ) cs 0 m e3 (33) Q Q elas D 0 J 1 2 e1 e1 − − / + μγ 2λ˜ 2 . For incompressible materials λ˜ = λ 1 2, and the stretch ratio λ can 2 D e2 e2 (35) be determined by solving the following polynomial equation It is easy to see that the resulting expressions for the phase veloci- 3 2 2 λ 1 + D γ1 + 2 γ2 λ = 1 . (34) ties of S-waves are the same as given by expressions (32) and (33), and the corresponding expression for the phase velocity of P-wave Hence, the phase velocity of the in-plane shear wave (with po- has the form = larization m e2 ) explicitly depends on the electric ﬁeld in con- = μ + λ˜ 2 + ( /μ − / ) λ2 λ˜ 4 + 2 (γ λ−2 + γ + γ λ2 ) λ˜ −4 /ρ . trast to the result (24)2 for the ideal DE model. Fig. 6 shows the cp 1 K 2 3 D 0 1 2 0 (36) P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25 23

Fig. 7. Divergence angle as function of non-dimensional electric displacement for ϕ = π/ 6 (a) and incident angle for D = 1 (b) in the nearly incompressible neo-Hookean DE with K/μ = 300 .

Expression (36) for the P-wave velocity differs from (31) by Acknowledgments the additional term containing the electric displacement magni- tude. However, according to our observations for K / μ ࣡ 100, this This research was supported by the ISRAEL SCIENCE FOUNDA- term can be neglected for small and moderate levels of electric TION (grants 1550/15 and 1973/15 ). SR gratefully acknowledges the displacement. support of Taub Foundation through the Horev Fellowship –Lead- ers in Science and Technology.

Appendix A. Notation of tensor isomers 4. Concluding remarks To achieve a more compact representation of the results, we

In this paper, we considered pressure (P-) and shear (S-) elas- have used the notation of isomers ﬁrstly introduced by Ryzhak S tic waves propagating in soft DEs subjected to ﬁnite deformations (1993); Nikitin and Ryzhak (2008). Let be a third-rank tensor in the presence of an electric ﬁeld. To allow for the consideration with the following representation as the sum of a certain number of P-wave propagation, we utilized the ideal and enriched material of triads: models accounting for the compressibility effects. Explicit expres- S = a 1 a 2 a 3 + b 1 b 2 b 3 + ··· (A.1) sions for the generalized acoustic tensor and phase velocities of Let (ikj) be some permutation of the set (123). Then the iso- elastic waves for DEs subjected to an electric ﬁeld were presented. ( ) mer S ik j is deﬁned to be the third-rank tensor determined by the We found that, for the ideal DE model, the elastic wave propaga- relation tion is explicitly independent of an applied electric ﬁeld, while it is ( ) S ik j = + + ··· inﬂuenced through the deformation induced via bias electric ﬁeld; ai ak a j bi bk b j (A.2) this is despite the fact that all electroelastic moduli tensors explic- Analogously, we can deﬁne isomers for higher-rank tensors. For itly depend on the applied electric ﬁeld. However, for the enriched example, if S = b I , where b is an arbitrary vector and I is material model, including all three electroelastic invariants I , I ( ) ( ) ( ) 4e 5e the unit tensor, then S 231 = S 321 = I b and S 132 = S. If S = and I , elastic wave propagation explicitly depends on the applied 6 e M N , where N and M are arbitrary second-rank tensors, then electric ﬁeld; in particular, the phase velocity of the in-plane shear ( ) S 3412 = N M . wave decreases when an electric ﬁeld is applied.

These ﬁndings were applied to explore the phenomenon of dis- Appendix B. Components of the electroelastic moduli and entangling P-and S-elastic waves in DEs by an electric ﬁeld. We generalized acoustic tensors showed that the divergence angle between P-and S-waves strongly depends on the value of the applied electric ﬁeld and direction Here we introduce the following notations of wave propagation. Moreover, we found that an increase in the (2) 2 2 = · · , = · · , = · , material compressibility weakens the separation of P-and S-waves. Lab a L b Lab a L b L L L This is due to the fact that the P-wave also refracts (in the same (− ) − (− ) − − − − L 1 = a · L 1 · b , L 2 = a · L 2 · b , L 2 = L 1 · L 1, direction as the S-wave) from the initial direction of wave prop- ab ab ( ) (− ) − 3 = · 3 · , 3 = 2 · , 3 = · 3 · , agation, while for nearly incompressible materials the change in Lab a L b L L L Lab a L b the P-wave direction is negligible. The phenomenon can be used −3 −2 −1 s 1 to manipulate elastic waves by a bias electrostatic ﬁeld; this can L = L · L , a b = a b + b a , 2 be beneﬁcial for applications in small length-scale devices, such 2 2 a = a · b, a = (a ) , (B.1) as micro-electromechanical systems, where an electric ﬁeld is the b b b preferred control parameter. Thanks to the mathematical similar- where L is an arbitrary second-rank tensor, a and b are arbitrary ities in the description of electro- and magneto-active materials, vectors. the disentangling phenomenon can be utilized to control P-and S- −1 (1342) C = B (I I + I I ) , waves in magnetorheological elastomers by applying an external 4e DD (2134) magnetic ﬁeld. C 5 e = 2( D I D − D D I − I D D ) 24 P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25

( ) + ( + 1342 ) , + γ γ 2( β − ) + γ γ 2 ( + β ) DD I I I I 0 2 4 BDn 2Dn BDn 1 2 BDn BDn 2 Dn (2134) (1432) 2 C = ( ( · ) + + γ γ ( βD + 2 B )D , 6e 2 D I B D B D D 2 1 n Dn n (2134) (2134) + D B D + (B · D ) I D 2 (2) 2 (2) (3) a = γ γ I B − (B nn ) + B nn B − B ( ) 3 2 2 1 nn nn nn + D D B 1324 + D B D (− ) ( ) − ( ) + γ − 1 2 + ( 1 ) 2 − ( ) 2 −I (B · D ) D − I D (B · D ) 0 Bnn Bnn Bnn I : B Bnn Bnn ( ) −D (B · D ) I − (B · D ) D I ) + γ 2 − ( ) 2 , 1 Bnn Bnn ( ) + ( + 1342 ) . BDD I I I I (B.2) 3 3 (2) (3) = γ γ γ ( − β ) − γ − γ − a4 2 0 1 2 Dn 2 4 BDn 1 Dn 2 I1 BDn BDn

(−1) 2 Q = 2 B n n , − γ γ β D 4e DD 0 1 4 n ( ) (− ) 2 2 s 2 2 1 Q = 2((D + D ) n n + D ˆI − 2 D D n ) , + γ0 γ 3 B Dn − β4 B + I 1 B B nn − 2 D n 5e D n n n 2 Dn Dn (−1) (2) 2 Q = 2((2 B D + B ) n n + 2 B D ˆI + − + γ γ ( − ) 6e Dn n DD Dn n DnBnn BDn Bnn 1 2 BDn Bnn 2I1 s 2 s − + + ( · ) (− ) − (− ) 2BDn D n Dn B 2Dn B n D + γ γ 2 1 ( 1 ) − 2 − β 2 0 Bnn B I : B B 2Dn 4 s Dn Dn − 2 D n (B · D ) n + B nn D D ) . (B.3)

− γ γ 2( β + ) , 2 1 Dn 2BDn −1 M = −2 I (B · D ) , = γ γ 2 ( β − ) + γ γ β 2 4e a5 2 2 BDn 2Dn BDn 2 0 1 4 Dn (213) M 5 e = 2( D I + D I − I D ) ,

( ) 2 2 2 213 + γ0 γ2 D n ( 2 β4 B Dn − D n ) + 2 γ1 γ2 βD + γ D , (B.8) M 6 e = 2( D B + D B + (B · D ) I n 1 n ( ) +(B · D ) I 213 − I (B · D )) . (B.4) ( ) = γ γ 2 2 + ( − ) + γ γ β a6 2 2 2 Dn Bnn I1 BDn Dn Bnn 0 1 4 Dn −1 R = −2 n (B · D ) , 4e − (− ) + γ γ ( 1 ) ( − ) − 1 = ( + − ) , 0 2 I : B BDn Dn Bnn Bnn BDn R 5 e 2 Dn I D n n D

R = 2(D B + D (B · n ) + B I + γ γ ( + β ) + γ 2 , 6e n Dn 1 2 BDn Dn 1 Dn + (B · D ) n − n (B · D )) . (B.5)

= − γ γ 2β + γ γ β + γ γ ( β − ) a7 2 2 2 BDn 2 0 1 4 Dn 0 2 4 BDn 2Dn (− ) − − (− ) η = γ 2 2 − 1 1 − ( 1 ) 2 2 2Bnn B : B Bnn + 2 γ γ βD + γ D , 0 1 2 n 1 n 2 (2) 2 + γ 2 B − B : B − (B ) 2 nn nn (−1) 2 a = 2 γ γ γ B ( I D − B ) − D 8 2 0 2 Dn 1 n Dn n − (− ) 2 + γ 1 − 1 + γ + γ β + γ 2 0 I : B Bnn 1 ( 2 1 ) 2 (−1) −1 (−2) 2 (2) − (− ) + D n γ B (I : B ) − B − γ B + γ γ ( 1 ) β − 1 − 0 Dn Dn 2 Dn 2 0 2 I : B I1 Bnn 1 (B.6) (− ) − γ γ 1 − γ γ , 0 1 BDn 1 2 BDn

= + + + s + + ( · ) s Ae a1 n n a2 I a3 D D a4 n D a5 B a6 B n D = γ 2 ( γ ( β − ) + ( γ β − γ ) ), a9 2 Dn 2 Dn 2BDn Dn 0 4 1 s s 2 2 s + a 7 (B · D ) n + a 8 (B · n ) n + a 9 B + a 10 (B · n ) D 2 a = 2 γ ( γ ( I D n − B ) + γ β D n ), 10 2 2 1 Dn 0 4 + ( 2 · ) s + ( 2 · ) s + ( · ) ( · ) a11 B D n a12 B n n a13 B n B n = γ 2( γ ( − β ) − ( γ β − γ ) ), a11 2 2 2 BDn Dn Dn 0 4 1 3 3 s 3 s + a B + a (B · n ) D + a (B · D ) n (− ) 14 15 16 = − γ γ 2 1 , − − a12 2 0 2 Dn B + ( 2 · ) ( · ) s + 1 + ( 1 · ) s Dn a17 B n B n a18 B a19 B n n − = γ 2 γ ( − ) + γ − γ ( 1 ) , −1 s −1 s a13 2 Dn 2 2BDn I1 Dn 1 Dn 0 Dn I : B + a 20 (B · n ) D + a 21 (B · D ) n

= −γ 3 2, = − γ 3 , = − , = − , −1 s −2 s a 14 D a15 2 Dn a16 a15 a17 2a14 + a 22 (B · n ) (B · n ) + a 23 (B · D ) n , (B.7) 2 n 2 (− ) = −γ ( γ + γ )2 , = − γ 2 1 ( γ + γ ), a18 0 1 Dn 2 BDn a19 2 0 B 1 Dn 2 BDn where Dn (− ) (− ) − (− ) (− ) (− ) a = 2 γ γ B ( γ D + γ B ), = γ 3 2 − ( 1 ) 2 1 − 1 2 − 3 20 0 2 nn 1 n 2 Dn a1 0 BDD BDn I : B Bnn BDD BDD a 21 = 2 γ0 ( γ2 γ0 ( D n − β4 B Dn ) − γ2 β( γ1 D n + γ2 B Dn ) − γ1 γ0 β4 D n ), (−1) (−2) 3 + + γ 2BDn BDn 1 DD = γ γ ( γ + γ ), = γ 2( γ + γ ), a22 2 0 2 Dn 1 Dn 2 BDn a23 2 0 1 Dn 2 BDn ( ) ( ) (− ) (− ) 3 2 3 1 1 − (− ) + γ βB − B + 2 γ0 γ1 γ2 βB + B Dn B β = − β = 1 − 1 . 2 DD DD DD Dn I1 Bnn and 4 I : B Bnn (B.9) + β − ) 4 BDD DD 2 (−1) 2 (2) + γ γ β D + B + γ γ β B − 3 B + 2 βD References 0 1 4 D DD 0 2 4 DD DD D (− ) ( ) + 1 2 Aboudi, J. , 2015. Micro-electromechanics of soft dielectric matrix composites. Int. J. 2BDn BDn Solids Struct. 64, 30–41 . (− ) (− ) (− ) ( ) + γ γ 2 β 1 − 2 + ( 1 ) 2 + γ γ 2 β − 2 Achenbach, J.D. , 1973. Wave Propagation in Elastic Solids. Applied Mathematics and 1 0 2 4 B B B 1 2 2 BDD B DD DD Dn DD Mechanics. North-Holland Publishing Company . 2 (−2) (−1) (−1) (−1) Bar-Cohen, Y. , 2002. Electroactive polymers as artiﬁcial muscles: A review. J. + γ2 γ βB − 3 B + 2 β4 D D + B 2 D n − I 1 B 0 DD DD Dn Dn Spacecr. Rockets 39 (6), 822–827 . 2 + γ γ ( βD + B ), Bortot, E., Denzer, R., Menzel, A., Gei, M., 2016. Analysis of viscoelastic soft dielectric 2 1 D DD elastomer generators operating in an electrical circuit. Int. J. Solids Struct. 78-79, = γ 3 2 + γ 3β( ) 2 + γ γ γ ( β − ) + γ γ 2β 2 a2 1 Dn 2 BDn 2 0 1 2 Dn 4 BDn Dn 0 1 4 Dn 205–215. P.I. Galich, S. Rudykh / International Journal of Solids and Structures 91 (2016) 18–25 25

Brochu, P. , Pei, Q. , 2010. Advances in dielectric elastomers for actuators and artiﬁcial Madsen, F.B. , Yu, L. , Daugaard, A.E. , Hvilsted, S. , Skov, A.L. , 2014. Silicone elastomers muscles. Macromol. Rapid Commun. 31 (1), 10–36 . with high dielectric permittivity and high dielectric breakdown strength based Cao, C. , Zhao, X. , 2013. Tunable stiffness of electrorheological elastomers by design- on dipolar copolymers. Polymer 55 (24), 6212–6219 . ing mesostructures. Appl. Phys. Lett. 103, 041901 . Maugin, G.A. , 1985. Nonlinear Electromechanical Effects and Applications, 1. World Carpi, F. , De Rossi, D. , Kornbluh, R. , Pelrine, R.E. , Sommer-Larsen, P. , 2011. Dielectric Scientiﬁc . Elastomers as Electromechanical Transducers: Fundamentals, Materials, Devices, Miehe, C. , Vallicotti, D. , Zäh, D. , 2015. Computational structural and material sta- Models and Applications of an Emerging Electroactive Polymer Technology. El- bility analysis in ﬁnite electro-elasto-statics of electro-active materials. Int. J. sevier Science . Numer. Methods Eng. 102 (10), 1605–1637 . Chatzigeorgiou, G. , Javili, A. , Steinmann, P. , 2015. Interface properties inﬂuence Nikitin, L.V. , Ryzhak, E.I. , 2008. On stability and instability of a compressed block the effective dielectric constant of composites. Philos. Mag. 95 (28–30), 3402– pressed to a smooth basement. Mech. Solids 43 (4), 558–570 . 3412 . O’Halloran, A. , O’Malley, F. , McHugh, P. ,2008. A review on dielectric elastomer ac- Chen, W. , Dai, H. , 2012. Waves in pre-stretched incompressible soft electroactive tuators, technology, applications, and challenges. J. Appl. Phys. 104 (7), 071101 . cylinders: exact solution. Acta Mech. Solida Sinica 25 (5), 530–541 . Ogden, R.W. , 1997. Non-Linear Elastic Deformations. Dover Publications, New York . Cohen, N. , deBotton, G. , 2014. Multiscale analysis of the electromechanical coupling Pelrine, R. , Kornbluh, R. , Pei, Q. , Joseph, J. , 20 0 0. High-speed electrically actuated in dielectric elastomers. Eur. J. Mech. A/Solids 48, 48–59 . elastomers with strain greater than 100. Science 287 (5454), 836–839 . Cohen, N. , Menzel, A. , deBotton, G. , 2016. Towards a physics-based multiscale mod- Rogers, J.A. , 2013. A Clear Advance in Soft Actuators. Science 341 (6149), 968–969 . elling of the electro-mechanical coupling in electro-active polymers. Proc. R. Rudykh, S. , Bertoldi, K. , 2013. Stability of anisotropic magnetorheological elastomers Soc. A 472, 20150462 . in ﬁnite deformations: a micromechanical approach. J. Mech. Phys. Solids 61, Destrade, M. , Ogden, R.W. , 2011. On magneto-acoustic waves in ﬁnitely deformed 949–967 . elastic solids. Math. Mech. Solids 16, 594–604 . Rudykh, S. , Bhattacharya, K. , deBotton, G. , 2012. Snap-through actuation of thick- Dorfmann, A. , Ogden, R.W. , 2005. Nonlinear electroelasticity. Acta Mech. 174, -wall electroactive balloons. Int. J. Nonlinear Mech. 47, 206–209 . 167–183 . Rudykh, S. , Bhattacharya, K. , deBotton, G. , 2014. Multiscale instabilities in soft het- Dorfmann, A. , Ogden, R.W. , 2010. Electroelastic waves in a ﬁnitely deformed elec- erogeneous dielectric elastomers. Proc. R. Soc. A 470, 20130618 . troactive material. J. Appl. Math. 75, 603–636 . Rudykh, S. , Boyce, M.C. , 2014. Transforming wave propagation in layered media via Galich, P.I. , Rudykh, S. , 2015a. Comment on ”disentangling longitudinal and shear instability-induced interfacial wrinkling. Phys. Rev. Lett. 112, 034301 . elastic waves by neo-hookean soft devices” [appl. phys. lett. 106, 161903 Rudykh, S. , deBotton, G. , 2011. Stability of anisotropic electroactive polymers with (2015)]. Appl. Phys. Lett. 107 (5), 056101 . application to layered media. Z. Angew. Math. Phys. 62, 1131–1142 . Galich, P.I. , Rudykh, S. , 2015b. Inﬂuence of stiffening on elastic wave propagation in Rudykh, S. , Lewinstein, A. , Uner, G. , deBotton, G. , 2013. Analysis of microstructural extremely deformed soft matter: from nearly incompressible to auxetic materi- induced enhancement of electromechanical coupling in soft dielectrics. Appl. als. Extreme Mech. Lett. 4, 156–161 . Phys. Lett. 102, 151905 . Galipeau, E. , Rudykh, S. , deBotton, G. , Ponte Castañeda, P. , 2014. Magnetoactive Ryzhak, E.I. , 1993. On stable deformation of unstable materials in a rigid triaxial elastomers with periodic and random microstructures. Int. J. Solids Struct. 51, testing machine. J. Mech. Phys. Solids 41 (8), 1345–1356 . 3012–3024 . Sarvazyan, A. , Rudnenko, O. , Swanson, S. , Fowlkes, J. , Emelianov, S. , 1998. Shear Gei, M. , Colonnelli, S. , Springhetti, R. , 2014. The role of electrostriction on the sta- wave elasticity imaging: a new ultrasonic technology of medical diagnostics. Ul- bility of dielectric elastomer actuators. Int. J. Solids Struct. 51 (3–4), 848–860 . trasound Med. Biol. 24 (9), 1419–1435 . Gei, M. , Roccabianca, S. , Bacca, M. , 2011. Controlling bandgap in electroactive poly- Shmuel, G. , Gei, M. , deBotton, G. , 2012. The rayleigh-lamb wave propagation in di- mer-based structures. IEEE/ASME Trans. Mechatron. 16 (1), 102–107 . electric elastomer layers subjected to large deformations. Int. J. Nonlinear Mech. Hossain, M. , Vu, D.K. , Steinmann, P. , 2015. A comprehensive characterization of 47 (2), 307–316 . the electro-mechanically coupled properties of VHB 4910 polymer. Arch. Appl. Siboni, M.H. , Avazmohammadi, R. , Ponte-Castañeda, P. , 2014. Electromechanical in- Mech. 85 (4), 523–537 . stabilities in ﬁber-constrained, dielectric-elastomer composites subjected to al- Huang, C. , Zhang, Q.M. , deBotton, G. , Bhattacharya, K. , 2004. All-organic dielec- l-around dead-loading. Math. Mech. Solids 1081286514551501 . tric-percolative three-component composite materials with high electrome- Spinelli, S.A. , Lopez-Pamies, O. , 2015. Some simple explicit results for the elastic di- chanical response. Appl. Phys. Lett. 84 (22), 4391–4393 . electric properties and stability of layered composites. Int. J. Eng. Sci. 88, 15–28 . Itskov, M. , Khiêm, V.N. , 2014. A polyconvex anisotropic free energy function for elec- Suo, Z. , 2010. Theory of dielectric elastomers. Acta Mech. Solida Sinica 23 (6), tro-and magneto-rheological elastomers. Math. Mech. Solids 1081286514555140 . 549–578 . Jabareen, M. , 2015. On the modeling of electromechanical coupling in electroac- Suo, Z. , Zhao, X. , Greene, W.H. , 2008. A nonlinear ﬁeld theory of deformable di- tive polymers using the mixed ﬁnite element formulation. Procedia IUTAM 12, electrics. J. Mech. Phys. Solids 56, 467–486 . 105–115 . Toupin, R.A. , 1956. The elastic dielectric. J. Ration. Mech. Anal. 5, 849–915 . Keip, M.A. , Steinmann, P. , Schröder, J. , 2014. Two-scale computational homogeniza- Toupin, R.A. , 1963. A dynamical theory of elastic dielectrics. Int. J. Eng. Sci. 1, tion of electro-elasticity at ﬁnite strains. Comput. Methods Appl. Mech. Eng. 101–126 . 278, 62–79 . Volokh, K.Y. , 2012. On electromechanical coupling in elastomers. J. Appl. Mech. 79 Kornbluh, R. , Pelrine, R. , Prahlad, H. , Wong-Foy, A. , McCoy, B. , Kim, S. , Eckerle, J. , (4), 044507 . Low, T. , 2012. From boots to buoys: Promises and challenges of dielectric elas- Wissler, M. , Mazza, E. , 2007. Electromechanical coupling in dielectric elastomer ac- tomer energy harvesting. In: Lenore, R. (Ed.), Electroactivity in Polymeric Mate- tuators. Sens. Actuators A Phys. 138 (2), 384–393 . rials. Springer, US, pp. 67–93 . Zhao, X. , Hong, W. , Suo, Z. , 2007. Electromechanical hysteresis and coexistent states Li, B. , Chen, H. , Qiang, J. , Hu, S. , Zhu, Z. , Wang, Y. , 2011. Effect of mechanical in dielectric elastomers. Phys. Rev. B 76, 134113 . pre-stretch on the stabilization of dielectric elastomer actuation. J. Phys. D Appl. Zhao, X. , Suo, Z. , 2008. Method to analyze programmable deformation of dielectric Phys. 44 (15), 155301 . elastomer layers. Appl. Phys. Lett. 93, 251902 . Zhao, X. , Suo, Z. , 2010. Theory of dielectric elastomers capable of giant deformation of actuation. Phys. Rev. Lett. 104, 178302 . J. Mech. Phys. Solids 98 (2017) 390–410

Contents lists available at ScienceDirect

Journal of the Mechanics and Physics of Solids

journal homepage: www.elsevier.com/locate/jmps

Elastic wave propagation in ﬁnitely deformed layered materials ⁎ cross Pavel I. Galicha, Nicholas X. Fangb, Mary C. Boycec, Stephan Rudykha, a Department of Aerospace Engineering, Technion – Israel Institute of Technology, Haifa 32000, Israel b Department of Mechanical Engineering, Massachusetts Institute of Technology, Cambridge 02139-4307, MA, USA c School of Engineering and Applied Science, Columbia University, New York 10027, USA

ARTICLE INFO ABSTRACT

Keywords: We analyze elastic wave propagation in highly deformable layered media with isotropic Layered materials hyperelastic phases. Band gap structures are calculated for the periodic laminates undergoing Elastic waves large deformations. Compact explicit expressions for the phase and group velocities are derived Finite deformations for the long waves propagating in the ﬁnitely deformed composites. Elastic wave characteristics Band gaps and band gaps are shown to be highly tunable by deformation. The inﬂuence of deformation on Phononic crystals shear and pressure wave band gaps for materials with various composition and constituent properties are studied, ﬁnding advantageous compositions for producing highly tunable complete band gaps in low-frequency ranges. The shear wave band gaps are inﬂuenced through the deformation induced changes in eﬀective material properties, whereas pressure wave band gaps are mostly inﬂuenced by deformation induced geometry changes. The wide shear wave band gaps are found in the laminates with small volume fractions of a soft phase embedded in a stiﬀer material; pressure wave band gaps of the low-frequency range appear in the laminates with thin highly compressible layers embedded in a nearly incompressible phase. Thus, by constructing composites with a small amount of a highly compressible phase, wide complete band gaps at the low-frequency range can be achieved; furthermore, these band gaps are shown to be highly tunable by deformation.

1. Introduction

Metamaterials have attracted considerable attention due to their unusual properties such as negative elastic moduli (Babaee et al., 2013), mass density (Brunet et al., 2013), and negative refractive index (Liu et al., 2011). Soft metamaterials, capable of large deformations, open promising opportunities for tuning and switching acoustic properties by deformation (Bertoldi and Boyce, 2008a; Rudykh and Boyce, 2014b; Babaee et al., 2016). Even relatively simple deformable homogeneous materials can exhibit switchable acoustic functionalities upon applied deformations (Galich and Rudykh, 2015a). Indeed, soft microstructured metamaterials possess even greater capability for transforming and tuning wave propagation by external stimuli, such as mechanical loading (Rudykh and Boyce, 2014b; Bertoldi and Boyce, 2008b), electric (Gei et al., 2011; Galich and Rudykh, 2016) or magnetic ﬁelds (Destrade and Ogden, 2011). Applied deformation can lead to a change in the internal geometry of a phononic crystal giving rise to formation and/or transformation of phononic band gaps (BGs) (Kushwaha et al., 1993, 1994; Tanaka et al., 2000; Hussein, 2009). Moreover, local material properties can also change as a result of inhomogeneous distribution of local deformation ﬁelds leading to local softening or stiﬀening (Galich and Rudykh, 2015b). In fact, these eﬀects are of signiﬁcant importance for understanding elastic wave phenomena in soft biological tissues that are frequently found in a deformed state due to growth or other

⁎ Corresponding author. E-mail address: [email protected] (S. Rudykh). http://dx.doi.org/10.1016/j.jmps.2016.10.002 Received 4 July 2016; Received in revised form 27 September 2016; Accepted 6 October 2016 Available online 11 October 2016 0022-5096/ © 2016 Elsevier Ltd. All rights reserved. P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410 biological processes. Large deformations together with material heterogeneity may give rise to elastic instabilities (Bertoldi et al., 2008; Rudykh and deBotton, 2012; Li et al., 2013; Slesarenko and Rudykh, 2016) – a phenomenon actively used in material design by nature (Crosby, 2010). Recently, this approach has been employed to utilize instability-induced dramatic microstructure transformations and achieve remarkable tunability of acoustic metamaterials (Bertoldi and Boyce, 2008a; Rudykh and Boyce, 2014b; Babaee et al., 2016). Inspired by possible applications – such as noise reducers, acoustic mirrors and ﬁlters, waveguides, to name a few – a number of recent works were dedicated to the analysis of inﬂuence of material parameters (Zhou et al., 2009), topologies (Mousanezhad et al., 2015), deformations (Bertoldi and Boyce, 2008a), and stiﬀening eﬀects (Wang et al., 2013) on elastic wave propagation and band gap structure in various phononic crystals. Nevertheless, realization of the complex microstructures remains challenging, especially, at small length-scales desirable for some applications. Recent advances in additive and layer-by-layer material manufacturing allow fabrication of highly structured layered materials ranging from sub-light-wavelength scale (Kolle et al., 2013) to meso-length-scale (Li et al., 2013; Rudykh et al., 2015). These layered materials can produce complete phononic BGs – the frequency ranges where neither pressure nor shear waves can propagate – spanning diﬀerent frequency ranges depending on the characteristic microstructure size. Moreover, these BGs can be further actively controlled by deformation. In this work, we speciﬁcally focus on identifying the key parameters deﬁning the appearance of shear wave, pressure wave, and complete BGs in ﬁnitely deformed layered composites with isotropic phases. Special attention is given to the inﬂuence of deformation on the acoustic characteristics and BGs. The layered media exhibit both geometrical and material non-linearities when subjected to ﬁnite strains; hence, these non-linear eﬀects need to be taken into account in the model. To this end, we ﬁrst obtain the solution for the ﬁnitely deformed state of hyperelastic periodic layered materials, and then perform the wave propagation analysis in terms of the incremental small amplitude motions superimposed on the ﬁnitely deformed state. By utilizing an exact analytical solution for the ﬁnitely deformed incompressible laminates with alternating isotropic hyperelastic phases, we derive explicit relations for the phase and group velocities in ﬁnitely deformed incompressible laminates in the long wave limit. Moreover, based on the expressions of the phase velocities for ﬁnitely deformed compressible homogeneous materials, we estimate the phase velocities of pressure and shear waves propagating perpendicular to the layers in ﬁnitely deformed laminates comprised of compressible phases. Next, considering steady- state plane waves in layered media, we thoroughly analyze band gap structures for shear and pressure waves propagating perpendicular to the layers in soft laminates with nearly incompressible and highly compressible phases. We show that wide shear wave BGs at the low-frequency range can be achieved by constructing laminates with thin soft layers embedded in a stiﬀer matrix. Moreover, these band gaps can be further tuned by deformation through the change in the geometry and eﬀective properties of the phases. We ﬁnd that for layers with pronounced stiﬀening eﬀects (such as Gent materials), the change in the material eﬀective properties prevails over the change in the geometry. However, for the materials with weak stiﬀening eﬀects (such as neo-Hookean materials) the deformation induced change in the material properties is entirely compensated by the change in the geometry. We ﬁnd that wide pressure wave BGs at the low-frequency range are attainable in laminates with small amount of highly compressible phase embedded in a nearly incompressible matrix. These pressure wave BGs are highly tunable by deformation. The laminate geometry change induced by deformation is shown to be the dominant factor inﬂuencing pressure wave BGs (as compared to the inﬂuence of the change in the eﬀective material properties). Consequently, wide complete BGs at low-frequency range can be achieved by including a small amount of thin highly compressible phase into a nearly incompressible matrix. Furthermore, these complete BGs can be widened and shifted via deformation.

2. Theoretical background

Consider a continuum body and identify each point in the undeformed conﬁguration with its position vector X. When the body is deformed, the new location of a point is deﬁned by mapping function x =(,χ X t). Thus, the deformation gradient is Fx=∂ /∂X, and its determinant J ≡detF >0. For a hyperelastic material whose constitutive behavior is described in terms of a strain energy function ψ (F), the ﬁrst Piola–Kirchhoﬀ stress tensor is given by ∂()ψ F P = . ∂F (1) The corresponding true or Cauchy stress tensor is related to the ﬁrst Piola–Kirchhoﬀ stress tensor via the relation σ = J−1PFT . In the absence of body forces the equations of motion can be written in the undeformed conﬁguration as

D2χ DivP =ρ , 0 Dt2 (2)

2 2 where ρ0 is the initial density of the material, and the D (•)/Dt operator represents the material time derivative. If the deformation is applied quasi-statically, the right hand part of Eq. (2) can be assumed to be zero, and the equilibrium equation is obtained, namely DivP = 0. (3)

2.1. Wave propagation in homogeneous media

Consider next small amplitude motions1 superimposed on the equilibrium state. The equations of the incremental motions are

391 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

D2u DivP =ρ , 0 Dt2 (4) where Ṗ is an incremental change in the ﬁrst Piola–Kirchhoﬀ stress tensor and u is the incremental displacement. The incremental change in the deformation gradient is F˙ =Gradu. The linearized constitutive law can be written as

PFij̇ = 0 ijkl kl̇ (5)

2 with the tensor of elastic moduli deﬁned as 0iαkβ =∂ψFF /∂iα ∂ kβ. Under substitution of Eq. (5) into Eq. (4) the incremental motion equation takes the form of

2 Dui 0,ijkluρ k lj = . 0 Dt2 (6) To analyze small amplitude motions superimposed on a ﬁnite deformation, we present (6) in the updated Lagrangian formulation

2 ∂ ui ijkluρ k, lj = , ∂t2 (7)

−1 −1 where iqkp = JFF 0ijkl pl qj and ρ = Jρ0 is the density of the deformed material. We seek a solution for Eq. (7) in the form of the plane waves with constant polarization ugnx=(·−),hct (8) where h is a twice continuously diﬀerentiable function and unit vector g is the polarization; the unit vector n deﬁnes the direction of propagation of the wave, and c is the phase velocity of the wave. By substitution of (8) into (7), we obtain

Qn()·= gρc2 g , (9) where

Qij= ijklnn j l (10) is the acoustic tensor which deﬁnes the condition of propagation of the inﬁnitesimal plane waves. For incompressible materials J = 1 and g·=0n , and Eq. (9) reads as

Qn()·= gρc2 g , (11) where QIQI = ^··^ and ^IIn=− ⊗n is the projection on the plane normal to n.

2.2. Wave propagation in periodic layered media

Consider periodic laminates constructed of two alternating phases with initial volume fractions va and vba=1−v . Here and thereafter, the ﬁelds and parameters of the constituents are denoted by subscripts (•)a and (•)b, respectively. Geometrically, the o o o o o layers are characterized by their thicknesses da = vda and db = vdb , where d is the initial period of the laminate (see Fig. 1(a)). When laminates are deformed (see Fig. 1(b)), the layer thicknesses change as follows:

o o o daa=,=,and=,λd11a dbb λdb d λd 1 (12) where λ11=+vλaa vλ bb 1; λ1,ab are the stretch ratios in the direction e1 for phases a and b, respectively. Let us consider steady-state compression small amplitude plane waves superimposed on a ﬁnitely deformed state and propagating along the x direction orthogonal to the interface between the layers (Bedford and Drumheller, 1994) (see Fig. 1(b) and (c)). For each layer, the one-dimensional wave equation takes the form

∂2u ∂2u ξ = c2 ξ , ∂t2 ξ ∂x2 (13) where uξ denotes the displacement in x direction, and subscript ξ stands for a or b. We seek a solution within each layer in the following form2:

ikx(−)ξξ ωt ikxωt (−−) uAeξξ=+, Beξ (14) where ω denotes the angular frequency, and kξ =/ωcξ is the wave number. The normal stress within each layer is

1 Note that we consider only small amplitude elastic waves (Ogden, 1997); the amplitudes of the superimposed on ﬁnite deformations displacements of the material points are assumed to be much (inﬁnitesimally) smaller than any characteristic dimension of the composite, |u|/d ⪡1; so that its geometry and the constitutive properties of the material (such as density and tangent elastic moduli) at each point of the composite are assumed to be unchanged by these small amplitude motions. 2 Note that we consider only small amplitude elastic waves here, i.e. udξ/⪡1.

392 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 1. Schematic representation of the undeformed (a) and deformed (b) periodic layered material with alternating phases a and b. A unit cell (c); (,eee123 , )is the orthonormal basis.

2 2 ∂uξξz ∂uξ σρcξ = ξ ξ = , ∂x ρξ ∂x (15) where zρcξ = ξ ξ is the acoustic impedance. The interface continuity condition between the layers implies

ututab(0, ) = (0, ) and σtσt ab (0, ) = (0, ), (16) where we assign x = 0 to be the interface between the layers of the unit cell (Fig. 1(c)). Two additional conditions are obtained from the periodicity of the material by the use of Floquet theorem. For this reason we adjust Eq. (14) to be the steady-state wave expression with the same wave number k for both materials

ikxωt(− ) uUxeξξ=() , (17) where

iK− x −iK+ x ± Uxξξ()= Aeξξ + Beξ and Kξ = kξ ± k. (18)

According to Floquet theorem, function Uxξ ( ) must be periodic functions of x with the period equal to the length of the unit cell, namely d =+ddab,

Udaa(− ) = Ud bb ( ). (19) The corresponding relations for the stress are

ikxωt(− ) σΣxeξξ=() , (20) where

iK− x −iK+ x Σxξξξ()= izωAe (ξξ − Beξ ) (21) and

393 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Σdaa(− ) = Σd bb ( ). (22) Thus, Eqs. (16), (19) and (22) together with (17), (18), (20) and (21) yield the dispersion relation ωωk=() for the steady-state wave (Rytov, 1956)

⎛ ωd ⎞ ⎛ ωd ⎞ 1 ⎛ z z ⎞ ⎛ ωd ⎞ ⎛ ωd ⎞ coskd = cos⎜ a ⎟ cos⎜ b ⎟ − ⎜ a +sinsinb ⎟ ⎜ a ⎟ ⎜ b ⎟. ⎝ ca ⎠ ⎝ cb ⎠ 2 ⎝ zb za ⎠ ⎝ ca ⎠ ⎝ cb ⎠ (23)

The dispersion relation (23) is derived for pressure waves. However, the same expression can be obtained for shear waves by considering displacements perpendicular to axis x in Eq. (13). In this case, the phase velocities of shear waves are used in (23) to obtain the dispersion relation for shear waves.

3. Results

The macroscopically applied loading is expressed in terms of the average deformation gradient

FF=+,vvaa bb F (24) where Fa and Fb are the corresponding deformation gradients within each phase. The displacement continuity condition along the interface between the layers yields the condition for Fa and Fb

(−)·=FFqab 0 (25) and the interface stress jump condition is

(−)·=,PPm0ab (26) where unit vector m denotes the initial lamination direction (see Fig. 1(a)), q is an arbitrary unit vector orthogonal to m. Loading paths. Although the analysis is general and can be applied for materials subjected to any deformation F, the examples are given for (i) in-plane and (ii) equibiaxial deformations. The corresponding macroscopic deformation gradients are (i) in-plane tension

Feeeeee=⊗+⊗+⊗,λλ11 1 2 2 3 3 (27) (ii) equibiaxial deformation

Fee=⊗+(−⊗),λλ11 1 Iee1 1 (28) where λ is the applied stretch in the direction of the layers (see Fig. 1), and λ1 is an unknown and needs to be calculated. For an −1 −2 incompressible laminate λ1 = λ and λ1 = λ for in-plane and equibiaxial deformations, respectively. To describe the behavior of incompressible phases, we utilize the neo-Hookean strain energy function (Ogden, 1997) μ inc ξ ψ = (:FFξξ −3), ξ 2 (29) where μξ is the initial shear modulus. The constitutive behavior of the compressible phases is assumed to be governed by the extended neo-Hookean strain energy function (Ogden, 1997) μ comp ξ Λξ 2 ψ = (:FFξξ −3)−ln+μJξ (Jξ − 1) , ξ 2 ξ 2 (30) where Λξ is the ﬁrst Lame's parameter. Recall that Λ relates to the bulk modulus as K =+2/Λμ3. By making use of strain energy function (30) together with (25) and (26), the unknown stretch ratios λ1a and λ1b are determined. In particular, the explicit expressions are (i) in-plane tension

ηλγ+ 2(4 + η (4 + η ) λ2 )(2 + ηλγ ( + 2 λ )) γ λ = aaabandλ = , 1a 2 1b 2 2(1 +ηλa ) γ 2(1 +ηλb ) (31)

2 where ηa =/Λμa a, ηb =/Λμb b, and γ =+4+(4+)ηλbbb η η λ; (ii) equibiaxial deformation

ηλζ2422+ 2(4 + η (4 + η ) λ )(2 + ηλ ( ζ + 2 λ )) ζ λ = aaabandλ = , 1a 4 1b 4 2(1 +ηλa ) ζ 2(1 +ηλb ) (32)

24 where ζ =+4+(4+)ηλbbb η η λ . To account for the stiﬀening eﬀects (for example, due to a ﬁnite extensibility of polymer chains) in ﬁnitely deformed incompressible laminates, we employ the strain-energy density function corresponding to an approximation of the Arruda–Boyce model (Arruda and Boyce, 1993), namely the Gent model (Gent, 1996)

394 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

⎛ ⎞ μJmξ FF:−3 inc ξ ⎜ ξξ ⎟ ψξ =− ln 1 − , 2 ⎝ Jmξ ⎠ (33) where Jmξ is the so-called dimensionless locking parameter deﬁning the lock-up stretch ratio, such that in the limit (:FFξξ −3)→J mξ, the strain energy becomes unbounded. Thus, for incompressible Gent materials under in-plane tension, the lock-up stretch ratios can be calculated as

lock λξ =(JJmξ +4 ± mξ )/2, (34) where “+” and “−” correspond to the extension (>1λ ) and contraction (<1λ ), respectively. Clearly, in the limit Jm → ∞, the strain- energy function (33) reduces to the neo-Hookean material model (29). The constitutive behavior of the compressible phases exhibiting strong stiﬀening is assumed to be governed by the extended Gent strain energy function (Horgan and Saccomandi, 2004; Wang et al., 2013) ⎛ ⎞ ⎛ ⎞ μJmξ FF:−3 Λ μ comp ξ ⎜ ξξ ⎟ ⎜ ξξ⎟ 2 ψξ =− ln 1 − −ln+μJξ ξ −(−1),Jξ 2 ⎝ Jmξ ⎠ ⎝ 2 Jmξ ⎠ (35)

Again, in the limit Jm → ∞, the strain-energy function (35) reduces to the extended neo-Hookean material model (30).

3.1. Long wave estimates for ﬁnitely deformed layered materials

3.1.1. Incompressible laminates First, let us consider layered materials with incompressible phases. The incompressibility assumption allows us to obtain a closed form exact solution for ﬁnitely deformed periodic layered materials with neo-Hookean phases (deBotton, 2005; Tzianetopoulou, 2007; Rudykh and Boyce, 2014a; Spinelli and Lopez-Pamies, 2015). By utilizing the exact analytical solution, an eﬀective strain energy function can be constructed (Spinelli and Lopez-Pamies, 2015) μμμ−˘⎛ 1 ⎞ ψ ()=FFF(: −3)− ⎜ mCm·· − ⎟, 2 2 ⎝ mC··−1 m⎠ (36) where CFF=·T is the average right Cauchy–Green deformation tensor, and ⎛ ⎞−1 v v μ =+vμ vμ and˘=+ μ ⎜ a b ⎟ . a a b b ⎝ μa μb ⎠ (37) Note that while the solution for ﬁnitely deformed laminates is provided in deBotton (2005), Tzianetopoulou (2007), Rudykh and Boyce (2014a), Spinelli and Lopez-Pamies (2015), the strain energy function in the form of (36) is reported by Spinelli and Lopez- Pamies (2015). The acoustic tensor (11) corresponding to the strain energy function (36), takes the form

^ ^ −−TT^ Qn(, F )=qq12 I+( IF··)⊗( m IF··), m (38) where

⎛ 2 ⎞ 2 μμ−˘⎜ 4β ⎟ qμ1 =(··)+(˘−)(··)nBn μμnFm and=q2 −1 , α2 ⎝ α ⎠ (39) where BFF=·T is the average left Cauchy–Green deformation tensor, α =·mC−1 ·m, and β =·nF−T · m. One can show that the acoustic tensor (38) has the following eigenvalues in the two-dimensional space normal to n:

2 aq1 =and=+(−).1 aqqαβ2 12 (40) In general, we have two distinct shear waves propagating in the ﬁnitely deformed incompressible laminate. The corresponding phase velocities are

(1) (2) csw =/aρ1 0 and=/, csw aρ2 0 (41) where ρ00=+vρa a vρb 0b is the average initial density of the laminate. Note that the phase velocities of shear waves (41) coincide only for special cases of applied deformation and direction of wave propagation. For instance, for wave propagating perpendicular to the layers, i.e. n ==me1, the phase velocities of shear waves coincide: (i) in-plane tension

(1) (2) −1 csw ===ccλμρsw sw ˘/,0 (42) (ii) equibiaxial deformation

(1) (2) −2 csw ===ccλμρsw sw ˘/.0 (43)

395 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

However, if the wave propagates along the layers, i.e. m = e1 and n = e2, the phase velocities of shear waves are distinct: (i) in-plane tension

(1) csw =/(=)λμρ0 ge3 (44) and

(2) −1 4 csw =λμλ ( ˘ + ( − 1) μρ )/0 (ge =1 ), (45)

(ii) equibiaxial deformation

(1) csw =/(=)λμρ0 ge3 (46) and

(2) −2 6 csw =λμλ ( ˘ + ( − 1) μρ )/0 (ge =1 ). (47)

Note that expressions (45) and (47) yield explicit expressions for the critical stretch ratios corresponding to the onset of macroscopic instability under in-plane and equibiaxial contractions: (i) in-plane tension ⎛ ⎞1/4 pt μ˘ ⎟ λcr =1−⎜ , ⎝ μ ⎠ (48)

(ii) equibiaxial deformation ⎛ ⎞1/6 bt μ˘ ⎟ λcr =1−⎜ . ⎝ μ ⎠ (49)

It is worth mentioning that Eq. (48) agrees with the results obtained by Rosen (1965), and Triantafyllidis and Maker (1985) utilizing distinct approaches. To illustrate the inﬂuence of the deformation and direction of wave propagation on the elastic waves in the layered materials, we construct slowness curves (which are commonly used in acoustics, Auld, 1990) by the use of the explicit relations (41). Fig. 2 shows examples of the slowness curves sφsw ()=1/() cφsw for (a) out-of-plane (with polarization e3) and (b) in-plane (with polarization lying in plane ee1 − 2) shear waves in layered material undergoing equibiaxial deformation, where the direction of propagation is deﬁned as n =(cosφφ ,sin ,0). Note that the critical stretch ratio for the laminate with va =0.1 and μab/=20μ undergoing equibiaxial bt contraction is λcr =0.92; therefore, we present slowness curves corresponding to the equibiaxially contracted laminate (λ =0.95)in the macroscopically stable state. The slowness curves clearly indicate the signiﬁcant inﬂuence of the applied deformation on the wave propagation. Speciﬁcally, an extension results in a decrease of the phase velocities of the shear waves propagating perpendicular to the layers; while the phase velocities increase for waves propagating along the layers since these directions experience extension. The phase velocity of the in-plane shear wave in the equibiaxially deformed laminate has maxima for certain directions of wave

Fig. 2. Slowness curves for (a) out-of-plane and (b) in-plane shear waves propagating in the laminate with va =0.1,μμab / =20, and ρ00ab/=ρ 1 under equibiaxial deformation. Scale is 0.4 per division, and the slownesses are normalized by μρ/ 0 .

396 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410 propagation (see Fig. 2(b)). In particular, these directions are expressed as ⎛ ⎞ ⎜ ⎟ 1 ⎜ 1−λ6 ⎟ ⎜ ⎟ φ0 =± arccos ⎞ +,πz z =0,1. 2 ⎜ ⎛ μ˘ ⎟ ⎜ 41−⎜ ⎟ ⎟ ⎝ ⎝ μ ⎠ ⎠ (50) In the undeformed state, φ =±ππ ,±3 . Moreover, these directions diﬀer from the principal directions in contrast to the out-of- 0 4 4 plane shear wave – the phase velocity of which has maxima in the directions of the principal axes. For example, in the equibiaxially deformed laminate the phase velocity of the out-of-plane shear wave is maximal for the wave propagation along the layers, i.e. for n =±e2 (see Fig. 2(a)). Note that in the undeformed state the phase velocity of the in-plane shear wave is the same for wave propagation along and perpendicular to the layers, namely Eq. (41)2 yields

(2) csw =˘/μρ0 . (51) The dispersion relations for long waves in the incompressible laminates are derived from (41)

(1) (2) ωbρωbρsw =/1 0 and=/sw 2 0 (52) where ⎛ ⎞⎛ ⎞ μμ−˘ 4β 2 β 2 bμ=(··)+(˘−)(··)kBk μμ kFm2 and= bb + ⎜ kk−−,kα2⎟⎜ ⎟ 1 21 2 ⎜ ⎟⎜ 2 ⎟ α ⎝ α ⎠⎝ k ⎠ (53) −T where k is the wave vector, k =|k| is the wave number, and βk =·kF ·m. Now we can ﬁnd the transmission velocity of a wave packet or the group velocity (Kittel, 2004)

vg =∇k ω. (54) From (52) and (54), we obtain the explicit formulae for the group velocities in homogenized laminates

(1) μμμBn·+(˘−)(··)· nFmFm vsw = ρa0 1 (55) and ⎛ ⎛ ⎞ ⎞ ⎞⎞ 1 μμ−˘ ⎛ 8β2 ⎛ 4β4 v(2) = ⎜μμμBn·+(˘−)(··)· nFmFm + ⎜β ⎜5− ⎟F−T ·+ m ⎜ −.α⎟n⎟⎟ sw 2 ⎝ ⎝ ⎠ ⎝ ⎠ ρa0 2 ⎝ α α α ⎠⎠ (56) To illustrate the derived results (55) and (56), energy curves (Nayfeh, 1995) are plotted in Fig. 3. Fig. 3 shows the energy curves for (a) out-of-plane and (b) in-plane shear waves in the laminate with va =0.1,μμab / =20, and ρ00ab/=ρ 1 under equibiaxial deformation. Clearly, the group velocities of the both shear waves strongly depend on the applied deformation and direction of wave

Fig. 3. Energy curves for (a) out-of-plane and (b) in-plane shear waves in the laminate under equibiaxial deformation (va =0.1,μμab / =20, and ρ00ab/=ρ 1). Scale is 0.2 per division, where group velocity is normalized by ρμ0/ .

397 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410 propagation. In particular, an equibiaxial extension increases the group velocity of the out-of-plane shear wave propagating perpendicular to the layers while it decreases the group velocity of the in-plane shear wave propagating in the same direction. An equibiaxial contraction increases group velocities of both the out-of-plane and the in-plane shear waves propagating perpendicular to the layers. Moreover, the energy curves of the in-plane shear waves have the cusps, and position of the cusps is highly tunable by deformation (see Fig. 3(b)). According to Nayfeh (1995) these cusps correspond to regions of null energy. However, for the out-of- plane shear wave the cusps are not observed (see Fig. 3(a)).

3.1.2. Compressible laminates Next we present long wave estimates for the phase velocities of pressure and shear waves propagating in the direction perpendicular to the layers in the ﬁnitely deformed laminate with compressible neo-Hookean and Gent phases. Recall (Boulanger et al., 1994) that the phase velocities of shear and pressure waves in the ﬁnitely deformed neo-Hookean material for

Feeeeeeξξ=⊗+⊗+⊗λλ11 1 22 ξ 2 λ 33 ξ 3and n = e1 are the following:

μ ΛJ2 +(1+) μ λ2 s ξ p ξ ξ ξ 1ξ cξ =λ1ξ andcξ = . ρ0ξ ρ0ξ (57) When the wavelength is much larger than the period of the laminate, the sines can be replaced by their arguments and only second order terms are retained from the cosines in Eq. (23), namely

⎛ ωd ⎞ ωd ⎛ ωd ⎞ ωd2 2 ⎜ ξ ⎟ ξ ⎜ ξ ⎟ ξ sin ≃ and cos ≃ 1 − 2 . ⎝ cξ ⎠ cξ ⎝ cξ ⎠ 2cξ (58) Under this assumption, substitution of (12) and (57) in (23) yields expressions for the phase velocities of shear and pressure waves propagating perpendicular to the layers (n ==me1) in the ﬁnitely deformed layered material with neo-Hookean phases: ˘ csw =λμρ1 ˘/0 and cpw = λΓρ1 /,0 (59) where

˘ −1 2 −2 ΓvΓvΓ=(aa / + bb / ) and ΓΛλλμξ = ξ (23 ξξ ) +ξ (1+ λ1ξ ). (60)

For the in-plane tension (27), λ2ξ = λ and λ3ξ = 1, while for the equibiaxial deformation (28) λ23ξξ==λλ. For the Gent material model, the phase velocities of shear and pressure waves are (Galich and Rudykh, 2015b)

s cξ =/()λμJθρ1ξ ξ mξ ξ 0ξ (61) and

2−2 2 2 p μηJJJθθλλξξ(1+( −2/mξ )ξ +mξ ξ (ξ +21ξξ )1 ) cξ = , ρ0ξ (62) where θJξmξ=3+ξ −FF : ξ. Hence, substitution of (12), (61) and (62) in (23) together with (58) yields expressions for the phase velocities of shear and pressure waves propagating perpendicular to the layers (n ==me1) in the ﬁnitely deformed layered material with Gent phases, namely ˘ ˘ csw = λΘρ1 /0 and cpw = λGρ1 /,0 (63) where ⎞−1⎞ −1 ⎛ v v ⎛ v v Θ˘ =+⎜ a b ⎟ andG˘ =+⎜ a b ⎟ , ⎝ ⎝ Θa Θb ⎠ Ga Gb ⎠ (64) where Θξ =/μJξ mξ θ ξ and ⎛ ⎛ ⎞ ⎞ ⎜ −2 ⎜ 2 ⎟ 2 −2 2 ⎟ Gξ =+−μλξ ⎜ 1ξ ηξ ⎟()+(+2)λλ23ξξ J mξ θξ θξ λ1ξ ⎟. ⎝ ⎝ Jmξ ⎠ ⎠ (65) Fig. 4 shows a comparison of the long wave estimates (59) and (63) with the exact solution (23) for the waves propagating o perpendicular to the layers under equibiaxial deformation. Here and thereafter, we present the normalized frequency fn =/˘fd ρ0 μ , where f =/(2ωπ). Remarkably, the long wave estimates (59) and (63) are in excellent agreement with the exact solution (23) for wavelengths exceeding the eﬀective period of the laminate, namely lπd≳ . For example, for ld=4 the diﬀerences in frequencies between the long wave estimates and exact solution are less than 1% for both shear and pressure waves (see Fig. 4).

3.2. Band gap structure

Band gap is a frequency range where waves cannot propagate due to, for example, Bragg scattering (Kushwaha et al., 1993) or/

398 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 4. Comparison of the long wave estimates (59) and (63) with the exact solution (23) for the waves propagating perpendicular to the layers in the laminates with neo-Hookean ((a) and (c)) and Gent ((b) and (d)) phases under equibiaxial deformation (λ =1.5). va =0.2,μμab / =100, ρ00 a / ρ b =1.5, Λμa /a =10, Λμb /=b 5, Jmb =2.5, and JJma/= mb 2. (a) and (b) correspond to shear waves and (c) and (d) – pressure waves.

Fig. 5. Dispersion diagrams for shear (a) and pressure (b) waves in the laminate with va = 0.3,μμab / = 100, Λμa /a = 100, Λμb /=10b , and ρ00ab/=ρ 1 under ωdo equibiaxial tension, λ =1.5. The shaded areas correspond to the shear (gray) and pressure (blue) wave band gaps. Frequency is normalized as fρμ=/˘ . (For n 2π 0 interpretation of the references to color in this ﬁgure caption, the reader is referred to the web version of this paper.)

399 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410 and local resonance (Auriault and Bonnet, 1985; Auriault, 1994; Liu et al., 2000; Auriault and Boutin, 2012). In case of layered media with high contrast in the mechanical properties between the phases both Bragg scattering and inner resonance of stiﬀer layer (Auriault and Boutin, 2012) participate in formation of band gaps (Khelif and Adibi, 2016). Mathematically, it corresponds to the situation when wave number k becomes imaginary in the dispersion relation (23), i.e. within a band gap displacement and stress amplitudes exponentially attenuate (see Eqs. (17) and (20)). Fig. 5 illustrates the band gap structures of shear and pressure waves in ﬁ 3 the nitely deformed laminate with va = 0.3,μμab / = 100, Λa / μa = 100, Λμb /=1b 0, and with identical densities of the phases, i.e. ρ00ab/=ρ 1. The laminate is subjected to equibiaxial tension with the magnitude of the stretch ratio λ =1.5. The shaded gray and blue areas correspond to the shear and pressure wave BGs, respectively. Clearly, the shear wave BGs appear earlier (i.e. at lower frequencies) than the pressure wave BGs (compare Fig. 5(a) and (b)); thus, to induce complete BGs at the low-frequency range, one needs to design laminates with pressure wave BGs at the low-frequency range. Next, we identify the key parameters that govern the shear and pressure wave band gaps.

3.2.1. Incompressible laminate Here we consider the inﬂuence of (a) microstructures, (b) deformations, and (c) elastic moduli on the band gap structures in incompressible laminates. Recall that incompressible materials support only shear waves; consequently, only shear wave band gaps (SBGs) are considered, while pressure wave BGs (PBG) will be considered in detail in the next section. (a) Material geometry. First, we investigate the inﬂuence of the material geometry on SBG structure. Fig. 6(a) presents the width of the ﬁrst SBG as a function of the volume fraction of phase a. The ﬁrst SBG has a maximal width for a certain volume fraction va; moreover, the maximal width of SBG with corresponding volume fraction of phase a strongly depends on the contrast in shear modulus between the phases (compare Fig. 6(a) and (b)). Thus, for the contrast in shear modulus of μab/=10μ , the maximal width of ﬁ ﬁ the rst SBG is Δfn = 0.41 with va =0.76; while for the contrast in shear modulus of μab/μ = 1000, the SBG width signi cantly increases up to Δfn = 2.25, and the corresponding volume fraction shifts to va =0.97. It is clear that an increase in the shear modulus contrast widens the maximal SBG width. Thus, wide SBGs can be achieved by composing laminates with thin soft layers embedded in the stiﬀ phase (vb =0.03 in Fig. 6(b)). As expected SBGs disappear when va =0or 1. (b) Deformation. Next, we analyze the inﬂuence of deformation on SBGs. We start from the consideration of laminates with phases characterized by weak stiﬀening, which can be described by neo-Hookean model (29). Substitution of the corresponding phase velocities (57)1 into the dispersion relation (23), together with the deformation induced change in geometry (12), yields ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ⎛ ⎞ ρ ρ ρμ ρμ ρ ρ o ⎜ o 000a ⎟ ⎜ o b ⎟ 1 ⎜ aa 0bb⎟ ⎜ o 00a ⎟ ⎜ o b ⎟ coskλ1 d = cos⎜ ωda ⎟cos⎜ωdb ⎟ − ⎜ +sinsin.⎟ ⎜ωda ⎟ ⎜ωdb ⎟ ⎝ μa ⎠ ⎝ μb ⎠ 2 ⎝ ρμ0bb ρμ0aa⎠ ⎝ μa ⎠ ⎝ μb ⎠ (66)

This result clearly shows that SBGs in layered materials with neo-Hookean phases do not depend on deformation. This is due to the ﬀ nH o equal contribution of two competing e ects induced by deformation: (i) the change in the phase properties (i.e. cξ /=cλξ 1ξ, where nH o cξ and cξ are the phase velocities in the deformed and undeformed material) and (ii) change in the layer thicknesses (i.e. o dξ/=dλξ 1ξ). Clearly, any deformation induced change in the geometry is fully compensated by the change in the phase velocity. However, for laminates with phases exhibiting stronger stiﬀening (such as Gent phases), the deformation induced change in the eﬀective properties prevails over the geometry changes. The phase velocities of the shear waves in a deformed Gent material are G nH larger than in the identically deformed neo-Hookean material (i.e. cξ /=cJθξ mξ /> ξ 1) while the changes in the geometry are the same. Fig. 7 presents the relative changes in the phase velocities of the shear waves as functions of the stretch for the neo-Hookean and Gent phases under in-plane tension. Clearly, for the contraction (λ < 1), the phase velocities of the shear waves in the Gent phase increase more signiﬁcantly than in the neo-Hookean phase. For the extension (λ > 1), the phase velocities of the shear waves in the Gent phase decrease in the beginning; however, the phase velocity starts to grow as the stiﬀening eﬀect becomes more pronounced with an increase in deformation. Eventually, the phase velocity becomes larger than the one in the undeformed material. This corresponds to a certain stretch ratio λ* < λlock (see Fig. 7); the expressions for this stretch ratio are

λpt* =1+Jm (67) for the in-plane tension and 1 λ* = 1+JJmmm + 9+(10+ )J bt 2 (68) for the equibiaxial extension. Since in laminates with Gent phases the deformation induced change in material properties (i.e. G o o cξ /=cλJθξ 1ξmξξ /) is not fully compensated by the change in the geometry (i.e. dξ/=dλξ 1ξ), the tunability of SBGs by deformation is observed. Fig. 8 illustrates the dependence of SBGs on in-plane ((a) and (c)) and equibiaxial ((b) and (d)) deformations for the layered lock lock materials with Gent phases. The lock-up stretches for Jm =2.5 are λ− =0.48 and λ+ =2.07 for the in-plane deformation; and lock lock λ− =0.68 and λ+ =1.64for the equibiaxial deformation. We observe that SBGs shift towards higher frequencies and widen as the ﬁ lock-up stretch ratio is approached. In particular, for the laminate with va =0.3,μμab / =100, Jma =5, and Jmb =2.5 the rst SBG widens from Δfn = 0.16 up to Δfn = 0.49 and its lower boundary shifts from fn =0.43 up to fn =1.35 by application of the in-plane

3 Typical deformable polymers are characterized by low densities that change only slightly from polymer to polymer. Therefore, we present the results for laminates with similar or identical phase densities; the values of the density contrast ratio are speciﬁed in each example.

400 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 6. First shear wave band gap vs. volume fraction of phase a for layered materials in undeformed state with (a) μab/=10μ and (b) μab/μ = 1000; ρ00ab/=ρ 1.

Fig. 7. Relative change in the phase velocities of shear waves as functions of in-plane tension for laminates with va = 0.97,μμab / = 1000, Jma = 5, Jmb =2.5, and ρ00ab/=ρ 1. deformation of the magnitude λ =0.5 or λ = 2 (see Fig. 8(a)). The equibiaxial deformation of magnitude λ =0.70or λ =1.58widens ﬁ the rst SBG from Δfn = 0.16 up to Δfn = 0.42 and shifts its lower boundary from fn =0.43 up to fn =1.14 (see Fig. 8(b)). Fig. 8(c) and (d) show the ﬁrst SBG as a function of the stretch ratio for the in-plane (c) and equibiaxial (d) deformations for the laminate with ﬁ the volume fraction producing a maximal width of the rst SBG in the undeformed laminate, namely va =0.97 and μab/μ = 1000. Consistent with the previous observations the ﬁrst SBG widens and shifts towards higher frequencies once the lock-up stretches are ﬁ attained. In particular, lower boundary of the rst SBG shifts from fn =0.33 up to fn =1.00and its width increases from Δfn = 2.25 up to Δfn = 2.73 in the laminate undergoing the in-plane contraction with λ =0.5 or extension with λ = 2 (Fig. 8(c)). Clearly, equibiaxial deformation has a more pronounced eﬀect on SBGs as compared to the in-plane deformation (compare Fig. 8(a) vs. (b) and (c) vs. (d)). Remarkably, contraction (λ < 1) and extension (λ > 1) of the laminate with Gent phases inﬂuence SBGs in similar ways, namely any homogeneous deformations considered here widen and shift up SBGs towards higher frequencies (see Fig. 8). This happens because for both contraction (λ < 1) and extension (λ > 1), the stiﬀening leads to an increase in the phase velocities of the G nH Gent phases compared to the phase velocities of the neo-Hookean constituents, i.e. cξ /=cJθξ mξ /> ξ 1 (see Fig. 7), whereas the ﬀ ﬀ o deformation induced geometry changes are identical for laminates with weak and strong sti ening e ects, i.e. dξ/=dλξ 1ξ. For G o example, the in-plane contraction of the magnitude λ =0.5 increases the phase velocities in the layers a and b up to ca /=2.ca 7 and G o o cb /=6.cb 3, respectively, whereas the layer thicknesses increase up to d/=d 2 only (see Fig. 7). Again, the in-plane extension of the G o G o magnitude λ = 2 decreases the phase velocity in the layer a down to ca /=0.ca 7 and increases it up to cb /cb = 1.6 in the layer b, whereas the layer thicknesses decrease down to d/=0.do 5 (see Fig. 7). Note that for the in-plane tension of magnitude λ =0.5 or λ = 2, the phase velocities in Gent phases increase by the same value compared to the phase velocities of the neo-Hookean phases, G nH G nH G nH G nH namely ca /ccca |λ=0.5 =a /a |λ=2 = 1.35 and cb /cccb |λ=0.5 =b /b |λ =2 = 3.16. This together with the identical deformation induced change in the geometry leads to the identical width and position of the SBGs for these values of the stretch ratio.

401 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 8. Shear wave band gaps vs. in-plane ((a) and (c)) and equibiaxial ((b) and (d)) deformations for the layered materials with Gent phases, namely ρ00ab/=ρ 1, JJma=5, mb =2.5, vμμ a =0.3,ab / =100((a) and (b)) and va = 0.97,μμab / = 1000 ((c) and (d)).

Fig. 9. Shear wave band gaps as a function of locking parameter Jmb for the layered material with vama= 0.3,J = 100, ρ00ab/=ρ 1, and μab/μ = 100 subjected to the in-plane tension of the magnitude λ = 2.

To illustrate the inﬂuence of the stiﬀening of the laminate constituents on the SBGs, we present SBGs as functions of locking parameter Jmb for the layered material with vam= 0.3,J a = 100, and μab/μ = 100 subjected to the in-plane tension of the magnitude λ = 2 in Fig. 9. We observe that SBGs widen and shift towards higher frequencies with a decrease in the locking parameter Jmb.In

402 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 10. Shear band gaps vs. shear modulus contrast for the layered material with va =0.9, ρ00ab/=ρ 1, and JJma== mb 1 in the undeformed state (a) and the one subjected to the in-plane tension with λ =1.5 (b).

ﬁ particular, the lower boundary of the rst SBG shifts from fn =0.44 up to fn =1.35 and its width increases from Δfn = 0.16 up to Δfn = 0.46 when locking parameter of phase b decreases from Jmb = 100 down to Jmb =2.5. This happens because the lock-up stretch ratio (34) decreases together with Jmb, leading to the signiﬁcant increase in the phase velocity of shear wave in the phase b (see Eq. (61)). (c) Shear modulus contrast. To illustrate the inﬂuence of the shear modulus contrast of the phases on SBGs, we present SBGs as functions of the shear modulus contrast for the laminates with va =0.9and Jmξ = 1 in Fig. 10. The corresponding lock-up stretch ratio is λ =1.62. The SBGs of the undeformed (λ = 1) laminate and the one subjected to the in-plane tension with λ =1.5 are presented in Fig. 10(a) and (b), respectively. Fig. 10(a) shows that the ﬁrst SBG rapidly widens with an increase in the contrast from 1 to ∼100, after that the upper boundary ﬂattens, and the SBG width changes slowly with further increase in the shear modulus contrast. The second and the following SBGs close at certain values of the shear modulus contrast. For example, the third SBG closes when

μab/=20μ and μab/=32μ 2; however, the SBG reopens again if the shear modulus contrast increases. For laminates with phases exhibiting strong stiﬀening (such as Gent phases), these BGs shift towards higher frequencies for any shear modulus contrast with ﬁ application of deformation. In particular, the rst SBG widens from Δfn = 0.79 up to Δfn = 1.44 and its lower boundary shifts from fn =0.35 up to fn =0.63 in the laminate with μab/=50μ subjected to the in-plane extension of the magnitude λ =1.5 (Fig. 10(b)).

3.2.2. Compressible laminates To analyze the pressure wave BGs (PBGs), we consider periodic layered materials with compressible phases to ensure the existence of pressure waves. Fig. 11 shows pressure and shear wave BGs as functions of the volume fraction of phase a in the undeformed and deformed laminates. Here and thereafter, gray, blue, and black colors correspond to the shear wave, pressure wave,

Fig. 11. Band gaps vs. volume fraction of the phase a in the undeformed laminate (a) and the one subjected to the in-plane tension of the magnitude λ =1.5 (b) with

μab/μΛμ = 100,a /a = 1000, Λμb /=10b , and ρ00ab/=ρ 1. The gray, blue, and black colors correspond to the shear wave, pressure wave, and complete BGs, respectively. (For interpretation of the references to color in this ﬁgure caption, the reader is referred to the web version of this paper.)

403 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 12. Band gaps vs. in-plane ((a) and (c)) and equibiaxial ((b) and (d)) deformation for laminates with va =0.1,μμab / =100, Λμa /a =1000, Λμb /=10b , and ρ00ab/=ρ 1. (a) and (b) refer to the laminate with neo-Hookean phases and (c) and (d) refer to the laminate with Gent phases having Jma = 5 and Jmb =2.5. and complete BGs, respectively. We refer to complete BGs when both pressure and shear waves cannot propagate. We ﬁnd that the ﬁrst PBG has a maximal width for a certain volume fraction va depending on the contrast in shear moduli and compressibility of each phase. Thus, diﬀerent complete BGs can be tailored by varying the initial material properties and geometry. In the case of shear waves, the ratio of acoustic impedances zzab/ is independent of deformation, although the acoustic impedances zρcξ = ξ ξ for both phases are functions of the principal stretches. Substitution of the corresponding phase velocities −1 (57)1, geometry changes (12), and densities ρξ = Jρξ 0ξ into (23) together with the boundary conditions (25), producing relations λ22ab= λ and λ33ab= λ , yields the dispersion relation (66). Consequently, the SBGs are not inﬂuenced by deformation in the laminates with compressible neo-Hookean phases. Similarly to the laminates with incompressible neo-Hookean phases, the deformation induced changes in the material properties are fully compensated by the changes in the geometry. In the case of pressure waves, the dominant factor inﬂuencing PBGs is the deformation induced change in the geometry. This is due to the fact that the phase velocities of pressure waves in neo-Hookean materials change very slowly with the deformation; moreover, the change is negligible in the case of nearly incompressible materials (see Eq. (57)2). A comparison of the BGs in the undeformed laminates (Fig. 11(a)) and the BGs in the laminates subjected to the in-plane tension, λ =1.5 (Fig. 11(b)), shows that the applied deformation does not change the SBGs while it signiﬁcantly inﬂuences the PBGs. To clarify how the pressure wave and complete BGs depend on deformation in the laminates with compressible phases exhibiting weak and strong stiﬀening, we present these BGs as functions of the applied stretch ratio in Fig. 12. Fig. 12(a) and (b) illustrate how the in-plane (27) and equibiaxial deformations (28) of the layered material with neo-Hookean phases inﬂuence the BG structure. We observe that PBGs narrow and shift towards lower frequencies in the laminate undergoing contraction while extension of the ﬁ laminate widens and shifts PBGs towards higher frequencies. In particular, the lower boundary of the rst PBG shifts from fn =1.65 up to fn =3.17 and its width increases from Δfn = 0.18 up to Δfn = 0.34 in the laminate subjected to the in-plane extension of the magnitude λ = 2 (see Fig. 12(a)). The equibiaxial deformation has a more pronounced eﬀect on the PBGs, in particular, the ﬁ equibiaxial extension of the magnitude λ =1.6shifts the lower boundary of the rst PBG from fn =1.65 up to fn =4.04 and widens it from Δfn = 0.18 up to Δfn = 0.44 (see Fig. 12(b)). Remarkably, complete BGs can be induced in a required frequency range by

404 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 13. Relative change in thicknesses of the layers (a) and phase velocities of pressure (b) waves as functions of equibiaxial deformation for the laminates with ﬁ va =0.1,μμab / =100, Λμa /a =1000, Λμb /=10b , Jma = 5, Jmb =2.5, and ρ00ab/=ρ 1. (For interpretation of the references to color in this gure caption, the reader is referred to the web version of this paper.) deformation while the undeformed laminates do not produce complete BGs in that range. For example, the laminate with va = 0.1,μμab / = 100, Λa / μa = 1000 and Λμb /=1b 0 has no complete BGs (in the considered frequency range) in the undeformed state while it has the complete BG of width Δfn = 0.15 when subjected to the in-plane contraction of the stretch ratio magnitude λ =0.85 (see Fig. 12(a)). In contrast to the in-plane tension, for the equibiaxial deformation we have more “islands” of the complete BGs in the same range of deformation, however, these “islands” are smaller (compare Fig. 12(a) and (b)). Fig. 12(c) and (d) illustrate how the in-plane (27) and equibiaxial deformations (28) of the layered material with compressible Gent phases inﬂuence the BG structure. We observe that in the laminate undergoing in-plane contraction PBGs shift towards lower frequencies less than in laminates with neo-Hookean phases (compare Fig. 12(a) and (c)). In particular, the lower boundary of the ﬁ ﬀ rst PBG shifts from fn =0.94 up to fn =1.23 due to the sti ening of the laminate induced by the in-plane contraction of the magnitude λ =0.5. Analogously, the equibiaxial contraction of the laminate with Gent phases shifts PBGs towards lower frequencies less than in the laminate with neo-Hookean phases (compare Fig. 12(b) and (d)). Speciﬁcally, the lower boundary of the second PBG ﬁ shifts from fn =1.86up to fn =2.39because the laminate under the equibiaxial contraction of the magnitude λ =0.7 signi cantly stiﬀens. Similar to the eﬀect of contraction in the laminate with Gent phases, the extension induced stiﬀening shifts PBGs towards higher frequencies compared to the laminates with neo-Hookean phases. In particular, the lower boundary of the ﬁrst PBG shifts from fn =3.17 up to fn =3.68 in the laminate with Gent phases undergoing the in-plane extension of the magnitude λ = 2 (compare Fig. 12(a) and (c)). Next, let us consider the mechanisms governing the PBGs in the ﬁnitely deformed compressible laminates exhibiting weak and strong stiﬀening. Fig. 13 presents the relative changes in the thicknesses of the layers (a), and the relative changes in the phase velocities of pressure waves (b) in each layer as functions of the stretch ratio. The example is given for the laminates with neo-

Hookean and Gent phases subjected to equibiaxial deformation. The laminate parameters are va = 0.1,μμab / = 100, Λa / μa = 1000, Λμb /=1b 0, Jma = 5, and Jmb =2.5. The corresponding dependence of the BGs on deformation is presented in Fig. 12(b) and (d). A comparison of Fig. 12(b) and (d) together with Fig. 13 shows a correlation between the position of PBGs and changes in the geometry and phase velocities of the layers. In particular, we observe that in the laminate with Gent phases undergoing equibiaxial contraction, the phase velocity of the pressure wave in the highly compressible Gent phase increases while it decreases for the highly compressible neo-Hookean phase (compare continuous blue and dotted black curves in Fig. 13(b)). For example, for the equibiaxial G o nH o contraction of the magnitude λ =0.7 the changes in the pressure wave velocities are cb /cb = 1.11 and cb /cb = 0.91 for the highly compressible Gent and neo-Hookean phases, respectively. On the other hand, the layer thickness of the highly compressible Gent G o nH o phase increases less than for the neo-Hookean phase, namely db /db = 1.53 and db /db = 1.62 for the laminate subjected to the equibiaxial contraction of λ =0.7 (compare continuous blue and dotted black curves in Fig. 13(a)). As a result, the PBGs in the laminates with Gent phases shift towards lower frequencies less than in the laminate with neo-Hookean phases. For the equibiaxial G o nH o extension of the magnitude λ =1.6, the changes in the pressure wave velocities are cb /cb = 1.02 and cb /cb = 1.03 for the highly G o compressible Gent and neo-Hookean phases, respectively (Fig. 13(b)); whereas the changes in the layer thicknesses are db /db = 0.37 nH o ﬀ and db /db = 0.42 (Fig. 13(a)). Although the di erence in the phase velocities and layer thicknesses between the Gent and neo- ﬁ Hookean phases is relatively small, the lower boundary of the rst PBG shifts from fn =4.04 in the laminate with neo-Hookean phases up to fn =4.50 in the laminate with Gent phases undergoing the equibiaxial extension of the magnitude λ =1.6 (see Fig. 12(b) and (d)). This happens because of the nonlinear dependence of PBGs on the changes in the material properties and geometry induced by deformation, especially in the case of the extreme deformations approaching the lock-up state (λlock =1.64). Finally, we consider the inﬂuence of compressibility of the laminate constituents on the BGs. Fig. 14 shows BGs as a function of compressibility of the thin softer layers embedded in the nearly incompressible stiﬀer phase. The results for the undeformed laminate are presented in Fig. 14(a) while the response of the laminate subjected to the equibiaxial compression (λ =0.5) is shown in

405 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 14. Band gaps vs. compressibility of the phase b for the laminate with va = 0.96,μμab / = 100, Λμa /a = 1000, and ρ00ab/=ρ 1 in the undeformed state (a) and the one subjected to the equibiaxial compression, λ =0.5 (b).

Fig. 14(b). We observe complete BGs in low-frequency range when compressibility of softer phase increases (i.e. Λμb / b decreases). ﬁ For example, for the undeformed laminate with Λμb /=1b 0 we observe the rst complete BG of width Δfn = 0.89 with the lower boundary at fn =1.25, while for Λμb />3b 5 there are no complete BGs in the considered frequency range (see Fig. 14(a)). Furthermore, the maximal width and position of the lowest complete BG vary depending on the applied deformation; thus, for the laminate with Λμb /=1b 0 undergoing equibiaxial contraction (λ =0.5), the lowest complete BG has width Δfn = 0.61 with the lower boundary at fn =0.50(see Fig. 14(b)). Note that an increase in compressibility of the thin layers results in a shift of PBGs towards lower frequencies, producing complete BGs at the low-frequency range. Thus, the wide complete BGs can be realized by composing laminates of a nearly incompressible matrix and highly compressible thin layers. Fig. 15 shows BGs as functions of deformations for the laminates with both highly compressible phases exhibiting weak ((a) and (c)) and strong ((b) and (d)) stiﬀening eﬀects. Consistent with the observations in Fig. 14, complete BGs shift down towards lower frequencies. Moreover, the position of complete BGs is highly tunable via deformation. In particular, in the undeformed laminate with va =0.95,μμab / =100, Λa / μa =10, and Λμb /=b 5, the lowest complete BG has the width Δfn = 0.29 with the lower boundary at fn =0.92, while for the laminate under in-plane compression, λ =0.5, the lowest complete BG has the width Δfn = 0.63 with the lower boundary at fn =0.57 (see Fig. 15(a)). In case of the equibiaxial compression, λ =0.5, the lowest complete BG has the width Δfn = 0.75 with the lower boundary at fn =0.46(see Fig. 15(c)). Consequently, the equibiaxial deformation has a more pronounced inﬂuence on the position of complete BGs as compared to the eﬀect of the in-plane deformation. A comparison of Fig. 15(a) and (b) (and also Fig. 15(c) and (d)) shows that in the laminate with Gent phases the PBGs are wider and they appear at higher frequencies compared to the PBGs in the laminates with neo-Hookean phases. This leads to the shifting of complete BGs towards higher frequencies. In particular, the lower boundary of the ﬁrst complete BG in the laminate undergoing the in-plane contraction of the magnitude λ =0.5 shifts from fn =0.57 up to fn =0.71 (compare Fig. 15(a) and (b)). In the case of the ﬁ equibiaxial contraction of magnitude λ =0.7, the lower boundary of the rst complete BG shifts from fn =0.57 up to fn =0.69 (compare Fig. 15(c) and (d)). Similarly to the laminates considered in Fig. 12, the transformations of the BGs correlate with the changes in the thicknesses of the layers and phase velocities within each layer. In particular, an increase in the thicknesses of the layers (d/>do 1) shifts BGs towards lower frequencies whereas a decrease in the layer thicknesses (d/

3.2.3. An example of band gap structures for possible realistic layered materials In this section, we provide a calculation of the BG structure for composites made of silicon rubber (Elite Double 32, Zhermarck) and one of a digital material used in multimaterial 3D printing (A85). Both of these materials can be described by the extended neo- Hookean strain energy function (30). Table 1 summarizes the corresponding parameters for these deformable materials. The phase a is made of the digital material A85, and the phase b is made of the silicon rubber Zhermarck Elite Double 32. Fig. 16 shows pressure and shear wave BGs as functions of the volume fraction of phase a in the undeformed and deformed laminates. We observe that the lowest complete BG has a maximal width for a certain volume fraction va in the undeformed laminate. In particular, for the laminate with va =0.87 the lowest complete BG has width Δfn = 0.26 with the lower boundary at fn =2.50, while for the laminate with va =0.1 the lowest complete BG has width Δ=0.fn 3 with the lower boundary at fn =3.4. Consistent with previous observations in this paper, an extension of the laminate does not change the position of SBGs and shifts up PBGs towards higher frequencies. For example, the ﬁ in-plane extension of the magnitude λ =1.3 shifts the lower boundary of the rst PBG from fn =2.50up to fn =3.23 in the laminate with va =0.87 (compare Fig. 16(a) and (b)). To clarify how the pressure wave and complete BGs depend on deformation in the laminates made of silicon rubber (Elite Double

406 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 15. Band gaps vs. stretch ratio for laminates subjected to ((a) and (b)) in-plane tension and ((c) and (d)) equibiaxial deformations. va =0.95,μμab / =100, Λμa /a =10, Λμb /=b 5, ρ00ab/=ρ 1, and JJma==2. mb 5. (a) and (c) refer to laminate with neo-Hookean phases and (b) and (d) refer to laminate with Gent phases.

32, Zhermarck) and the digital material (A85), we present BGs as functions of the applied stretch ratio in Fig. 17. Fig. 17(a) and (b) illustrate how the in-plane (27) and equibiaxial deformations (28) of the layered material with va =0.3 inﬂuence the BG structure. We observe that PBGs narrow and shift towards lower frequencies in the laminate undergoing contraction while an extension of the ﬁ laminate widens and shifts PBGs towards higher frequencies. In particular, the lower boundary of the rst PBG shifts from fn =3.05 down to fn =2.45 and its width decreases from Δfn = 1.33 down to Δfn = 1.07 in the laminate subjected to the in-plane contraction of the magnitude λ =0.8(see Fig. 17(a)). The equibiaxial deformation has a more pronounced eﬀect on the PBGs; in particular, the ﬁ equibiaxial contraction of the magnitude λ =0.8shifts the lower boundary of the rst PBG from fn =3.05 down to fn =1.98 and narrows it from Δfn = 1.33 down to Δfn = 0.86 (see Fig. 17(b)). Remarkably, complete BGs can be induced in a required frequency range by deformation while the undeformed laminate does not produce complete BGs in that range. For example, the considered here laminate has no complete BGs (in the frequency range up to fn = 3) in the undeformed state while it has the complete BG of width Δfn = 0.49 when subjected to the in-plane contraction of the stretch ratio magnitude λ =0.83 (see Fig. 17(a)). ()BL Fig. 17 also shows the Bragg limit frequency, f =/(2cπdpw ), and an estimate for the resonance frequency of stiﬀer layer, ()R f =/(2cπdpw a). Clearly, the ﬁrst complete BG occurs in the vicinity of the resonance frequency of the stiﬀer layer; moreover, it occurs above the Bragg limit. Hence, a composition of both Bragg scattering and inner resonance of stiﬀer layers participate in formation of complete BGs. In other words, in layered media the mechanism forming complete BGs is based on the destructive

Table 1 Material parameters.

Material μ, MPa Λ, MPa 3 ρ0,kg/m

Elite Double 32 0.444 22.2 1050 Digital material (A85) 22 1100 1200

407 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Fig. 16. Band gaps vs. volume fraction of the phase a in (a) the undeformed laminate and (b) the one subjected to the in-plane tension of the magnitude λ =1.3 with

μab/=50,/=5μΛμa a 0, Λμb /=50b , and ρ00ab/=1.1ρ 4. The gray, blue, and black colors correspond to the shear wave, pressure wave, and complete BGs, respectively. (For interpretation of the references to color in this ﬁgure caption, the reader is referred to the web version of this paper.)

Fig. 17. Band gaps vs. in-plane (a) and equibiaxial (b) deformations for the laminate with va =0.3,μμab / =50, Λμa /a =50, Λμb /=50b , and ρ00ab/=1.1ρ 4. The blue dash-dotted and red dashed curves correspond to estimates of the Bragg limit and the resonance frequency of stiﬀer layer, respectively. (For interpretation of the references to color in this ﬁgure caption, the reader is referred to the web version of this paper.) interference of the scattered waves by the stiﬀer layers and inner resonances of these layers.

4. Conclusions

We considered elastic wave propagation in soft periodic layered media undergoing ﬁnite deformations. Firstly, based on an exact analytical solution for ﬁnitely deformed laminates with alternating neo-Hookean phases, we derived explicit relations for phase (41) and group velocities (55) and (56). Secondly, we obtained long wave estimates (59) and (63) for the phase velocities of pressure and shear waves propagating perpendicular to the layers in the ﬁnitely deformed compressible laminates with neo-Hookean and Gent phases. These estimates provide the important information on elastic wave propagation with wavelengths larger than microstructure size, namely lπd≳ ; moreover, these explicit expressions may provide estimates for transversely isotropic ﬁber composites. Thirdly, we provided a detailed analysis of the band gap structures for the waves propagating perpendicular to the layers in the incompressible and compressible layered materials. Speciﬁcally, we identiﬁed the key parameters and mechanisms inﬂuencing the shear wave, pressure wave, and complete BGs. Based on the analysis, we revealed the advantageous compositions of the laminates producing the wide BGs in the low-frequency range. For incompressible laminates, we showed that (i) a small amount of a soft phase in a stiﬀer matrix produces wide SBGs; (ii) SBG structure in layered materials with phases exhibiting weak stiﬀening eﬀects is not inﬂuenced by deformation because deformation induced changes in geometry and eﬀective material properties compensate each other; (iii) contraction or extension of the laminate

408 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410 with stiﬀening in phases widens and shifts up SBGs towards higher frequencies due to the stronger eﬀect of deformation induced changes in the material properties (as compared to the geometry changes). For compressible laminates, we showed that (i) wide complete BGs can be produced by composing periodic laminates with thin highly compressible layers embedded in a nearly incompressible matrix; (ii) the dominant mechanism inﬂuencing PBGs is the deformation induced change in the thicknesses of the layers; (iii) by application of deformation to the laminates with highly compressible phases, complete BGs in the low-frequency range can be produced. These low-frequency range BGs are not accessible for laminates with nearly incompressible phases. In this work, we considered small amplitude motions (superimposed on ﬁnite deformations); therefore, the presented results cannot be fully applied for ﬁnite amplitude elastic waves propagating in soft microstructured materials. This can be potentially an interesting direction of future research. Another aspect is the inﬂuence of the direction of elastic wave propagation. We fully address this aspect in the analysis of long waves considering any direction of wave propagation and any applied deformations. However, our analysis of elastic wave band gaps focuses on the normal direction of wave propagation, and the consideration of oblique elastic waves would require diﬀerent techniques such as Bloch–Floquet numerical analysis or transfer matrix methods. Finally, we note that a consideration of dissipation can potentially improve the accuracy of the predictions, especially for the composites with constituents characterized by strong damping eﬀects (Babaee et al., 2015).

Acknowledgments

This work was supported by the BASF North American Center for Research of Advanced Materials. S.R. and P.G. gratefully acknowledge the support of the Israel Science Foundation (grant 1550/15 and 1973/15). S.R. thanks the support of Taub Foundation through the Horev Fellowship – Leaders in Science and Technology.

References

Arruda, E.M., Boyce, M.C., 1993. A three-dimensional constitutive model for the large stretch behavior of rubber elastic materials. J. Mech. Phys. Solids 41, 389–412. Auld, B., 1990. Acoustic Fields and Waves in Solids. Krieger Publishing Company, Malabar, Fl. Auriault, J.-L., 1994. Acoustics of heterogeneous media: macroscopic behavior by homogenization. Curr. Top. Acoust. Res. 1, 63–90. Auriault, J.-L., Bonnet, G., 1985. Dynamique des composites lastiques priodiques. Arch Mech. 37 (4–5), 269–284. Auriault, J.-L., Boutin, C., 2012. Long wavelength inner-resonance cut-oﬀ frequencies in elastic composite materials. Int. J. Solids Struct. 49, 3269–3281. Babaee, S., Shim, J., Weaver, J., Chen, E., Patel, N., Bertoldi, K., 2013. 3D soft metamaterials with negative Poisson's ratio. Adv. Mater. 25 (36), 5044–5049. Babaee, S., Viard, N., Wang, P., Fang, N.X., Bertoldi, K., 2016. Harnessing deformation to switch on and oﬀ the propagation of sound. Adv. Mater. 28 (8), 1631–1635. Babaee, S., Wang, P., Bertoldi, K., 2015. Three-dimensional adaptive soft phononic crystals. J. Appl. Phys. 117, 244903. Bedford, A., Drumheller, D., 1994. Elastic Wave Propagation. Wiley, Bedford. Bertoldi, K., Boyce, M.C., 2008a. Mechanically triggered transformations of phononic band gaps in periodic elastomeric structures. Phys. Rev. B 77 (5), 052105. Bertoldi, K., Boyce, M.C., 2008b. Wave propagation and instabilities in monolithic and periodically structured elastomeric materials undergoing large deformations. Phys. Rev. B 78, 184107. Bertoldi, K., Boyce, M.C., Deschanel, S., Prange, S.M., Mullin, T., 2008. Mechanics of deformation-triggered pattern transformations and superelastic behavior in periodic elastomeric structures. J. Mech. Phys. Solids 56 (8), 2642–2668. Boulanger, P., Hayes, M., Trimarco, C., 1994. Finite-amplitude plane waves in deformed Hadamard elastic materials. Geophys. J. Int. 118 (2), 447–458. Brunet, T., Leng, J., Mondain-Monval, O., 2013. Soft acoustic metamaterials. Science 342 (6156), 323–324. Crosby, A.J., 2010. Why should we care about buckling? Soft Matter 6, 5660. deBotton, G., 2005. Transversely isotropic sequentially laminated composites in ﬁnite elasticity. J. Mech. Phys. Solids 53, 1334–1361. Destrade, M., Ogden, R.W., 2011. On magneto-acoustic waves in ﬁnitely deformed elastic solids. Math. Mech. Solids 16, 594–604. Galich, P.I., Rudykh, S., 2015a. Comment on Disentangling longitudinal and shear elastic waves by neo-Hookean soft devices [Appl. Phys. Lett. 106 (2015) 161903]. Appl. Phys. Lett. 107, 056101., http://dx.doi.org/10.1063/1.4928392. Galich, P.I., Rudykh, S., 2015b. Inﬂuence of stiﬀening on elastic wave propagation in extremely deformed soft matter: from nearly incompressible to auxetic materials. Extreme Mech. Lett. 4, 156–161. Galich, P.I., Rudykh, S., 2016. Manipulating pressure and shear elastic waves in dielectric elastomers via external electric stimuli. Int. J. Solids Struct. 91, 18–25. Gei, M., Roccabianca, S., Bacca, M., 2011. Controlling bandgap in electroactive polymer-based structures. IEEE/ASME Trans. Mechatron. 16 (1), 102–107. Gent, A.N., 1996. A new constitutive relation for rubber. Rubber Chem. Technol. 69, 59–61. Horgan, C.O., Saccomandi, G., 2004. Compressible hyperelastic isotropic materials, constitutive models, limiting chain extensibility. J. Elast. 77 (2), 123–138. Hussein, M.I., 2009. Reduced Bloch mode expansion for periodic media band structure calculations. Proc. R. Soc. Lond. Ser. A 465 (2109), 2825–2848. Khelif, A., Adibi, A., 2016. Phononic Crystals. Springer, New York. Kittel, C., 2004. Introduction to Solid State Physics 8th ed.. Wiley, Hoboken, N.J. Kolle, M., Lethbridge, A., Kreysing, M., Baumberg, J., Aizenberg, J., Vukusic, P., 2013. Bio-inspired band-gap tunable elastic optical multilayer ﬁbers. Adv. Mater. 25 (15), 2239–2245. Kushwaha, M., Halevi, P., Dobrzynski, L., Djafari-Rouhani, B., 1993. Acoustic band structure of periodic elastic composites. Phys. Rev. Lett. 71 (13), 2022–2025. Kushwaha, M., Halevi, P., Martinez, G., Dobrzynski, L., Djafari-Rouhani, B., 1994. Theory of acoustic band structure of periodic elastic composites. Phys. Rev. B 49 (4), 2313–2322. Li, Y., Kaynia, N., Rudykh, S., Boyce, M.C., 2013. Wrinkling of interfacial layers in stratiﬁed composites. Adv. Eng. Mater. 15 (10), 921–926. Liu, X.N., Hu, G.K., Huang, G.L., Sun, C.T., 2011. An elastic metamaterial with simultaneously negative mass density and bulk modulus. Appl. Phys. Lett. 98, 251907. Liu, Z., Zhang, X., Mao, Y., Zhu, Y., Yang, Z., Chan, C., Sheng, P., 2000. Locally resonant sonic materials. Science 289 (5485), 1734–1736. Mousanezhad, D., Babaee, S., Ghosh, R., Mahdi, E., Bertoldi, K., Vaziri, A., 2015. Honeycomb phononic crystals with self-similar hierarchy. Phys. Rev. B 92, 104304. Nayfeh, A.H., 1995. Wave Propagation in Layered Anisotropic Media: With Applications to Composites. Elsevier Science, Amsterdam, New York. Ogden, R.W., 1997. Non-Linear Elastic Deformations. Dover Publications, New York. Rosen, B.W., 1965. Mechanics of composite strengthening. In: Fibre Composite Materials. American Society for Metals, Ohio, pp. 37–75. Rudykh, S., Boyce, M., 2014a. Analysis of elasmoid ﬁsh imbricated layered scale-tissue systems and their bio-inspired analogues at ﬁnite strains and bending. IMA J. Appl. Math. 79, 830–847. Rudykh, S., Boyce, M., 2014b. Transforming wave propagation in layered media via instability-induced interfacial wrinkling. Phys. Rev. Lett. 112, 034301. Rudykh, S., deBotton, G., 2012. Instabilities of hyperelastic ﬁber composites: micromechanical versus numerical analyses. J. Elast. 106, 123–147. Rudykh, S., Ortiz, C., Boyce, M., 2015. Flexibility and protection by design: imbricated hybrid microstructures of bio-inspired armor. Soft Matter 11, 2547–2554. Rytov, S., 1956. Acoustical properties of a thinly laminated medium. Sov. Phys. Acoust. 2, 68–80.

409 P.I. Galich et al. J. Mech. Phys. Solids 98 (2017) 390–410

Slesarenko, V., Rudykh, S., 2016. Harnessing viscoelasticity and instabilities for tuning wavy patterns in soft layered composites. Soft Matter 12, 3677–3682. Spinelli, S.A., Lopez-Pamies, O., 2015. Some simple explicit results for the elastic dielectric properties and stability of layered composites. Int. J. Eng. Sci. 88, 15–28. Tanaka, Y., Tomoyasu, Y., Tamura, S.-I., 2000. Band structure of acoustic waves in phononic lattices: two-dimensional composites with large acoustic mismatch. Phys. Rev. B 62 (11), 7387–7392. Triantafyllidis, N., Maker, B.N., 1985. On the comparison between microscopic and macroscopic instability mechanisms in a class of ﬁber-reinforced composites. J. Appl. Mech. Trans. ASME 52, 794–800. Tzianetopoulou, T., 2007. Micro-and Macromechanics of Single Crystal and Polygrannular Lamellar Block Copolymers (Ph.D. thesis). MIT. Wang, P., Shim, J., Bertoldi, K., 2013. Eﬀects of geometric and material non-linearities on the tunable response of phononic crystals. Phys. Rev. B 88, 014304. Zhou, X.-Z., Wang, Y.-S., Zhang, C., 2009. Eﬀects of material parameters on elastic band gaps of two-dimensional solid phononic crystals. J. Appl. Phys. 106, 1.

410 Shear Wave Propagation and Band Gaps in Finitely Deformed Dielectric Elastomer Laminates: Long Wave Estimates and Exact Solution

We analyze small amplitude shear waves (SWs) propagating in dielectric elastomer (DE) laminates subjected to ﬁnite deformations and electrostatic excitations. First, we derive Pavel I. Galich long wave estimates for phase and group velocities of the shear waves propagating in Department of Aerospace Engineering, any direction in DE laminates subjected to any homogenous deformation in the presence Technion—Israel Institute of Technology, of an electric ﬁled. To this end, we utilize a micromechanics-based energy potential for Haifa 32000, Israel layered media with incompressible phases described by neo-Hookean ideal DE model. The long wave estimates reveal the signiﬁcant inﬂuence of electric ﬁeld on the shear Stephan Rudykh wave propagation. However, there exists a conﬁguration, for which electric ﬁeld does not Department of Aerospace Engineering, inﬂuence shear waves directly, and can only alter the shear waves through deformation. Technion—Israel Institute of Technology, We study this speciﬁc conﬁguration in detail, and derive an exact solution for the steady- Haifa 32000, Israel state small amplitude waves propagating in the direction perpendicular to the ﬁnitely e-mail: [email protected] deformed DE layers subjected to electrostatic excitation. In agreement with the long wave estimate, the exact dispersion relation and the corresponding shear wave band gaps (SBGs)—forbidden frequency regions—are not inﬂuenced by electric ﬁeld. How- ever, SBGs in DE laminates with highly nonlinear electroelastic phases still can be manipulated by electric ﬁeld through electrostatically induced deformation. In particular, SBGs in DE laminates with electroelastic Gent phases widen and shift toward higher fre- quencies under application of an electric ﬁeld perpendicular to the layers. However, in laminates with neo-Hookean ideal DE phases, SBGs are not inﬂuenced either by electric ﬁeld or by deformation. This is due to the competing mechanisms of two governing factors: changes in geometry and material properties induced by deformation. In this particular case, these two competing factors entirely cancel each other. [DOI: 10.1115/1.4037159]

Keywords: dielectric elastomers, layered materials, wave propagation, ﬁnite deforma- tions, band gaps

1 Introduction has been revised recently by Dorfmann and Ogden [17], McMeek- ing and Landis [18], and Suo et al. [19]. More recently, Cohen Dielectric elastomers (DEs) can develop large deformations et al. [20] proposed a model based on considerations of polymer when excited by an external electric ﬁeld [1]. Therefore, these networks under electromechanical loadings. Motivated by poten- artiﬁcial muscles are of great interest for various applications, tial enhancement of electromechanical coupling, which is typi- such as soft robotics [2], various actuators [3,4], energy generators cally rather weak in DEs, microstructured DEs have been [5,6], to name a few. It has been recently shown that large defor- explored [21–23] showing signiﬁcant potential of this approach. mations can signiﬁcantly inﬂuence wave propagation even in rela- We note that microstructured DEs may develop instabilities at tively simple deformable materials without electromechanical different length scales [24–28]. coupling [7–10]. In turn, DEs offer a way to manipulate elastic The analysis of small amplitude wave propagation in ﬁnitely waves via application of an external electric ﬁeld. Thus, for exam- deformed nonlinear electroelastic materials in the presence of an ple, the effect has been used to control wave propagation in electric ﬁeld in the frame of the quasi-electrostatic approximation homogenous DEs [11–13]. Moreover, microstructured DEs hold was presented by Dorfmann and Ogden [29]. This paper has been even greater potential for active control of elastic waves by an followed by a number of works on elastic wave propagation in electric ﬁeld [14,15]. Hence, investigation of wave propagation in ﬁnitely deformed homogenous and composite DEs [11–13,30]. composite DEs opens new possibilities in improving of small Note that layered DEs are of speciﬁc importance since they may length-scale devices, for example, micro-electromechanical sys- be realized through various layer-by-layer material fabrication tems, where an electric ﬁeld is the preferred operated variable. techniques, which already allow manufacturing of deformable lay- Following the work of Toupin [16], the theory of nonlinear ered materials across length scales [31–33]. However, the existing electroelasticity for homogeneous isotropic hyperelastic media literature on elastic wave propagation in ﬁnitely deformed DE laminates in the presence of an electric ﬁeld reports some contra- Contributed by the Applied Mechanics Division of ASME for publication in the dictory results. In particular, Shmuel and deBotton [30] consid- JOURNAL OF APPLIED MECHANICS. Manuscript received April 11, 2017; ﬁnal manuscript received June 17, 2017; published online July 7, 2017. Assoc. Editor: ered shear wave band gap (SBGs) structures in DE laminates with Daining Fang. ideal dielectric neo-Hookean incompressible phases, and they

Journal of Applied Mechanics Copyright VC 2017 by ASME SEPTEMBER 2017, Vol. 84 / 091002-1

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use reported that these SBGs alter under application of an external where D and E denote electric displacement and electric ﬁeld electric ﬁeld. However, our results clearly show that the SBGs in applied in the current conﬁguration, respectively. Here and there- the neo-Hookean DE laminates are not inﬂuenced either by elec- after, the differential operators with the ﬁrst low-case letter refer tric ﬁeld or by induced deformation. We note that our results to the current conﬁguration, while the differential operators with agree with the exact solution for the long waves in DE laminates. the ﬁrst upper-case letter refer to the reference conﬁguration. Moreover, the derived dispersion relation reduces to the classical In the reference conﬁguration, the equations of electrostatics result for linear elastic layered media [34] in the absence of an read as electric ﬁeld and deformation. We should note that Shmuel and deBotton [35] have just published the corrigendum reporting that DivDL ¼ 0 and CurlEL ¼ 0 (2) the SBGs in the neo-Hookean DEs are shifted by electric ﬁeld toward higher frequencies. However, these new results by Shmuel where and deBotton [35] do not agree with the exact solution for long 1 T waves and with the exact solution for any wavelengths as detailed DL ¼ JF D and EL ¼ F E (3) in the Appendix. To shed light on the inﬂuence of electric ﬁeld on shear waves in are the Lagrangian counterparts of D and E, respectively. DE laminates, we analyze small amplitude shear wave propagat- ing in DE layered media comprised of two alternating isotropic 2.2 Mechanical Balance Laws. In the absence of body incompressible electroelastic phases. First, we derive the long forces, the linear and angular momentum balance for an electroe- wave estimates for phase and group velocities of shear waves lastic material are propagating in any direction in DE laminates undergoing any T homogenous deformation in the presence of an electric ﬁeld. To divs ¼ qx;tt and s ¼ s (4) this end, we make use of an exact solution for ﬁnitely deformed DE laminates allowing us to express an effective energy potential where s represents the total Cauchy stress tensor and q is the mass in terms of microstructure parameters and physical properties density of the material in the current conﬁguration. of the constituents. These estimates reveal the signiﬁcant In Lagrangian description, the balance equations (4) read as dependence of the shear wave characteristics on electric ﬁeld T T and deformation. However, we found that there is a unique DivP ¼ q0x;tt and P F ¼ F P (5) conﬁguration—when elastic waves propagate perpendicular to the layers—for which phase and group velocities are independent of where electric ﬁeld, and these acoustic characteristics can be inﬂuenced only through electrostatically induced deformations. This holds T P ¼ Js F and q0 ¼ Jq (6) true for any direction of an applied electric ﬁeld. Again, for any other direction of propagation, the phase and group velocities are the ﬁrst Piola–Kirchhoff total stress tensor and the mass den- explicitly depend on electric ﬁeld. We further analyze this speciﬁc sity of the material in the reference conﬁguration, respectively. conﬁguration and derive the dispersion relation for the small amplitude shear waves propagating perpendicular to ﬁnitely 2.3 Constitutive Equations. To model nonlinear behavior of deformed layers with electric ﬁeld applied perpendicular to the DEs, we consider an energy potential wðF; D Þ, as introduced in layers. The derived dispersion relation is shown to be of the same L Dorfmann and Ogden [17]. The strain energy-density potential is form as the relation for hyperelastic laminates [36] undergoing a function of deformation gradient F and Lagrangian counterpart ﬁnite deformations in the absence of an electric ﬁeld. Thus, shear of electric displacement D . Then, for an electroelastic material, waves propagating perpendicular to the layers in DE laminates are L the ﬁrst Piola–Kirchhoff total stress tensor and Lagrangian not affected by electric ﬁeld directly, and they can be inﬂuenced counterpart of electric ﬁeld are given by by electric ﬁeld only through induced deformations. Note that this result is in full agreement with the exact solution for long waves. @w @w Finally, we analyze SBGs in DE laminates by making use of the P ¼ and EL ¼ (7) derived dispersion relation. In particular, we show that SBGs @F @DL widen and shift up toward higher frequencies in DE laminates For an incompressible material, J ¼ 1, and the constitutive equa- with ideal dielectric Gent phases subjected to an electric ﬁeld tions (7) modify as through the thickness of the layers. Once again, SBGs in the DE laminates with neo-Hookean ideal dielectric phases do not depend @w T @w on electric ﬁeld. P ¼ pF and EL ¼ (8) @F @DL

2 Theoretical Background where p denotes an unknown Lagrange multiplier. To describe ﬁnite deformations of a continuous electroelastic body occupying X0 and Xt domains in the reference and current 2.4 Incremental Equations. For an electroelastic material, conﬁgurations, respectively, we introduce the deformation gradi- the incremental constitutive equations for the ﬁrst Piola–Kirchhoff ent FðX; tÞ¼@xðX; tÞ[email protected], where X and x are position vectors in stress and Lagrangian electric ﬁeld read as the reference and current conﬁgurations, respectively. Then, the Jacobian J detF > 0 deﬁnes the volume change of the body P_ ¼ C0 : F_ þ M0 D_ L and E_ L ¼ F_ : M0 þ K0 D_ L (9) with respect to the reference state. respectively. Here, the superposed dot represent incremental 2.1 Electrostatics. In this work, we adopt the so-called quasi- changes in the corresponding variables; C0; M0, and K0 are the electrostatic approximation assuming the absence of magnetic tensors of electroelastic moduli deﬁned as ﬁelds and neglecting electromagnetic interactions. Thus, in the absence of free body charges and currents, the equations of elec- @2w @2w @2w C0 ¼ ; M0 ¼ and K0 ¼ (10) trostatics in the current conﬁguration read as @[email protected] @[email protected] @[email protected]

For an incompressible material, the incremental equations (9) read divD ¼ 0 and curlE ¼ 0 (1) as

091002-2 / Vol. 84, SEPTEMBER 2017 Transactions of the ASME

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use _ _ T _ T T T _ 2 T P ¼ C0 : F þ pF F F p_F þ M0 DL and A^ ¼ Q^ R^ ðÞðÞtrK^ ^I K^ R^ (21) (11) 2 2 ðÞtrK^ trK^ E_ L ¼ F_ : M0 þ K0 D_ L where 2.5 Incremental Motions Superimposed on Finite Deformation in the Presence of an Electric Field. In the frame ^I ¼ I n n (22) of the updated Lagrangian formulation, the incremental forms of the governing Eqs. (2) and (5)1, describing small motions super- is the projection on the plane normal to n; K^ ¼ ^I K ^I; imposed on ﬁnite deformation, transform to Q^ ¼ ^I Q ^I and R^ ¼ ^I R ^I, where divD_ 0; curlE_ 0; and divP_ qx_ (12) L? ¼ L? ¼ ? ¼ ;tt Qik ¼ Cijklnjnl and R ¼ n M (23)

where Note that the generalized acoustic tensor A^ is symmetric. Recall that an incompressible electroelastic material is strongly elliptic D_ ¼ J1F D_ ; E_ ¼ FT E_ ; and P_ ¼ J1P_ FT (13) L? L L? L ? (stable), if its generalized acoustic tensor A^ is positively deﬁned, i.e., g A^ g > 0 for any unit vectors n and g satisfying the are the so-called push-forward versions of D_ L, E_ L, and P_ , respec- tively. Identifying the ﬁeld of incremental displacements as u ¼ x_ incompressibility constraint (J ¼ 1) n g ¼ 0 along an electrome- and then displacement gradient as H ¼ gradu ¼ F_ F1,we chanical loading path deﬁned through a combination of DL and F. obtain the following updated incremental relations (9): 3 Analysis and Results _ _ _ _ P? ¼ C : H þ M DL? and EL? ¼ H : M þ K DL? (14) Consider periodic laminates made out of two isotropic incom- pressible alternating ideal DE phases with volume fractions vðaÞ where and vðbÞ ¼ 1 vðaÞ. Here and thereafter, the ﬁelds and parameters 1 1 of the phases are denoted by superscripts • ðaÞ and • ðbÞ, respec- Cirks ¼ J C0ijklFrjFsl; Mirk ¼M0ijmFrjF and ð Þ ð Þ mk (15) tively. Geometrically, the layers are characterized by their thick- J T 1 K ¼ F K0 F nesses HðaÞ ¼ vðaÞH and HðbÞ ¼ vðbÞH, where H is the period of the undeformed laminate (see Fig. 1(a)). In the deformed lami- are the updated tensors of electroelastic moduli, possessing the nates (see Fig. 1(b)), the layer thicknesses change as follows: following symmetries: ðaÞ ðaÞ ðaÞ ðbÞ ðbÞ ðbÞ h ¼ k2 H ; h ¼ k2 H ; and h ¼ k2H (24) T Cirks ¼ Cksir; Mirk ¼ Mrik; and K ¼ K (16) ðaÞ ðaÞ ðbÞ ðbÞ ða;bÞ where k2 ¼ v k2 þ v k2 and k2 are the stretch ratios in the For an incompressible material, the incremental equations (14) direction e2 for phases a and b, respectively. read as

T P_ ? ¼ C : H þ pH p_I þ M D_ L? and (17) E_ L? ¼ H : M þ K D_ L?

moreover, the incompressibility assumption implies

trH div u ¼ 0 (18)

2.6 Plane Waves in Incompressible DEs Subjected to Electromechanical Loading. We seek for solution of Eq. (12) in the form of plane waves with constant polarizations [29]

u ¼ gf ðn x ctÞ; D_ ¼ dgðn x ctÞ; and L? (19) p_ ¼ Pðn x ctÞ

where f, g, and P are arbitrary twice continuously differentiable, continuously differentiable, and continuous functions, respec- tively; the unit vectors g and d represent polarization vectors of mechanical and electrical displacements, respectively; the unit vector n denotes the direction of wave propagation; and c is the phase velocity of the wave. Substitution of Eqs. (17) and (19) into Eqs. (12) and (18) yields

A^ g ¼ qc2g and g n ¼ 0 (20)

where A^ is the so-called generalized acoustic tensor deﬁning the condition of propagation of plane elastic waves in an incompressi- Fig. 1 Schematic representation of the undeformed (a) and ble electroelastic solid. The generalized acoustic tensor for an subjected to the electromechanical load (b) periodic layered electroelastic material with an arbitrary energy potential wðF; DLÞ material with alternating phases a and b. A unit cell (c); can be calculated as follows [37]: (e1; e2; e3) is the orthonormal basis.

Journal of Applied Mechanics SEPTEMBER 2017, Vol. 84 / 091002-3

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use The macroscopically applied electromechanical loads are where expressed in terms of the average deformation gradient F and ^ 2 Lagrangian electric displacement D L, namely A1 ¼ lðn B nÞþðl lÞðn F mÞ (35)

ðaÞ ðaÞ ðbÞ ðbÞ ðaÞ ðaÞ ðbÞ ðbÞ and F ¼ v F þ v F and DL ¼ v DL þ v DL (25) ^ 2 The continuity of the displacements along the interface between l l 4b 1 1 ðaÞ A2 ¼ 1 the layers yields condition for the deformation gradients F and a2 a ^e e FðbÞ 2 2 2 ðÞD L m 4 ðÞD L m b 1 2 ðaÞ ðbÞ þ ðÞn F D ðF F Þq ¼ 0 (26) a2 c a2 4 L and the continuity of the tractions across the interface between the ðÞD L m ðÞn F D L b (36) layers yields a

ðaÞ ðbÞ ðP P Þm ¼ 0 (27) where B ¼ F FT is the average left Cauchy–Green tensor, a m C 1 m, b n FT m, and c ae=^e b2 1 e=^e . where unit vector m denotes the initial lamination direction (see ¼ ¼ ¼ þ ð Þ One can show that the generalized acoustic tensor (34) has the fol- Fig. 1(a)), and q is an arbitrary unit vector perpendicular to m.In lowing eigenvalues in the two-dimensional space normal to : the absence of free charges at the interfaces, the jump conditions n for Lagrangian electric displacement and electric ﬁeld are 2 a1 ¼ A1 and a2 ¼ A1 þ A2ða b Þ (37) ðaÞ ðbÞ ðaÞ ðbÞ ðDL DL Þm ¼ 0 and ðEL EL Þm ¼ 0 (28) In general, we have two distinct shear waves propagating in In the current conﬁguration, the interface jump conditions (27) ﬁnitely deformed DE laminates in the presence of an electric ﬁeld. and (28) read as The corresponding phase velocities are ðsðaÞ sðbÞÞm ¼ 0; ðDðaÞ DðbÞÞm ¼ 0 and pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ (29) cð1Þ ¼ a =q and cð2Þ ¼ a =q (38) ðEðaÞ EðbÞÞm ¼ 0 sw 1 sw 2

where q ¼ vðaÞqðaÞ þ vðbÞqðbÞ is the average density of the lami- ð1Þ 3.1 Long Wave Estimates for DE Laminates Under nate. Remarkably, the ﬁrst shear wave phase velocity csw is Electromechanical Loads. Let us consider DE laminates with explicitly independent of the electric ﬁeld; moreover, it coincides isotropic incompressible dielectric phases described by the neo- with the phase velocity of the corresponding shear wave propagat- Hookean ideal dielectric model, namely ing in ﬁnitely deformed laminate in the absence of an electric ﬁeld ð2Þ [36]. However, the second shear wave phase velocity csw depends ðÞn l 1 ðÞn ðÞn explicitly on electric ﬁeld. wðÞn ¼ ðÞFðÞn : FðÞn 3 þ D CðÞn D (30) 2 2eðÞn L L Let us consider some particular cases, where for simplicity, we set where lðnÞ and eðnÞ are the shear modulus and the electric permit- T tivity in the undeformed state, respectively; C ¼ F F is the right m ¼ e2 and F ¼ k1e1 e1 þ k2e2 e2 þ k3e3 e3 (39) Cauchy–Green tensor. Under the incompressibility assumption, a closed-form exact solution for ﬁnitely deformed periodic layered First, we study shear waves propagating perpendicular to layers, electroactive materials with neo-Hookean ideal dielectric phases i.e., n ¼ e2. Regardless of the value and the direction of the can be derived [21,24–26]. By utilizing the exact analytical solu- applied electric displacement, the phase velocities of both shear tion, an effective free energy function can be constructed [37] waves are identical and independent of electric quantities, namely qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ^ l l l 1 ð1Þ ð2Þ ^ ðÞ csw ¼ csw ¼ csw ¼ k2 l =q (40) w F; DL ¼ F : F 3 m C m 1 2 2 m C m 2 1 1 1 1 ðÞD m Thus, the phase velocities (40) depend on electric ﬁeld only if L þ DL C DL þ ^ 1 (31) k2 ¼ k2ðD Þ. 2e 2 e e m C m L Second,qﬃﬃﬃﬃﬃﬃﬃ we apply an electric ﬁeld along the layers, T ^ where C ¼ F F is the average right Cauchy–Green tensor, and D L ¼ DL le e1, and study shear waves propagating along the ! layers. Thus, for wave propagation in the same direction as the 1 ðÞa ðÞb applied electric ﬁeld (n ¼ e ), the phase velocities of the shear ðÞa ðÞa ðÞb ðÞb ^ v v 1 l ¼ v l þ v l and l ¼ þ (32) waves are distinct, and one of them depends on the electric ﬁeld, lðÞa lðÞb namely ! pﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 ðÞa ðÞb ð1Þ k l=q ð1Þ ^ v v csw ¼ 1 ðg ¼ e3Þ (41) e ¼ vðÞa eðÞa þ vðÞb eðÞb and e ¼ þ (33) eðÞa eðÞb and vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ The generalized acoustic tensor (21) corresponding to the free u !! u ^ ^ ^ t 2 l 2 e e l energy function (31) takes the form cðÞ2 ¼ k 1 þ k 1 þ D2 1 gðÞ2 ¼ e sw 2 l 1 L e e q 2 T T A^ ðn; F; D LÞ¼A1^I þ A2ð^I F mÞð^I F mÞ (34) (42)

091002-4 / Vol. 84, SEPTEMBER 2017 Transactions of the ASME

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use qﬃﬃﬃﬃﬃﬃﬃ ðnÞ ^ ðnÞ 2 However, for wave propagation perpendicular to the electric ﬁeld where in our case, D ¼ D2e2 ¼ kDL le e2 and B ¼ k e2 1 (n ¼ e3), the phase velocities of the shear waves are distinct and e2 þ k ðI e2 e2Þ. Hence independent of electric ﬁeld, namely ðnÞ ðnÞ ðnÞ 1 ðnÞ pﬃﬃﬃﬃﬃﬃﬃﬃﬃ s11 ¼ s33 ¼ l k p and ð1Þ ð1Þ (50) csw ¼ k3 l=q ðg ¼ e1Þ (43) ðnÞ ðnÞ 2 ðnÞ 1 ^ 2 2 ðnÞ s22 ¼ l k þðe Þ le k DL p and vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ The continuity condition (29)1 and (47)3 yield u !! u ^ t 2 l 2 l ðaÞ ðbÞ ðaÞ ðaÞ ðbÞ ðbÞ cðÞ2 ¼ k 1 þ k gðÞ2 ¼ e (44) s22 ¼ s22 ¼ 0 and v s11 þ v s11 ¼ 0 (51) sw 2 l 3 q 2 By solving the system of equations (51), we obtain an expression for the induced stretch Third, weqﬃﬃﬃﬃﬃﬃﬃ apply an electric ﬁeld perpendicular to the layers ^ (D L ¼ DL le e2) and analyze shear wave propagation along the 2 1=3 k ¼ð1 þ DLÞ (52) layers (n ¼ e1;3). In this case, the phase velocities of shear waves are different, and the phase velocity of the so-called in-plane shear In terms of the Lagrangian electric ﬁeld ð2Þ wave (with polarization g ¼ e2) depends explicitly on electric rﬃﬃﬃﬃ ﬁeld, i.e., l E L ¼ EL e2 (53) pﬃﬃﬃﬃﬃﬃﬃﬃﬃ ^e ð1Þ ð1Þ csw ¼ k1;3 l=q ðg ¼ e3;1Þ (45) 2 where EL ¼ k DL. Equation (52) reads as and vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ E2 ¼ kð1 k3Þ (54) u !! L u ^ ^ t l e l ðÞ2 2 2 2 ðÞ2 Equation (54) yields only one physically relevant solution, csw ¼ k1;3 þ k2 1 DL 1 g ¼ e2 l e q namely (46) pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ g k 1 12g3 1 ﬃﬃﬃ (55) ¼ þ p3 Now, let us consider the example when deformation of DE lam- 2 6 inates is induced by an electric ﬁeld applied perpendicular to the layers, i.e., where vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ qﬃﬃﬃﬃﬃﬃﬃ u sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ^ u 3 2 u 8 3E 3 m ¼ e2; DL ¼ DL le e2; and urﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃL 6 (47) g ¼ qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ þ 29þ 327 256EL ðaÞ ðaÞ ðbÞ ðbÞ t s ¼ v s þ v s ¼ 0 3 6 9 þ 327 256EL

Then, the symmetry of the problem in the plane he1; e3i, the (56) incompressibility assumption, and the continuity condition for dis- placements along interfaces between the layers (26) yield the Note that Eq. (54) yields expressions for the so-called limiting average deformation gradient in the form electric ﬁeld and the corresponding stretch induced by this ﬁeld, namely F ¼ ke e þ k1=2ðI e e Þ (48) pﬃﬃﬃ 2 2 2 2 3 Elim ¼ pﬃﬃﬃ ’ 0:687; klim ¼ 22=3 ’ 0:63; and L 2 3 2 (57) The total Cauchy stress and electric ﬁeld within each phase are pﬃﬃﬃ lim DL ¼ 3 ’ 1:732 ðnÞ ðnÞ ðnÞ ðnÞ 1 ðnÞ ðnÞ ðnÞ ðnÞ ðnÞ ðnÞ s ¼ l B þðe Þ D D p I and E ¼ D =e Figure 2(a) shows the induced stretch (55) as the function of the (49) dimensionless Lagrangian electric ﬁeld. Remarkably, the limiting

Fig. 2 Induced stretch as function of dimensionless Lagrangian (a) and Eulerian (b) electric ﬁelds

Journal of Applied Mechanics SEPTEMBER 2017, Vol. 84 / 091002-5

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use 2=3 c c ; therefore, all presented curves are valid for any induced stretch klim ¼ 2 does not depend on composition of 0 ¼ swjDL¼0 the laminate and coincides with the limiting stretch for homogene- density contrasts qðaÞ=qðbÞ between the layers; moreover, thanks ous DEs [38]. The induced stretch can be expressedqﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ as a function to the normalization the dash-dotted gray curve, corresponding to T ^ the wave propagating perpendicular to the layers, is valid for any of the Eulerian electric ﬁeld, E ¼ F E ¼ E l=e e , where L 2 composition of DE laminates. The phase velocities of both shear 1 E ¼ k EL. Thus, Eq. (54) reads as waves propagating perpendicular to the layers coincide and monotonically decrease with an increase in electric displacement; 2 1 2 E ¼ k k (58) in particular, the phase velocities decrease by 37 % for D ¼ Dlim (see the dash-dotted gray curve in Fig. 3). Figure 2(b) shows the induced stretch as the function of the nor- To illustrate the inﬂuence of electric ﬁeld and direction of wave malized true or Eulerian electric ﬁeld as described by Eq. (58). propagation on the characteristics of elastic waves in the layered Analogously to the case of homogeneous DEs [38], the limiting DEs, we consider wave propagation in the plane he1; e2i, i.e., value of electric ﬁeld may be interpreted as the starting point of n ¼ cos u e1 þ sin u e2. Thus, the expression for the phase veloc- thinning down without limit, afterpﬃﬃﬃ the critical value of electric ities (38) together with Eqs. (48) and (52) reduces to ﬁeld is reached, E Elim ¼ 22=3 3. Hence, in the continuation, vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ we present our examples for electric ﬁelds ranging from 0 up to u ! lim u ^ E . ðÞ 1=3t l l c 1 ðÞu ¼ 1 þ D2 1 þ D2 cos2u þ sin2u (63) For the considered electrostatically induced deformations (48) sw L L l q and (52), the expressions for the phase velocities (40), (45), and (46) read as and (1) n ¼ e2 qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðÞ2 2 1=3 ð1Þ ð2Þ 2 1=3 ^ csw ðÞu ¼ 1 þ DL csw ¼ c ¼ c ¼ð1 þ D Þ l =q (59) vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sw sw L u ! u ^ 1 t l 2 e 2 l (2) n ¼ e1;3 cos22u þ sin 2u þ D2 cos2u cos2u þ sin u l L ^e q pﬃﬃﬃﬃﬃﬃﬃﬃﬃ ð1Þ 2 1=6 ð1Þ (64) csw ¼ð1 þ DLÞ l=q ðg ¼ e3;1Þ (60) and v ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ! By making use of the explicit relations (63) and (64), we construct u u ^ ^ the polar diagrams of slownesses sswðuÞ¼1=cswðuÞ. Figure 4 1=3 e l l ðÞ2 2 t 2 ðÞ2 shows an example of the slowness curves for the so-called out-of- csw ¼ 1 þ DL 1 þ DL ^ g ¼ e2 (61) e l q plane (with polarization g ¼ e3) and in-plane (with polarization lying in the plane he1; e2i) shear waves in the DE laminates sub- Note that if lðaÞ=lðbÞ ¼ eðaÞ=eðbÞ, then ^e =e ¼ l^ =l; hence, for jected to an electric ﬁeld applied perpendicular to the layers. lðaÞ=lðbÞ ¼ eðaÞ=eðbÞ, Eq. (61) reduces to Remarkably, the slownesses of the in-plane shear waves increase qﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ for any direction of wave propagation in DE laminates subjected ^ to an electric ﬁeld, if contrast in electric permittivities is larger cð2Þ ¼ð1 þ D2 Þ1=6 l =q ðgð2Þ ¼ e Þ (62) sw L 2 than the contrast in shear moduli (see Fig. 4(d)). The dispersion relations for long waves in the incompressible Figure 3 shows the normalized phase velocities of the shear waves DE laminates are derived from Eq. (38), and have the following (59)–(61) as functions of the dimensionless Lagrangian electric form: displacement. We normalize the phase velocities by the corre- pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ sponding values in the absence of an electric ﬁeld, i.e., ð1Þ ð2Þ x sw ¼ b1=q and x sw ¼ b2=q (65)

where

^ 2 b1 ¼ lðk B kÞþðl lÞðk F mÞ (66)

and " ^ 2 2 2 l l 4bk 1 1 b2 ¼ b1 þ ak b 1 k a2 ak2 ^e e

2 2 2 ðÞD m 4 ðÞD m b 1 2 L L k þ ðÞk F D a2 c a2 4 L k ðÞD m ðÞk F D b L L k (67) a

where k is the wave vector, k ¼jkj is the wave number, bk ¼ T 2 ^ 2 ^ k F m and ck ¼ ak e=e þ bkð1 e=e Þ. Now, group velocity can be calculated as Fig. 3 The phase velocities of shear waves (59)–(61) as func- tions of the dimensionless electric displacement for laminates vg ¼rkx (68) with v(a) 5 0:2 and l(a)/l(b) 5 5. The phase velocities are nor- malized by the corresponding values in the absence of electric From Eqs. (65) and (68), we obtain the explicit formulae for the ﬁeld. shear wave group velocities in homogenized DE laminates

091002-6 / Vol. 84, SEPTEMBER 2017 Transactions of the ASME

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use Fig. 4 Slowness curves for the out-of-plane (a)–(c) and in-plane (d)–(f) shear waves propagating in the DE laminates with differ- qentﬃﬃﬃ compositions subjected to electric ﬁeld perpendicular to the layers. Scale is 0.4 per division, and slowness is normalized by ^ l/q. Note that the horizontal and vertical axes with the corresponding labels n1/c and n2/c serve for showing the principal directions and physical quantity presented on the polar plot only.

lB n þ l^ l ðÞn F m F m where Dm ¼ DL m and FnD ¼ n F DL. We note that, for vðÞ1 ¼ pﬃﬃﬃﬃﬃﬃﬃﬃ (69) m ¼ e and F ¼ k e e þ k e e þ k e e , the absolute sw qa 2 1 1 1 2 2 2 3 3 3 1 values of the group velocities coincide with the phase velocities for the waves propagating along the principal directions in the DE and laminates subjected to the electric ﬁeld along or perpendicular to the layers. ðÞ2 ﬃﬃﬃﬃﬃﬃﬃﬃ1 ^ To illustrate the inﬂuence of electric ﬁeld and direction of wave vsw ¼ p lB n þ l l ðÞn F m F m qa2 propagation on the energy propagation in DE laminates, we con- sider wave propagation in the plane he1; e2i, i.e., n ¼ cos u e1 ^ 2 4 l l 8b T 4b þsin u e . Recall that the outer normal to the slowness curve þ b 5 F m þ a n 2 a2 a a deﬁnes the direction of the energy ﬂow [39]. Thus, by assigning the absolute value of the group velocity (i.e., jv j) to the normal 1 1 D2 sw þ m bFT m an to the slowness curve for all possible propagation directions, we ^e e a2 construct the polar diagrams for the group velocity or the energy curves [39,40]. In particular, the expression for the group veloc- 2 bD a þ 2b2 bD m F þ F2 n ities (69) and (70) together with Eqs. (48) and (52) yields energy c2 m a nD 4 nD curves shown in Fig. 5. Clearly, the group velocities of shear waves (SWs) strongly depend on the propagation direction and 1 Dmb þ ca b2 F F D applied electric ﬁeld. Application of electric ﬁeld perpendicular to 2 nD a L !!the layers increases the group velocity of the out-of-plane SW 2 propagating along the layers and decreases it for SW propagating b 2Dmb a 2 þ b Dmb FnD þ FnD FnD perpendicular to the layers regardless of laminate composition a a 2 (see Figs. 5(a)–5(c)). While the group velocity of the in-plane SW propagating along the layers can either decrease or increase with eD 2b2 m 2 application of electric ﬁeld depending on the laminate composi- þ ^ 2Dmb 1 þ FnD 2b a e a tion (compare Figs. 5(d)–5(f)). Moreover, the energy curves of the 4 in-plane SWs have intersections, meaning that the absolute values b 2Dmb T F F m (70) and directions of the group velocities coincide for two distinct a nD a wave propagation directions. Remarkably, the position of these

Journal of Applied Mechanics SEPTEMBER 2017, Vol. 84 / 091002-7

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use Fig. 5 Energy curves for the out-of-plane (a)–(c) and in-plane (d)–(f) shear waves propagating in the DE laminates with different compositionsﬃﬃﬃ subjected to electric ﬁeld perpendicular to the layers. Scale is 0.4 per division, where group velocity is normalized p ^ by q/l. Note that the horizontal and vertical lines with the corresponding labels (n1v) and (n2v) serve for showing the principal directions and physical quantity presented on the polar plot only.

intersections changes with a change in the magnitude of the (along the x2 direction, see Fig. 1(c)) in the laminate subjected to applied electric ﬁeld. It is worth noting also that the energy curves macroscopically applied electromechanical loads of plane waves presented here may serve as a tool to deﬁne the wave fronts of impulsive point source excited waves in homoge- qﬃﬃﬃﬃﬃﬃﬃ ^ nized laminates [40,41]. In this case, the intersections of the F ¼ k1e1 e1 þ k2e2 e2 þ k3e3 e3 and D L ¼ DL le e2 energy curves correspond to the regions of null energy [40]. (73)

3.2 Band Gap Structure. In this section, we consider lami- Here, we use the displacement continuity along the interface nates with incompressible electroelastic phases describing by the ðaÞ ðbÞ ðaÞ ðbÞ between the layers (26) producing k1 ¼ k1 k1 and k3 ¼ k3 following energy potential: ðaÞ ðbÞ k3, and the incompressibility assumption yielding k2 ¼ k2 1 k2. Following Tiersten [42], we assume that the incremental wðÞn FðÞn ; DðÞn ¼ wðÞn IðÞn þ IðÞn (71) L elas 1 ðÞn 5 ðnÞ _ ðnÞ ðnÞ 2e ﬁelds u ; DL? , and p_ depend on the coordinate x2 and time t only. Under these assumptions, substitution of Eqs. (17), (18), and where I1 ¼ trC ¼ F : F is the ﬁrst invariant of the right T (72) into Eq. (12) yields Cauchy–Green deformation tensor C ¼ F F,andI5 ¼ DL C DL is the additional invariant accounting for the electromechanical cou- 2 ðÞn 2 2 ðÞn ðÞn 2 ðÞn 2 2 ðÞn pling. The tensors of electroelastic moduli (15) for energy potential @ u1 ðÞn @ u1 @p_ @ u3 ðÞn @ u3 2 ¼ csw 2 ; ¼ 0; and 2 ¼ csw 2 (71) are @t @x2 @x2 @t @x2 (74) 1 CðÞn 2 d BðÞn wðÞn 2BðÞn BðÞn wðÞn d DðÞn DðÞn ; ijkl ¼ ik lj 1 þ ij kl 11 þ ðÞn ik l j e (72) where ðÞn 1 ðÞn ðÞn ðÞn 1 rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ. Mijk ¼ dikDj þ djkDi ; Kij ¼ dij eðÞn eðÞn ðnÞ ðnÞ ðnÞ csw ¼ k2 2w1 q (75) ðnÞ ðnÞ ðnÞ ðnÞ ðnÞ ðnÞ where w1 ¼ @w [email protected] and w11 ¼ @w1 [email protected] . We consider steady-state transversal small amplitude excita- Next, substitution of Eqs. (18), (72), and (73) into Eq. (17) tions propagating perpendicular to the interface between the layers yields

091002-8 / Vol. 84, SEPTEMBER 2017 Transactions of the ASME

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use ! ðÞn ðÞn ðÞn ðaÞ ðaÞ ðbÞ ðbÞ ðÞn @u D @u ðÞn U1 ðh Þ¼U1 ðh Þ (85) P_ 2k2wðÞn 1 2 DðÞn 1 D_ ; ?12 ¼ 2 1 þ ðÞn 2 þ L?1 @x2 e @x2 ! Thus, substitution of Eq. (84) into Eq. (85) yields ðÞn ðÞn 1 ðÞn @u1 ðÞn E_ D D_ ðaÞ ðaÞ ðaÞ ðaÞ ðbÞ ðbÞ ðbÞ ðbÞ L?1 ¼ ðÞn 2 þ L?1 iK h ðaÞ iK h ðaÞ iK h ðbÞ iK h ðbÞ e @x2 e A þ e þ B e A e þ B ¼ 0 ðÞn 2 ðÞn (86) P_ DðÞn D_ p_ ðÞn (76) ?22 ¼ ðÞn 2 L?2 e ! ðnÞ ðnÞ _ iðkx2xtÞ ðÞn ðÞn ðÞn Next, substituting Eq. (83) and DL?1 ¼ d1 ðx2Þe into ðÞn @u D @u ðÞn P_ 2k2wðÞn 3 2 DðÞn 3 D_ ; Eq. (76)1, we obtain ?32 ¼ 2 1 þ ðÞn 2 þ L?3 @x2 e @x2 ! ðÞn _ ðÞn ikxðÞ2xt ðÞn E ðÞx2; t ¼E ðÞx2 e ; ðÞn 1 @u ðÞn L?1 1 E_ ¼ DðÞn 3 þ D_ L?3 ðÞn 2 L?3 1 ix ðÞn ðÞn e @x ðÞn ðÞn iK x2 ðÞn iK x2 ðÞn 2 E ðÞx2 ¼ D2 A e B e þ þ d ðÞx2 1 eðÞn cðÞn 1 ðnÞ (87) where D2 ¼ D2 according to Eq. (29)2. The incremental jump conditions across the interface between and the layers (x2 ¼ 0) are ðÞn ðaÞ ðbÞ ðaÞ ðbÞ ðaÞ ðbÞ _ ðÞn ikxðÞ2xt ______P?12ðÞx2; t ¼P1 ðÞx2 e ; P?12 ¼ P?12; P?22 ¼ P?22; P?32 ¼ P?32; (77) ðÞn 2 ðÞn ix n ðÞn n ðÞn ðÞn ðaÞ ðbÞ ðaÞ ðbÞ ðaÞ ðbÞ ðÞ iK x2 ðÞ iKþ x2 ______P1 ðÞx2 ¼ 2k2w1 A e B e þ D2E1 ðÞx2 EL?1 ¼ EL?1; EL?3 ¼ EL?3; DL?2 ¼ DL?2 cðÞn (88) Hence, substitution of Eq. (76) into Eq. (77) yields where according to Floquet theorem ðÞa ðÞb ðÞa @u1 ðÞb @u1 w1 ¼ w1 ; ðaÞ ðaÞ ðbÞ ðbÞ ðaÞ ðaÞ ðbÞ ðbÞ @x2 @x2 P1 ðh Þ¼P1 ðh Þ; E1 ðh Þ¼E1 ðh Þ; x2¼0 x2¼0 (89) ðaÞ ðaÞ ðbÞ ðbÞ ðÞa ðÞb d1 ðh Þ¼d1 ðh Þ ðÞa @u3 ðÞb @u3 (78) w1 ¼ w1 ; @x2 x ¼0 @x2 x ¼0 2 2 Finally, substitution of Eq. (88) into Eq. (89) yields 1 1 ðÞb ðÞa a a p_ p_ ¼ D2D_ L?2 ðÞ ðÞ ðÞb ðÞb ðÞa w1 iKðÞa hðÞa a w1 iKðÞa hðÞa a w1 iKðÞb hðÞb ðÞb e e e AðÞ e þ BðÞ e A cðÞa cðÞa cðÞb We seek solution for Eq. (74)1 in the form ðÞb w1 iKðÞb hðÞb ðÞb e þ B 0 (90) þ ðÞ ¼ ðnÞ ðnÞ b ðnÞ ðnÞ iðk x2xtÞ ðnÞ iðk x2xtÞ c u1 ¼ A e þ B e (79) System of equations (81), (82), (86), and (90) has a nontrivial where x represents the angular frequency, and kðnÞ ¼ x=cðnÞ is the solution if wave number. The perfect bonding between the layers implies 2 3 111 1 ðaÞ ðbÞ 6 7 u j ¼ u j (80) 6 a a 7 1 x2¼0 1 x2¼0 6 wðÞ wðÞ wðÞb wðÞb 7 6 1 1 1 1 7 Then, the substitution of Eq. (79) into Eq. (80) yields 6 cðÞa cðÞa cðÞb cðÞb 7 det 6 7¼0 6 ðÞa ðÞa ðÞa ðÞa ðÞb ðÞb ðÞb ðÞb 7 6 iK h iKþ h iK h iKþ h 7 ðaÞ ðaÞ ðbÞ ðbÞ 6 e e e e 7 A þ B A B ¼ 0 (81) 6 7 4 ðÞa ðÞa ðÞb ðÞb 5 w1 iKðÞa hðÞa w1 iKðÞa hðÞa w1 iKðÞb hðÞb w1 iKðÞb hðÞb e e þ e e þ Next, the substitution of Eq. (79) into Eq. (78)1 yields cðÞa cðÞa cðÞb cðÞb (91) wðÞa wðÞa wðÞb wðÞb 1 AðÞa 1 BðÞa 1 AðÞb þ 1 BðÞb ¼ 0 (82) cðÞa cðÞa cðÞb cðÞb One can show that Eq. (91) together with Eq. (75) reduces to ! Two additional conditions for constants AðaÞ; BðaÞ; AðbÞ, and ðbÞ xhðÞa xhðÞb B are obtained from the periodicity consideration. Hence, we cos kh ¼ cos cos adjust the form of the solution (79) to be the steady-state wave cðÞa cðÞb expression with the same wave number k for both phases ! ! 1 qðÞa cðÞa qðÞb cðÞb xhðÞa xhðÞb n n þ sin sin (92) ð Þ ð Þ iðkx2xtÞ ðÞb ðÞb ðÞa ðÞa ðÞa ðÞb u1 ¼ U1 ðx2Þe (83) 2 q c q c c c

where describing the dispersion relation x ¼ xðkÞ with cðnÞ and hðnÞ being functions of deformation, which can be induced by electric ðnÞ ðnÞ ðnÞ ðnÞ ðnÞ iK x2 ðnÞ iKþ x2 ðnÞ ﬁeld or otherwise, for example, purely mechanically. The U ðx2Þ¼A e þ B e and K ¼ k 6k (84) 1 6 obtained dispersion relation fully agrees with the exact solution for long waves (40) propagating perpendicular to the layers in ðnÞ According to Floquet theorem, functions U1 ðx2Þ must be peri- electroelastic laminates, clearly showing that shear wave propaga- odic with the period equal to the length of the unit cell (see tion is independent of electric ﬁeld for this conﬁguration. We note Fig. 1(c)), namely h ¼ hðaÞ þ hðbÞ that the dispersion relation (92) is different from those presented

Journal of Applied Mechanics SEPTEMBER 2017, Vol. 84 / 091002-9

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use by Shmuel and deBotton [30,35] as detailed in the Appendix. energy becomes unbounded. Recall that the stiffening effects Moreover, the dispersion relation (92) has the same form as the describing by the Gent model, which is an approximation of the classical result for purely elastic laminates [34], if no deformation Arruda–Boyce model [44], refer to ﬁnite extensibility of polymer is applied. Recently, the dispersion relation by Rytov [34] has chains. For DE laminates with electroelastic Gent phases sub- been extended to account for ﬁnite deformations in purely jected to the electric ﬁeld perpendicular to the layers (as deﬁned mechanical hyperelastic laminates [36]. Remarkably, the disper- in Eq. (47)), the relation between the induced stretch and Lagran- sion relation (92) is identical to the one considered in Galich et al. gian electric displacement is [36] for the purely mechanical problem; the only difference, vﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ! which, however, does not affect the way how SBGs change, is u u 3 ðÞa ðÞa ðÞa ðÞb ðÞb ðÞb tk 1 Jm v l Jm v l that here the deformation is induced by an electric ﬁeld. Thus, the D ¼ k1 þ L ðÞa 3 ðÞb 3 analysis and conclusions of Galich et al. [36] can be fully applied l 2 3 þ Jm k þ k 2 3 þ Jm k þ k here. In particular, Galich et al. [36] showed that SBGs do not (94) depend on deformation in laminates with neo-Hookean phases. This is due to the fact that the two main factors—changes in the Substitution of Eq. (93) into Eq. (75) yields [8] geometry and phase velocity induced by deformation— completely cancel each other [36]. This is again in contradiction sﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ðÞn ðÞn with the conclusions of Shmuel and deBotton [30,35], and Shmuel ðÞn Jm l c ¼ k (95) and Band [43]; these works utilized different dispersion relations, G ðÞn 2 1 ðÞn 3 þ Jm k 2k q but all arrived at the conclusions that SBGs are tunable by an elec- tric ﬁeld [30,35] or by deformation [43] in neo-Hookean ideal Next, by making use of Eqs. (94), (95), (24), and (92), SBG struc- dielectric or purely mechanical neo-Hookean laminates, respec- tures can be constructed for electroelastic laminates subjected to tively. Once again, the SBGs do not depend either on deformation the electric ﬁeld perpendicular to the layers. Figures 6(a)–6(c) or on electric ﬁeld in the neo-Hookean ideal dielectric or purely show the SBGs as functions of the Lagrangian electric displace- mechanical neo-Hookean laminates. ment applied perpendicular to the layers for wave propagating To achieve electric ﬁeld (or deformation)-induced tunability of perpendicular to the layers in the DE laminates with the Gent elec- the SBGs, one should consider laminates with phases exhibiting troelastic phases. Thanks to the speciﬁc normalizationqﬃﬃﬃﬃﬃﬃﬃ of the stronger stiffening, for example, Arruda–Boyce [44] or Gent [45] ^ phases. To illustrate this, we consider laminates with electroelastic Lagrangian electric displacement, namely DL ¼ DL le e2, the phases describing by the energy potential (71) with Gent elastic presented band gaps correspond to DE laminates with any contrast part [45] in electric permittivities eðaÞ=eðbÞ between the layers. The lock-up ! stretch for Jm ¼ 0:5isklock ’ 0:65. Application of DL ¼ 3:5 leads lðÞn JðÞn IðÞn 3 the contraction of the considered DE laminates down to k ’ 0:68. wðÞn ðÞFðÞn ¼ m ln 1 1 (93) elas 2 ðÞn Clearly, the application of the electric ﬁeld perpendicular to the Jm layers widens and shifts SBGs up to the higher frequencies. In particular, the application of the Lagrangian electric displacement ðnÞ where J is the dimensionless parameter deﬁning the lock-up ðaÞ ðaÞ ðbÞ m of DL ¼ 3:5 to the laminate with v ¼ 0:5 and l =l ¼ 10 ðnÞ ðnÞ stretch ratio, such that in the limit ðI1 3Þ!Jm , the strain shifts the lower boundary of the ﬁrst SBG from fn ¼ 0:41 up to

Fig. 6 Shear wave band gaps as functions of dimensionless Lagrangian electric displacement for waves propagating perpen- dicular to the layers. The band gap structures are true for any contrast in electric permittivities e(a)/e(b) between the layers. The (a) (b) (a) (b) locking parameters for Gentqﬃﬃﬃﬃﬃﬃﬃﬃ phases are Jm 5 Jm 5 0:5. The densities of the layers are identical, i.e., q /q 5 1. Frequency is ^ normalized as fn 5 (xH/2p) q/l.

091002-10 / Vol. 84, SEPTEMBER 2017 Transactions of the ASME

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use fn ¼ 0:95 and widens it from Dfn ¼ 0:26 up to Dfn ¼ 0:62 (see Fig. 6(b)). Once again, these changes in SBGs occur due to electrostatically induced deformation. As a comparison, Figs. 6(d)–6(f) show the SBGs as functions of the Lagrangian electric displacement applied perpendicular to the layers for the waves propagating perpendicular to the layers in the DE laminates with the neo-Hookean electroelastic phases. Recall that for the neo- Hookean dielectric elastomer laminates, the normalizedpﬃﬃﬃ limiting lim electric displacement is constant, i.e., DL ¼ 3, while for the Gent dielectric elastomer laminates, the limiting electric ﬁeld depends on the on the locking parameter Jm. Note that for the Gent DE laminates discussed in Fig. 6, the limiting electric ﬁelds are higher than the ones needed to reach the lock-up stretches. Finally, we note that the inﬂuence of stiffening effects on band gap structures in ﬁnitely deformed incompressible and compressi- ble layered materials was thoroughly analyzed by Galich et al. [36]. The only difference is that here we induce deformation by application of an electric ﬁeld.

Fig. 7 Comparison of the exact solution for long waves (59), 4 Conclusion dispersion relation (92), and results reported by Shmuel and We considered shear wave propagation in electroelastic layered deBotton [30,35] for the shear waves propagating perpendicular media subjected to ﬁnite deformations and electric ﬁelds. First, to the layers in the laminates with incompressible ideal DE we derived the long wave estimates—the exact solution for the neo-Hookean phases subjected to electric ﬁeld perpendicular long waves—for phase and group velocities of shear waves propa- to layers, namely DL 5 1:27. The laminate is made of VHB-4910 and ELASTOSIL RT-625: v(a) 5 0.5, l(a)/l(b) 5 1.19, e(a)/e(b) 5 1.74, gating in the laminates with electroelastic neo-Hookean phases. and q(a)/q(b) 5 0.94, where l(b) 5 342 kPa, e(b) 5 2.7, and The derived formulae are expressed in terms of the volume frac- q(b) 5 1020 kg/m3. tions and electroelastic constants of the phases. Moreover, these long wave estimates are given for any direction of wave propaga- tion, and for any applied electric ﬁeld and homogenous ﬁnite deformations. Furthermore, we have found that the shear wave propagation perpendicular to the layers depends on electric ﬁeld only though the induced deformation. Second, we derived the dispersion relations for the shear waves propagating perpendicular to the layers in the laminates with incompressible hyperelastic ideal dielectric phases, described by the energy potential (71). Consistently with the long wave esti- mates, the derived dispersion relation is independent of electric ﬁeld, and the dispersion relation has the same form as its analog for the purely elastic laminates. The dispersion relation shows that SBGs in the electroelastic laminates are tunable by an electric ﬁeld only through induced deformation. In particular, the applica- tion of an electric ﬁeld to the DE laminates with electroelastic Gent phases widens and shifts SBGs toward higher frequencies. However, SBGs do not depend on deformation (induced by an electric ﬁeld or mechanically) in DE laminates with electroelastic neo-Hookean phases. Finally, we emphasize that consideration of dissipation can potentially improve the accuracy of the predic- tions, especially for the composites with constituents character- ized by strong damping effects [46]. Fig. 8 Comparison of the exact solution for long waves (59),dis- persion relation (92), and dispersion relation by Shmuel and Acknowledgment deBotton [35] for the waves propagating perpendicular to the S.R. thanks the support of Taub Foundation through the Horev layers in the laminates with incompressible neo-Hookean phases subjected to electric ﬁeld perpendicular to layers, namely, Fellowship—Leaders in Science and Technology. P.G. thanks the (a) (a) (b) (a) (b) (a) (b) support through the Jacobs Fellowship. DL 5 0:37; v 5 0:8; l /l 5 e /e 5 20, and q /q 5 1

Funding Data vector and frequency as in Shmuel and deBotton [30]. The DE laminate is subjected to the electrostatic excitation of DL ¼ 1:27 Israel Science Foundation (1550/15). (corresponding to D^ ¼ 1:5 in Shmuel and deBotton [30,35]). The continuous black and dotted blue curves correspond to the exact solution for long waves (59) and dispersion relation (92), respec- Appendix: Comparison of Dispersion Relation, Exact tively. The dotted and dashed red curves refer to the results Solution for Long Waves, and Results by Shmuel and reported by Shmuel and deBotton [30] (see Fig. 8(a) therein) and the results presented in Shmuel and deBotton [35] (see Fig. 7(b) deBotton therein), respectively. We observe that the curves for dispersion Figure 7 shows a comparison of the exact solution for long relation (92) and exact solution for long waves (59) overlap, while waves (59), dispersion relation (92), and the results reported by the dispersion curves from Shmuel and deBotton [30,35] signiﬁ- Shmuel and deBotton [30,35]. For clarity, we normalize the wave cantly differ from the exact solution for long waves.

Journal of Applied Mechanics SEPTEMBER 2017, Vol. 84 / 091002-11

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use For completeness, we show a comparison of the exact solution [18] McMeeking, R. M., and Landis, C. M., 2005, “Electrostatic Forces and Stored for long waves (59), dispersion relation (92), and dispersion rela- Energy for Deformable Dielectric Materials,” ASME J. Appl. Mech., 72(4), pp. 581–590. tion reported by Shmuel and deBotton [35] for the DE laminates [19] Suo, Z., Zhao, X., and Greene, W. H., 2008, “A Nonlinear Field Theory of with a more pronounced dispersion. In particular, the comparison Deformable Dielectrics,” J. Mech. Phys. Solids, 56(2), pp. 467–486. is shown for the DE laminates with incompressible neo-Hookean [20] Cohen, N., Dayal, K., and deBotton, G., 2016, “Electroelasticity of Polymer ðaÞ ðaÞ ðbÞ ðaÞ ðbÞ ðaÞ ðbÞ Networks,” J. Mech. Phys. Solids, 92, pp. 105–126. phases with v ¼ 0:8, l =l ¼ e =e ¼ 20, and q =q ¼ 1 [21] deBotton, G., Tevet-Deree, L., and Socolsky, E. A., 2007, “Electroactive Heter- in Fig. 8. The laminate is subjected to the electric ﬁeld perpendicular ogeneous Polymers: Analysis and Applications to Laminated Composites,” Mech. Adv. Mater. Struct., 14(1), pp. 13–22. to the layers, namely, DL ¼ 0:37 (corresponding to D^ ¼ 3inthe [22] Tian, L., Tevet-Deree, L., deBotton, G., and Bhattacharya, K., 2012, “Dielectric notation of Shmuel and deBotton [35]). We observe that dispersion Elastomer Composites,” J. Mech. Phys. Solids, 60(1), pp. 181–198. relation (92) and the exact solution for long waves (59) are in excel- [23] Rudykh, S., Lewinstein, A., Uner, G., and deBotton, G., 2013, “Analysis of lent agreement for the corresponding wavelengths, whereas the Microstructural Induced Enhancement of Electromechanical Coupling in Soft results reported by Shmuel and deBotton [35] produce signiﬁcantly Dielectrics,” Appl. Phys. Lett., 102(15), p. 151905. [24] Rudykh, S., and deBotton, G., 2011, “Stability of Anisotropic Electroactive different results from the exact solution for long waves (59) even in Polymers With Application to Layered Media,” Z. Angew. Math. Phys., 62(6), the long wave limit of kh ! 0. In particular, for this case, the phase pp. 1131–1142. velocity predicted by the exact solution (59) signiﬁcantly differs [25] Bertoldi, K., and Gei, M., 2011, “Instabilities in Multilayered Soft Dielectrics,” from the phase velocity calculated from the dispersion relation by J. Mech. Phys. Solids, 59(1), pp. 18–42. ðSDÞ [26] Rudykh, S., Bhattacharya, K., and deBotton, G., 2014, “Multiscale Instabilities ShmuelanddeBotton[35] by a factor of 2, namely, c ’ 2csw. in Soft Heterogeneous Dielectric Elastomers,” Proc. R. Soc. A, 470(2162), p. 20130618. [27] Abu-Salih, S., 2017, “Analytical Study of Electromechanical Buckling of a References Micro Spherical Elastic Film on a Compliant Substrate—Part I: Formulation [1] Pelrine, R., Kornbluh, R., Pei, Q.-B., and Joseph, J., 2000, “High-Speed Electri- and Linear Buckling of Periodic Patterns,” Int. J. Solids Struct., 109, pp. cally Actuated Elastomers With Strain Greater Than 100%,” Science, 180–188. 287(5454), pp. 836–839. [28] Goshkoderia, A., and Rudykh, S., 2017, “Electromechanical Macroscopic Insta- [2] Bar-Cohen, Y., 2004, Electroactive Polymer (EAP) Actuators as Artiﬁcial bilities in Soft Dielectric Elastomer Composites With Periodic Micro- Muscles: Reality, Potential, and Challenges, Vol. 136, SPIE Press, Bellingham, structures,” Eur. J. Mech. A, 65, pp. 243–256. WA. [29] Dorfmann, A., and Ogden, R. W., 2010, “Electroelastic Waves in a Finitely [3] Rudykh, S., Bhattacharya, K., and deBotton, G., 2012, “Snap-Through Actua- Deformed Electroactive Material,” IMA J. Appl. Math., 75(4), pp. 603–636. tion of Thick-Wall Electroactive Balloons,” Int. J. Nonlinear Mech., 47(2), [30] Shmuel, G., and deBotton, G., 2012, “Band-Gaps in Electrostatically Controlled pp. 206–209. Dielectric Laminates Subjected to Incremental Shear Motions,” J. Mech. Phys. [4] Li, T., Keplinger, C., Baumgartner, R., Bauer, S., Yang, W., and Suo, Z., Solids, 60(11), pp. 1970–1981. 2013, “Giant Voltage-Induced Deformation in Dielectric Elastomers Near [31] Kolle, M., Lethbridge, A., Kreysing, M., Baumberg, J., Aizenberg, J., and the Verge of Snap-Through Instability,” J. Mech. Phys. Solids, 61(2), pp. Vukusic, P., 2013, “Bio-Inspired Band-Gap Tunable Elastic Optical Multilayer 611–628. Fibers,” Adv. Mater., 25(15), pp. 2239–2245. [5] McKay, T., O’Brien, B., Calius, E., and Anderson, I., 2010, “An Integrated, [32] Rudykh, S., Ortiz, C., and Boyce, M., 2015, “Flexibility and Protection by Self-Priming Dielectric Elastomer Generator,” Appl. Phys. Lett., 97(6), Design: Imbricated Hybrid Microstructures of Bio-Inspired Armor,” Soft Mat- p. 062911. ter, 11(13), pp. 2547–2554. [6] Kornbluh, R. D., Pelrine, R., Prahlad, H., Wong-Foy, A., McCoy, B., Kim, S., [33] Slesarenko, V., and Rudykh, S., 2016, “Harnessing Viscoelasticity and Instabil- Eckerle, J., and Low, T., 2012, “From Boots to Buoys: Promises and Challenges ities for Tuning Wavy Patterns in Soft Layered Composites,” Soft Matter, of Dielectric Elastomer Energy Harvesting,” Electroactivity in Polymeric Mate- 12(16), pp. 3677–3682. rials, Springer, Berlin, pp. 67–93. [34] Rytov, S., 1956, “Acoustical Properties of a Thinly Laminated Medium,” Sov. [7] Rudykh, S., and Boyce, M., 2014, “Transforming Wave Propagation in Layered Phys. Acoust., 2, pp. 68–80. Media Via Instability-Induced Interfacial Wrinkling,” Phys. Rev. Lett., 112(3), [35] Shmuel, G., and deBotton, G., 2017, “Corrigendum to ‘Band-Gaps in Electro- p. 034301. statically Controlled Dielectric Laminates Subjected to Incremental Shear [8] Galich, P. I., and Rudykh, S., 2015, “Inﬂuence of Stiffening on Elastic Wave Motions’ [J. Mech. Phys. Solids, 60 (2012) 1970–1981],” J. Mech. Phys. Solids, Propagation in Extremely Deformed Soft Matter: From Nearly Incompressible 105, pp. 21–24. to Auxetic Materials,” Extreme Mech. Lett., 4, pp. 156–161. [36] Galich, P. I., Fang, N. X., Boyce, M. C., and Rudykh, S., 2017, “Elastic Wave [9] Galich, P. I., and Rudykh, S., 2015, “Comment on “Disentangling Longitudinal Propagation in Finitely Deformed Layered Materials,” J. Mech. Phys. Solids, and Shear Elastic Waves by neo-Hookean Soft Devices” [Appl. Phys. Lett., 98, pp. 390–410. 106, 161903 (2015)],” Appl. Phys. Lett., 107(5), p. 056101. [37] Spinelli, S. A., and Lopez-Pamies, O., 2015, “Some Simple Explicit Results for [10] Galich, P. I., Slesarenko, V., and Rudykh, S., 2017, “Shear Wave Propagation the Elastic Dielectric Properties and Stability of Layered Composites,” Int. J. in Finitely Deformed 3D Fiber-Reinforced Composites,” Int. J. Solids Struct., Eng. Sci., 88, pp. 15–28. 110–111, pp. 294–304. [38] Zhao, X., Hong, W., and Suo, Z., 2007, “Electromechanical Hysteresis and [11] Gei, M., Roccabianca, S., and Bacca, M., 2011, “Controlling Bandgap in Elec- Coexistent States in Dielectric Elastomers,” Phys. Rev. B, 76(13), p. 134113. troactive Polymer-Based Structures,” IEEE/ASME Trans. Mechatronics, 16(1), [39] Musgrave, M., 1970, Crystal Acoustics: Introduction to the Study of Elastic pp. 102–107. Waves and Vibrations in Crystals, Holden-Day, San Francisco, CA. [12] Galich, P. I., and Rudykh, S., 2016, “Manipulating Pressure and Shear Elastic [40] Nayfeh, A. H., 1995, Wave Propagation in Layered Anisotropic Media: With Waves in Dielectric Elastomers Via External Electric Stimuli,” Int. J. Solids Applications to Composites, Elsevier Science, New York. Struct., 91, pp. 18–25. [41] Langenberg, K. J., Marklein, R., and Mayer, K., 2010, “Energy vs. Group [13] Wu, B., Su, Y., Chen, W., and Zhang, C., 2017, “On Guided Circumferential Velocity for Elastic Waves in Homogeneous Anisotropic Solid Media,” IEEE Waves in Soft Electroactive Tubes Under Radially Inhomogeneous Biasing URSI International Symposium on Electromagnetic Theory (EMTS), Berlin, Fields,” J. Mech. Phys. Solids, 99, pp. 116–145. Aug. 16–19, pp. 733–736. [14] Yang, W.-P., and Chen, L.-W., 2008, “The Tunable Acoustic Band Gaps of [42] Tiersten, H. F., 1963, “Thickness Vibrations of Piezoelectric Plates,” J. Acoust. Two-Dimensional Phononic Crystals With a Dielectric Elastomer Cylindrical Soc. Am., 35(1), pp. 53–58. Actuator,” Smart Mater. Struct., 17(1), p. 015011. [43] Shmuel, G., and Band, R., 2016, “Universality of the Frequency Spectrum of [15] Celli, P., Gonella, S., Tajeddini, V., Muliana, A., Ahmed, S., and Ounaies, Z., Laminates,” J. Mech. Phys. Solids, 92, pp. 127–136. 2017, “Wave Control Through Soft Microstructural Curling: Bandgap Shifting, [44] Arruda, E. M., and Boyce, M. C., 1993, “A Three-Dimensional Constitutive Reconﬁgurable Anisotropy and Switchable Chirality,” Smart Mater. Struct., Model for the Large Stretch Behavior of Rubber Elastic Materials,” J. Mech. 26(3), p. 035001. Phys. Solids, 41(2), pp. 389–412. [16] Toupin, R. A., 1956, “The Elastic Dielectric,” Arch. Ration. Mech. Anal., 5, pp. [45] Gent, A. N., 1996, “A New Constitutive Relation for Rubber,” Rubber Chem. 849–915. Technol., 69(1), pp. 59–61. [17] Dorfmann, A., and Ogden, R. W., 2005, “Nonlinear Electroelasticity,” Acta. [46] Babaee, S., Wang, P., and Bertoldi, K., 2015, “Three-Dimensional Adaptive Mech., 174(3–4), pp. 167–183. Soft Phononic Crystals,” J. Appl. Phys., 117(24), p. 244903.

091002-12 / Vol. 84, SEPTEMBER 2017 Transactions of the ASME

Downloaded From: http://appliedmechanics.asmedigitalcollection.asme.org/pdfaccess.ashx?url=/data/journals/jamcav/936374/ on 07/08/2017 Terms of Use: http://www.asme.org/about-asme/terms-of-use International Journal of Solids and Structures 110–111 (2017) 294–304

Contents lists available at ScienceDirect

International Journal of Solids and Structures

journal homepage: www.elsevier.com/locate/ijsolstr

Shear wave propagation in ﬁnitely deforme d 3D ﬁb er-reinforced composites

∗ Pavel I. Galich, Viacheslav Slesarenko, Stephan Rudykh

Department of Aerospace Engineering, Technion –Israel Institute of Technology, Haifa 320 0 0, Israel

a r t i c l e i n f o a b s t r a c t

Article history: We investigate the propagation of shear waves in ﬁnitely deformed 3D ﬁber-reinforced composites. We Received 19 September 2016 employ a micromechanics based approach and derive explicit expressions for the phase and group ve-

Revised 19 November 2016 locities of the shear waves in the long wave limit. Thus, we obtain the important characteristics of the Available online 13 December 2016 shear waves in terms of the volume fractions and material properties of the constituents. We ﬁnd that

Keywords: the phase and group velocities signiﬁcantly depend on the applied deformation and direction of wave Fiber-reinforced composites propagation. To account for interactions between the elastic waves and microstructure in ﬁnitely de- Wave propagation formed 3D periodic ﬁber-reinforced materials, we employ the Bloch wave analysis superimposed on large Finite deformations macroscopically applied homogeneous deformations, and we implement the technique into a ﬁnite el- Dispersion ement code. The Bloch wave numerical analysis reveals the essential dispersion phenomenon for the

Transversely isotropic shear waves propagating along the ﬁbers in the ﬁnitely deformed 3D periodic ﬁber-reinforced materials. Micromechanics We ﬁnd that the appearance of the dispersion phenomenon and the corresponding wavelengths can be tuned by material composition and deformation. ©2016 Elsevier Ltd. All rights reserved.

1. Introduction can be controlled by deformation ( Bertoldi and Boyce, 2008b; Bertoldi et al., 2008; Gei, 2008; Rudykh and Boyce, 2014b; Galich Nature actively exploits sophisticated microstructures to et al., 2017; Babaee et al., 2016; Chen and Elbanna, 2016 ). Even achieve remarkable material properties and functionalities. In in relatively simple homogeneous hyperelastic materials, elastic particular, the ﬁber-reinforced deformable composites, possessing wave characteristics can be signiﬁcantly transformed via defor- a light weight, high strength and ﬂexibility at the same time, are mation ( Dorfmann and Ogden, 2010; Galich and Rudykh, 2015b; widely present in nature ( Saheb and Jog, 1999 ). However, natural 2015a; 2016 ). It is worth noting that many soft biological tissues materials are biodegradable and poorly resistant to moisture, and are found to possess ﬁber-matrix microstructures ( Humphrey, not always they can provide desirable properties; therefore, syn- 2002 ), and the soft tissues frequently experience large defor- thetic composite materials are of a great interest. The mechanical mations due to growth or other physiological processes. Hence, performance of composite materials can be tailored by designing investigation of elastic wave propagation in 3D ﬁber compos- microstructures combining soft and stiff constituents. Recent ites (FCs) undergoing ﬁnite deformations can be beneﬁcial for advances in the material fabrication techniques and 3D-printing biomedical applications such as ultrasound testing. already allow realization of microstructured metamaterials with Small amplitude elastic wave propagation in ﬁnitely deformed various properties and functionalities ( Babaee et al., 2013; Kolle homogeneous isotropic materials was pioneered by Biot (1940) on et al., 2013; Rudykh and Boyce, 2014a; Lin et al., 2014; Ge et al., the basis of the static nonlinear theory ( Biot, 1939 ). Waves of 2013; Bafekrpour et al., 2014; Rudykh et al., 2015; Celli and a ﬁnite amplitude propagating in a pre-stressed elastic medium Gonella, 2015; Srivastava, 2016; Golub et al., 2012; Fomenko et al., were investigated by John (1966) , and Currie and Hayes (1969) . 2014 ). Moreover, soft metamaterials can be reversibly deformed, Boulanger and Hayes (1992) considered wave propagation in and, thus, enabling us to manipulate their effective properties via ﬁnitely deformed incompressible Mooney–Rivlin materials and deformation ( Li et al., 2013; Slesarenko and Rudykh, 2016 ). Thus, derived explicit relations for wave velocities. Boulanger et al. for example, elastic wave propagation in soft composite materials (1994) extended this work to a broader class of ﬁnitely deformed compressible Hadamard materials and ﬁrst obtained the explicit expressions for the phase velocities of longitudinal and transver-

∗ Corresponding author. sal waves. Recently, Destrade and Ogden (2013) have revised and

E-mail address: [email protected] (S. Rudykh). generalized the problem of an inﬁnitesimal wave propagation in http://dx.doi.org/10.1016/j.ijsolstr.2016.12.007 0020-7683/© 2016 Elsevier Ltd. All rights reserved. P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304 295 the ﬁnitely deformed hyperelastic materials by application of the the new location of the corresponding points is deﬁned by map- invariant theory. More recently, Galich and Rudykh (2015b ) have ping function x = χ(X , t) . Hence, the deformation gradient is F = investigated inﬁnitesimal wave propagation in ﬁnitely deformed ∂ x /∂ X , and its determinant J ≡ det F > 0 . For a hyperelastic ma- compressible Gent materials, exhibiting pronounced stiffening ef- terial described by a strain energy function ψ( F ), the ﬁrst Piola– fects, and obtained closed form expressions for the phase velocities Kirchhoff stress tensor can be calculated as follows of longitudinal and transversal waves. ∂ψ(F ) By employing the nonlinear elastic theory ( Truesdell and P = . (1) ∂F Noll, 1965 ) and a phenomenological approach, Scott and Hayes = (1976) considered small amplitude plane waves superimposed For an incompressible material, J 1 and Eq. (1) modiﬁes as on a homogeneous deformation in the so-called idealized ﬁber- ∂ψ(F ) − P = − pF T , (2) reinforced materials, assuming an incompressible matrix and in- ∂F extensible ﬁbers. Later, Scott (1991, 1992) extended this analysis where p represents an unknown Lagrange multiplier. The corre- and considered inﬁnitesimal vibrations of an arbitrary form su- sponding Cauchy stress tensor is related to the ﬁrst Piola-Kirchhoff perimposed on a ﬁnite deformation for a broad class of elastic stress tensor via the relation σ = J −1 P · F T . anisotropic materials. The inﬁnitesimal elastic wave propagation In the absence of body forces the equations of motion can be in nearly incompressible and nearly inextensible ﬁber-reinforced written in the undeformed conﬁguration as materials with unidirectional and orthogonal ﬁbers was examined by Rogerson and Scott (1994) . More recently, Ogden and Singh D 2 χ DivP = ρ , (3) (2011) revisited the problem of inﬁnitesimal wave propagation in 0 Dt 2 an incompressible transversely isotropic elastic solid in the pres- ρ where 0 is the initial density of the material and the operator ence of an initial stress. In their work, Ogden and Singh (2011) ex- D 2( • )/ Dt 2 represents the material time derivative. If the deforma- ploited the phenomenological theory of invariants and presented a tion is applied quasi-statically, the right hand part of Eq. (3) can more general and transparent formulation of the theory for small be assumed to be zero, and the equilibrium equation is obtained amplitude waves propagating in a deformed transversely isotropic as hyperelastic solid. In this work, we employ a micromechanics based approach ac- DivP = 0 . (4) counting for the phase properties and their spatial distribution Consider next inﬁnitesimal motions superimposed on the equi- to analyze the wave propagation in ﬁnitely deformed 3D FCs, as librium state. The equations of the incremental motions are opposite to previous works that employ phenomenological ap- proach ( Scott and Hayes, 1976; Scott, 1991, 1992; Rogerson and D 2 u DivP ˙ = ρ , (5) Scott, 1994; Ogden and Singh, 2011 ), or numerically model the 0 Dt 2 composites in 2D settings ( Rudykh and Boyce, 2014b; Bertoldi and where P˙ is the incremental change in the ﬁrst Piola–Kirchhoff Boyce, 2008b ), or do not consider ﬁnite deformations ( Aberg and stress tensor and u is the incremental displacement. Gudmundson, 1997; Kushwaha et al., 1993 ). Here, we derive ex- The linearized constitutive law can be written as plicit closed form expressions for phase and group velocities of = A , the shear waves for any direction of wave propagation in ﬁnitely P˙ij 0 ijkl F˙kl (6) deformed 3D ﬁber-reinforced materials with neo-Hookean phases.

These explicit expressions provide important information on the where F˙ = Grad u is the incremental change in the deformation A = elastic wave propagation in the long wave limit. To account for gradient, and the tensor of elastic moduli is deﬁned as 0 iαkβ ∂ 2 ψ/∂ ∂ the interaction of the elastic waves with the composite microstruc- Fiα Fkβ . Under substitution of Eq. (6) into Eq. (5) the incre- ture, the Bloch wave analysis is implemented in the ﬁnite ele- mental motion equation takes the form ment code, allowing us to analyze small amplitude motions su- 2 D u i perimposed on ﬁnite macroscopically applied homogeneous defor- A u , = ρ . (7) 0ijkl k lj 0 Dt 2 mations. It should be noted that we analyze the ﬁnitely deformed ﬁbrous materials in fully 3D settings –both the deformation and 3. Long wave estimates for ﬁnitely deformed incompressible the direction of the wave propagation – which, to the best of our ﬁber composites knowledge, is not covered in the existing literature. We investi- gate the role of the material composition and phase properties To analyze small amplitude motions superimposed on a ﬁnite in the dispersion of shear waves. We speciﬁcally focus on the in- deformation, we present equation of motion (7) in the updated La- ﬂuence of deformation on the dispersion of the shear waves. By grangian formulation considering the waves propagating in the direction of ﬁbers, we 2 ﬁnd that the applied deformation strongly affects the long waves; ∂ u i A u , = ρ , (8) whereas the inﬂuence of the deformation is weaker for the ranges ijkl k lj ∂t 2 of short wavelengths. The effect of deformation is found to be −1 −1 where A = J A F F and ρ = J ρ is the density of the more pronounced in FCs with moderate and large shear modu- iqkp 0ijkl pl qj 0 deformed material. lus contrasts between the phases and with large volume fractions We seek a solution for Eq. (8) in the form of plane waves with of ﬁbers. Finally, we compare the micromechanics based homog- constant polarization enization technique and the numerical Bloch wave analysis, thus, bringing together the different length-scale analyses, and showing u = g h (n · x − ct ) , (9) the equivalence of these distinct approaches at certain ranges of where h is a twice continuously differentiable function and unit wavelengths. vector g denotes the polarization; the unit vector n deﬁnes the direction of wave propagation, and c is the phase velocity of the 2. Theoretical background wave. Substituting (9) into (8) , we obtain Consider a continuum body and identify each point in the un- deformed conﬁguration with its vector X . In the deformed body, Q (n ) · g = ρc 2g , (10) 296 P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304

T where I 4 = m · C¯ · m , and C¯ = F¯ · F¯ is the average right Cauchy- Green deformation tensor; + μ + μ 1 v f f vm m μ = μ + μ μ = μ ¯ v f f vm m and ˜ m (20) μ + + μ vm f 1 v f m are the homogenized elastic moduli. The acoustic tensor (14) corresponding to the strain energy function (19) takes the form

Qˆ (n , F¯ ) = q 1 ˆI + q 2 ˆI · F¯ · m ˆI · F¯ · m , (21) where − / 2 = μ · ¯ · + ( μ − μ ) − 3 2 · ¯ · q1 ˜ n B n ¯ ˜ 1 I4 n F m (22) and Fig. 1. Schematic representation of the FC with random distribution of ﬁbers. (e1, −5 / 2 2 = ( μ − μ ) · ¯ · , e2 , e3 ) is the orthonormal basis. q2 3I4 ¯ ˜ n F m (23) where B¯ = F¯ · F¯ T is the average left Cauchy–Green deformation ten- where sor. The acoustic tensor (21) has the following nontrivial eigenval- ues with the eigenvectors lying in the plane normal to n Q = A n n (11) ij ijkl j l 2 is the acoustic tensor deﬁning the condition of propagation of the a 1 = q 1 and a 2 = q 1 + q 2 I 4 − n · F¯ · m . (24) inﬁnitesimal plane waves. For incompressible materials Eq. (8) modiﬁes as Thus, we have two distinct shear waves propagating in a ﬁnitely 2 deformed incompressible FC with the corresponding phase veloci- ∂ u A + = ρ i , ijkl uk,lj p˙ ,i (12) ties ∂t 2 ( ) a ( ) a together with the incompressibility constraint 1 = 1 2 = 2 , c¯sw and c¯sw (25) ρ¯0 ρ¯0 u i,i = 0 . (13) = ( · − ) , where ρ¯ = v ρ + v m ρ is the average initial density of the FC. Substitution of (9) and p˙ p0 h n x ct where p0 is a scalar, 0 f 0 f 0m into (12) and (13) yields The phase velocities of the shear waves (25) coincide only for

special cases of applied deformations and directions of wave prop- ˆ ( ) · = ρ 2 · = , Q n g c g and g n 0 (14) agation. For instance, let us consider a uniaxially deformed FC with where Qˆ = ˆI · Q · ˆI and ˆI = I − n n is the projection onto the plane the corresponding macroscopic deformation gradient normal to n . −1 / 2 F¯ = λe 2 e 2 + λ ( I − e 2 e 2 ), (26) Next, let us consider a FC made out of aligned ﬁbers embedded = − λ in a softer matrix with the volume fractions vf and vm 1 v f . where is the applied macroscopic stretch ratio. Then, for waves Here and thereafter, the ﬁelds and parameters of the constituents propagating perpendicular to the ﬁbers, i.e. m = e 2 and n = e 1 , the • • are denoted by the subscripts ( )f and ( )m for ﬁbers and matrix, phase velocities of the shear waves coincide respectively. In the reference conﬁguration the volume fractions of ( ) ( ) μ˜ the phases can be calculated as = 1 = 2 = . c¯sw c¯sw c¯sw (27) λρ¯0 = / η = / − η , v f 1 f ( X)d X and vm 1 1 f ( X) dX (15) The phase velocities also coincide for the waves propagating along η = η = the ﬁbers, i.e. n = m = e , where f 1 if X is within the ﬁber phase and f 0 otherwise; 2 is the volume occupied by the composite in the reference state. − ( ) ( ) μ¯ + ( μ˜ − μ¯ ) λ 3 = 1 = 2 = λ . The macroscopic deformation gradient is deﬁned as c¯sw c¯sw c¯sw (28) ρ¯0 ¯ = / ( ) . F 1 F X dX (16) However, for an oblique propagation of the waves relative√ to the ﬁber direction, for example, m = e 2 and n = ( e 1 + e 2 )/ 2, the The boundary conditions for F and F m , and for P and P m at the f f phase velocities of the shear waves are distinct interfaces between the ﬁbers and matrix are F − F · m = 0 and P − P · w = 0 , (17) μ + λ3 − μ f m f m ( ) 2 ˜ 1 ¯ 1 = = c¯sw ( g e3 ) (29) where the unit vector m denotes the initial ﬁber directions (see 2 λρ¯0 Fig. 1 ), and w is the arbitrary unit vector orthogonal to m . and In this work, we consider ﬁber-reinforced materials with incom- pressible phases described by a neo-Hookean strain energy func- μ + μ + λ3 √ ( ) ˜ ¯ 1 2 tion (Ogden, 1997) 2 = = − / . c¯sw g ( e2 e1 ) 2 (30) μ 4 λρ¯0 inc ξ ψ ξ = (F ξ : F ξ − 3) , (18) 2 Note that (28) yields an explicit expression for the critical stretch where μξ is the initial shear modulus. For a FC with incompress- ratio corresponding to the onset of macroscopic instability under ible neo-Hookean phases, an effective strain energy density func- uniaxial contraction ( Rudykh and deBotton, 2012 ), namely tion can be constructed ( deBotton et al., 2006 ) 1 / 3 μ μ μ − μ ˜ ˜ ¯ ˜ −1 / 2 λ = 1 − . (31) ψ( F¯ ) = F¯ : F¯ − 3 + I + 2 I − 3 , (19) cr μ 2 2 4 4 ¯ P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304 297

a b

= . , μ /μ = , ρ /ρ = Fig. 2. Slowness curves for the out-of-plane (a) and in-plane (b) shear waves propagating in the FC with v f 0 2 f m 10 and 0 f 0 m 1 under uniaxial tension (26). Scale is 0.4 per division, and slowness is normalized by μ˜ / ρ¯0 . Note that the horizontal and vertical axes with the corresponding labels n 1 /c and n 2 /c serve for showing the principal directions and physical quantity presented on the polar plot only.

To illustrate the inﬂuence of the deformation and direction of the directions of the principal axes. For example, in the uniaxially wave propagation on the characteristics of elastic waves in the stretched FC the phase velocity of the out-of-plane shear wave is = = ± FCs, we consider wave propagation in the plane e1 , e2 , i.e. n maximal for the wave propagation along the ﬁbers, i.e. for n e2 cos ϕ e 1 + sin ϕ e 2 . By the use of the explicit relations (25) we (see Fig. 2 (a)). construct the polar diagrams of slowness s¯ sw (ϕ) = 1 / c¯ sw (ϕ) , also The dispersion relations for the long waves in an incompress- known in literature as slowness curves ( Musgrave, 1970; Nayfeh, ible neo-Hookean FC are derived from (25) and have the following 1995 ). Fig. 2 shows an example of the slowness curves for the so- form called out-of-plane (with polarization g = e 3 ) and in-plane (with ( ) b ( ) b ω 1 = 1 ω 2 = 2 polarization lying in plane e1 , e2 ) shear waves in the FC under- ¯ sw and ¯ sw (33) ρ¯ ρ¯ going uniaxial tension along the ﬁbers. The examples are given for 0 0 = . , μ /μ = , = the FC with v f 0 2 f m 10 and the ﬁber direction m e2 . where The continuous black curves correspond to the undeformed FC, −3 / 2 2 b 1 = μ˜ (k · B¯ · k ) + ( μ¯ − μ˜ ) 1 − I k · F¯ · m (34) while the dash-dotted green and dotted blue curves are for the FC 4 λ = . λ = . and under the uniaxial contraction ( 0 85) and extension ( 1 5), − / 2 − 2 respectively. Note that the critical stretch ratio for the consid- = + 5 2( μ − μ ) · ¯ · − 2 · ¯ · , b2 b1 3I4 ¯ ˜ k F m I4 k k F m (35) ered FC undergoing uniaxial contraction is λcr = 0 . 80 ; therefore, the presented slowness curves for the compressed ( λ = 0 . 85 ) FC where k is the wave vector and k = | k | is the wave number. correspond to a macroscopically stable state. The slowness curves Hence, we can ﬁnd the corresponding group velocity deﬁned as clearly indicate the signiﬁcant inﬂuence of the applied deforma- = ∇ ω. tion on the shear wave propagation. Speciﬁcally, the contraction vg k (36) along the ﬁbers results in a signiﬁcant decrease of the phase ve- Substitution of (33) into (36) yields explicit expressions for the locities of the shear waves propagating in the direction of ﬁbers; group velocities of the long waves propagating in the ﬁnitely de- while the phase velocities increase for the waves propagating per- formed FC pendicular to the ﬁbers since these directions experience exten- − / μ ¯ · + ( μ − μ ) − 3 2 · ¯ · ¯ · sion. Note that the phase velocity of the in-plane shear wave in ( 1 ) ˜ B n ¯ ˜ 1 I4 n F m F m v = (37) the uniaxially deformed FC is maximal for certain directions of sw ρ¯0 a 1 wave propagation n0 . To ﬁnd these directions, we substitute (26),

= ϕ + ϕ , = and n0 cos 0 e1 sin 0 e2 and m e2 into (25)2 , and then solve (2) ( ) 1 the extreme value problem for the phase velocity c¯ as a func- 2 = μ ¯ · + sw vsw ˜ B n ϕ ρ tion of 0 : ¯0 a2 −5 / 2 3 ( μ − μ ) · ¯ · · ¯ · + (38) − λ3 ¯ ˜ n F m 3I4 n F m n 1 1 ϕ = ± arccos + πz, z = 0 , 1 . (32) 0 μ − / − 2 2 3 1 − ˜ + 3 2 − 1 · ¯ · ¯ · . μ¯ 1 2I4 1 3I4 n F m F m π π ϕ = ± , ± 3 In the undeformed state 0 4 4 . Moreover, these directions In particular, the group velocities of the shear waves coincide for differ from the principal directions in contrast to the out-of-plane waves propagating perpendicular to the ﬁbers (i.e. m = e 2 and n = shear wave –the phase velocity of which has the maxima in e 1 ) in the uniaxially deformed FC 298 P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304

abn2v n2v

n1v n1v

= . , μ /μ = , ρ /ρ = Fig. 3. Energy curves for (a) – out-of-plane and (b) – in-plane shear waves propagating in the FC with v f 0 2 f m 10 and 0 f 0 m 1 under uniaxial tension. Scale is 0.4 per division, where group velocity is normalized by ρ¯0 / μ˜ . Note that the horizontal and vertical axes with the corresponding labels (n 1 v) and (n 2 v) serve for showing the principal directions and physical quantity presented on the polar plot only.

Next, let us consider slowness and energy curves near to, and ( ) ( ) μ˜ 1 = 2 = . vsw vsw e1 (39) at the onset of instability point. Fig. 4 shows the slowness curves λρ¯ 0 of the shear waves propagating in the FC subjected to the uniax- λ = . λ = . The group velocities also coincide for the waves propagating along ial contraction of 0 81 (dash-dotted green) and 0 80 (dot- ted red), while λcr = 0 . 80 . A comparison of Figs. 2 and 4 shows the ﬁbers, i.e. n = m = e 2 ,

that the slowness of both shear waves propagating along the ﬁbers − dramatically increases (or phase velocity decreases) when the crit- ( ) ( ) μ¯ + ( μ˜ − μ¯ ) λ 3 1 = 2 = λ . vsw vsw e2 (40) ical stretch is approached. In particular, in the FC contracted to λ = ρ¯ 0 0 . 81 , the slownesses of shear waves propagating in the direction of To illustrate the derived results (37) and (38), we consider wave ﬁbers are 3.8 times larger than in the undeformed FC. Eventually, = ϕ + ϕ the slownesses tend to inﬁnity in the FC contracted to the critical propagation in the plane e1 , e2 , i.e. n cos e1 sin e2 . Re- λ = . call that the outer normal to the slowness curve shows the di- stretch ratio, i.e. at 0 80. This is due to the fact that the phase rection of the energy ﬂow ( Musgrave, 1970; Nayfeh, 1995 ). Hence, velocities of the shear waves propagating along the ﬁbers attain zero value in the FC subjected to λ = λ (see (28) ). Lastly, Fig. 5 by assigning the absolute value of the group velocity (i.e. | v sw |) cr to the normal to the slowness curve for all possible propaga- shows the energy curves of the shear waves propagating in the FC λ = . tion directions, the polar diagrams of group velocity or the en- subjected to the uniaxial contraction of 0 81 ((a) and (b)) and λ = . ergy curves ( Musgrave, 1970; Nayfeh, 1995 ) are constructed. Fig. 3 0 80 ((c) and (d)). We observe that the energy curve of the λ shows an example of the energy curves for (a) out-of-plane and out-of-plane shear wave for the FC subjected to cr degenerates (b) in-plane shear waves propagating in the uniaxially deformed into the three dots (see Fig. 5 (c)). The dot in the center means that = . , μ /μ = , ρ /ρ = the absolute value of the group velocity is zero for the wave prop- FC with v f 0 2 f m 10 and 0 f 0 m 1. The continuous black curves correspond to the undeformed FC while the dash- agating in direction of ﬁbers (see (40) ); the other two dots mean dotted green and dotted blue curves refer to the uniaxial contrac- that the absolute value and direction of the group velocity do not tion ( λ = 0 . 85 ) and extension ( λ = 1 . 5 ), respectively. Clearly, the change with the wave propagation direction. For the in-plane shear group velocities of the shear waves strongly depend on the applied wave, the energy curve degenerates into the dot and two curved deformation and direction of wave propagation. Moreover, the en- triangles (see Fig. 5 (d)). The dot in the center corresponds to the ergy curve of the in-plane shear wave has intersections, and their zero group velocity of the wave propagating along the ﬁbers, while position can be manipulated by deformation (see Fig. 3 (b)). These the curved triangles refer to the curvature of the corresponding intersections of the energy curves mean that the absolute values slowness curve (see Fig. 4 (b)) in the vicinity of the wave prop- = ± and directions of group velocity coincide for two different direc- agation directions perpendicular to the ﬁbers (i.e. n e1 ). tions of wave propagation. For the out-of-plane shear wave the in- tersections are not observed (see Fig. 3 (a)). It is worth mention- 4. Bloch wave analysis for wave propagation in 3D periodic FCs ing also that the energy curves of plane waves coincide with the wave fronts of impulsive point source excited waves in homoge- To obtain the dispersion relations for ﬁnitely deformed 3D pe- neous anisotropic materials ( Langenberg et al., 2010; Nayfeh, 1995 ). riodic FCs, we employ the Bloch wave analysis superimposed on In this case, these cusps of energy curves will correspond to the a ﬁnite deformation ( Aberg and Gudmundson, 1997; Bertoldi and regions of null energy ( Nayfeh, 1995 ). Boyce, 20 08b; 20 08a; Rudykh and Boyce, 2014b ). We implement P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304 299 ab

= . , μ /μ = , ρ /ρ = Fig. 4. Slowness curves for the out-of-plane (a) and in-plane (b) shear waves propagating in the FC with v f 0 2 f m 10 and 0 f 0 m 1 under uniaxial ten- sion (26) near the instability. Scale is 0.5 per division, and slowness is normalized by μ˜ / ρ¯0 . the analysis in the ﬁnite element code. Fig. 6 shows an example where R deﬁnes the distance between the nodes on the oppo- of the corresponding representative volume element (RVE) for a FC site faces of the RVE in the reference conﬁguration. The periodicity with a square periodic unit cell. Geometrically, the ﬁbers are char- conditions (45) are imposed in the ﬁnite element code through the = /π, acterized by their diameters, namely d 2a v f where a is the corresponding boundary conditions for the displacements of the period of the FC (see Fig. 6 ). The periodic unit cell occupies a do- opposite faces ( Slesarenko and Rudykh, 2017; Bertoldi and Boyce, main in the undeformed conﬁguration, namely 20 08a; 20 08b; Wang and Bertoldi, 2012 ). The dispersion relations

− / ≤ ≤ / , − / ≤ ≤ / , are obtained by solving the eigenvalue problem stemming from a 2 x1 a 2 h 2 x2 h 2 (41) Eqs. (43) –(45) for a range of the wave vectors K 0. − / ≤ ≤ / . and a 2 x3 a 2 We start from comparing the results of the Bloch wave numer- ical analysis and the analytical estimates (33) for the long wave First, a solution for a ﬁnitely deformed state is obtained.

The macroscopic deformation gradient F¯ = 1 / F dV is applied limit. Fig. 7 presents the comparisons for the wave propagating through periodic boundary conditions imposed on the displace- in the direction of ﬁbers. The FCs are subjected to the uniaxial λ = . ments of the RVE faces such that tension (26) along the ﬁber direction of the magnitude 1 25. Fig. 7 (a) and (b) show the comparison for FCs with v = 0 . 25 , U − U = F¯ − I · ( X − X ) = H¯ · ( X − X ), (42) f B A B A B A μ /μ = μ /μ = , f m 10 and f m 1000 respectively; while Fig. 7 (c) and where A and B are the nodes on the opposite faces of the RVE = . , μ /μ = (d) show the comparison for FCs with v f 0 01 f m 10 and boundary, H¯ is the average displacement gradient tensor, and U = μ /μ = , f m 1000 respectively. The continuous black curves refer to − x ( X ) X is the displacement ﬁeld. The macroscopic ﬁrst Piola– the numerical simulations while the dashed red curves correspond

Kirchhoff stress tensor and the corresponding Cauchy stress tensor to the long wave estimates (33) . Here and thereafter, we consider ¯ = / σ = / σ , are calculated as P 1 PdV and ¯ 1 dV respectively. FCs with constituents having identical densities (i.e. ρ /ρ = 1 ), 0 f 0m Rigid body motions are prevented by ﬁxing the displacements of and frequency is normalized as f = fa ρ¯ / μ˜ , where f = ω/ ( 2 π ). a single node. Although the analysis is general and it can be ap- n 0 Fig. 7 (a) and (c) show that the long wave estimates are in excel- plied for materials subjected to any macroscopically applied homo- lent agreement with the results of numerical simulations up to the geneous deformation F¯, here the examples are given for a uniaxial wavelengths comparable with the period a of the unit cell for FCs loading (26) . possessing a small amount of ﬁbers and a moderate contrast in Second, the Bloch wave analysis is performed for the ﬁnitely the shear modulus between the constituents. However, for larger deformed state. The corresponding incremental change in the dis- contrasts in the shear moduli, the long wave estimates are in good placement and the ﬁrst Piola–Kirchhoff stress tensor can be ex- agreement with the Bloch wave analysis only for wavelengths sig- pressed as niﬁcantly exceeding the period of the unit cell, namely l ࣡ π 2 a −iωt −iωt u ( X , t ) = κ˙ ( X )e and P˙ = P˙ e , (43) (see Fig. 7 (b) and (d)). Thus, the difference between the long wave where ω is the angular frequency. By substitution (43) in (5) , we estimates (33) and Bloch wave analysis increases with an increase obtain in the volume fraction and shear modulus of ﬁbers (i.e. the role of

2 the ﬁbers becomes more signiﬁcant). DivP ˙ + ρ ω κ˙ = 0 . (44) 0 Fig. 8 presents the dispersion curves for the periodic FCs

According to the Floquet theorem (Kittel, 2004) with v = 0 . 25 and (a) μ /μm = 10 , (b) μ /μm = 100 , and (c) f f f −i K 0·R μ /μ = κ˙ ( X + R ) = κ˙ ( X )e , (45) f m 1000 undergoing uniaxial deformations along the ﬁbers. 300 P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304 a Out-of-plane shear waveb In-plane shear wave

c d

= . , μ /μ = , ρ /ρ = Fig. 5. Energy curves for the out-of-plane (a, c) and in-plane (b, d) shear waves propagating in the FC with v f 0 2 f m 10 and 0 f 0 m 1 under uniaxial ten- sion (26) near the instability. Scale is 0.3 per division, and group velocity is normalized by ρ¯0 / μ˜ .

The dispersion curves presented in Fig. 8 (and also in Fig. 9 ) are obtained by utilizing the Bloch wave analysis implemented in the ﬁnite element code. Clearly, for the FC with the low shear mod- μ /μ = ulus contrast between the ﬁbers and matrix (e.g., f m 10), the deformation slightly inﬂuences dispersion curves ( Fig. 8 (a)). However, the inﬂuence of deformation increases for the FCs with μ /μ = moderate and high shear modulus contrasts (e.g., f m 100 μ /μ = and f m 1000). Speciﬁcally, deformation considerably inﬂu- ences the dispersion of the waves with wavelengths exceeding the characteristic length-scale of the FC ( Fig. 8 (b) and (c)). For exam- ple, for the wavenumber ka/ (2 π ) = 0 . 2 , the uniaxial tension of the magnitude λ = 1 . 5 shifts the dispersion curve from f = 0 . 29 up to Fig. 6. RVE for a 3D periodic FC with a square arrangement of ﬁbers. n P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304 301

Fig. 7. Comparison of the long wave estimates (33) and the Bloch wave numerical analysis for the shear waves propagating in the direction of ﬁbers. Periodic FCs with = . μ /μ = , μ /μ = , = . μ /μ = , μ /μ = v f 0 25 and (a) f m 10 (b) f m 10 00 and v f 0 01 and (c) f m 10 (d) f m 1000 are subjected to the uniaxial tension along the ﬁber direction,

λ = . = ωa ρ / μ 1 25. Frequency is normalized as fn 2 π ¯0 ˜ .

= . μ /μ = , μ /μ = , μ /μ = Fig. 8. Dispersion curves for the shear waves propagating in the direction of ﬁbers in FCs with v f 0 25 and (a) f m 10 (b) f m 100 and (c) f m 1000. The FCs are subjected to the uniaxial tension of the magnitude λ = 0 . 98 (dashed green curves), λ = 1 (continuous black curves), λ = 1 . 5 (dotted blue curves), and λ = 2

= ωa ρ / μ (dash-dotted red curves). Frequency is normalized as fn 2 π ¯0 ˜ . (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.) 302 P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304

μ /μ = Fig. 9. Dispersion curves for shear waves propagating in the direction of ﬁbers in FCs with f m 1000 in the undeformed state (a) and for the FCs subjected to the uniaxial tension of magnitude λ = 1 . 5 (b) and λ = 2 (c).

f n = 0 . 55 as compared to the response of the undeformed FC with = . μ /μ = v f 0 25 and f m 100 (Fig. 8 (b)). Remarkably, the dispersion curves for the short waves (i.e. l ࣠ 2 a ) are barely affected by the uniaxial deformation ( Fig. 8 (b) and (c)). Moreover, the dispersion curves change more slowly with deformation after a certain level of stretch is reached (compare dash-dotted red and dotted blue curves in Fig. 8 ). This happens because the phase velocities (28) of the long shear waves start to change slowly when a certain level of deformation is achieved. To clarify the inﬂuence of the deformation on the dispersion phenomenon in FCs with various volume fractions of the ﬁbers, μ /μ = we present dispersion curves for FCs with f m 1000 in the undeformed state (a) and for the FCs subjected to the uniaxial ten- sion of magnitude λ = 1 . 5 (b) and λ = 2 (c) in Fig. 9 . The con- tinuous black, dotted blue, and dashed-dotted red curves corre- Fig. 10. RVE for a 3D periodic FC with a rectangular arrangement of ﬁbers. = . , = . , = . , spond to v f 0 01 v f 0 10 and v f 0 25 respectively. We ob- serve that the dispersion of shear waves in the ﬁber direction is more pronounced for the periodic FCs with large volume fractions of ﬁbers (compare continuous black and dash-dotted red curves in Fig. 9 (a)). Moreover, a uniaxial extension of the periodic FCs along the ﬁbers signiﬁcantly affects dispersion curves ( Fig. 9 (b) and (c)); however, an increase in the loading leads to a moderate change in the dispersion curve after a certain level of deformation (com- pare Fig. 9 (b) and (c)). For example, the frequency of the shear / ( π ) = . = . wave with ka 2 0 1 propagating in the FC with v f 0 25 and μ /μ = = . f m 1000 increases from fn 0 21 in the undeformed FC up to f n = 0 . 64 in the FC subjected to the uniaxial tension of the mag- nitude λ = 1 . 5 while it increases only up to f n = 0 . 66 in the FC subjected to the uniaxial tension of the magnitude λ = 2 (compare dash-dotted red curves in Fig. 9 ). This is due to the fact that the phase velocities (28) of long shear waves change more slowly after a certain level of deformation is reached. Finally, we consider the inﬂuence of the ﬁber arrangement on the shear wave propagation in the direction of ﬁbers. Fig. 10 shows an example of RVE for a FC with a rectangular periodic unit cell. Geometrically, the ﬁbers are characterized by their diameters, = /π namely d 2 abv f (see Fig. 10). The periodic unit cell occupies a domain in the undeformed conﬁguration, namely Fig. 11. Dispersion curves for shear waves propagating in the direction of ﬁbers = . μ /μ = in FCs with v f 0 25 and f m 100 in the undeformed state with square and rectangular ( b = 2 a ) arrangements of ﬁbers. −a/ 2 ≤ x 1 ≤ a/ 2 , − h/ 2 ≤ x 2 ≤ h/ 2 , (46) and − b/ 2 ≤ x 3 ≤ b/ 2 .

= . Fig. 11 presents a comparison of the dispersion curves for shear pare FCs with the same volume fractions of ﬁbers (i.e. v f 0 25); waves propagating along the ﬁbers in the FC with the square as a result, the dispersion curves of the long shear waves (i.e. and rectangular ( b = 2 a ) arrangements of the ﬁbers. The dispersion l 5(a + b) / 2 ) coincide for both square and rectangular periodic curves of the shear waves vary in the FC with rectangular arrange- FCs. Consistently with the previous observations, a signiﬁcant non- ment of ﬁbers, because we have two distinct characteristic lengths, linearity of dispersion curves is observed for the shear waves with namely a and b , as opposite to the square arrangement. We com- wavelengths being comparable to the characteristic lengths of the P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304 303

FC, namely l ∼ (a + b) . The dispersion curves for shorter waves (i.e. waves with wavelengths being comparable to the characteristic l (a + b) / 3 ) are affected only slightly by the ﬁber arrangement. lengths of the FC are signiﬁcantly affected by the ﬁber arrange- ment, and (iii) short shear waves are affected only slightly by the 5. Concluding remarks ﬁber arrangement.

We considered the shear wave propagation in the 3D ﬁber- Acknowledgments reinforced composites undergoing ﬁnite deformations. First, we derived the explicit closed form expressions for the phase and This work was supported by the Israel Science Foundation group velocities of the shear waves propagating in the ﬁnitely de- (grant №1550/15 and 1973/15 ). Stephan Rudykh gratefully acknowl- formed 3D FCs on the basis of a micromechanical approach ac- edges the support of Taub Foundation through the Horev Fellow- counting for the material properties and distribution of the phases. ship –Leaders in Science and Technology. Viacheslav Slesarenko Hence, the derived explicit relations for the phase and group ve- thanks the support through the Technion Postdoctoral Fellowship. locities were expressed in terms of the actual mechanical prop- erties of composite constituents and their volume fractions. By utilizing these expressions, we constructed the slowness and en- References ergy curves revealing the strong inﬂuence of deformation on the Aberg, M. , Gudmundson, P. , 1997. The usage of standard ﬁnite element codes for propagation of shear waves. In particular, the shear wave veloc- computation of dispersion relations in materials with periodic microstructure. J. ities were shown to vary considerably with the deformation and Acoust. Soc. Am. 102, 2007–2013 . direction of wave propagation. Moreover, the energy curve of the Babaee, S. , Shim, J. , Weaver, J. , Chen, E. , Patel, N. , Bertoldi, K. , 2013. 3D soft meta- materials with negative poisson’s ratio. Adv. Mater. 25 (36), 5044–5049 . in-plane shear wave was shown to have deformation tunable in- Babaee, S. , Viard, N. , Wang, P. , Fang, N.X. , Bertoldi, K. , 2016. Harnessing deformation tersections, meaning that the absolute values and directions of the to switch on and off the propagation of sound. Adv. Mater. 28 (8), 1631–1635 . group velocities coincide for the different directions of wave prop- Bafekrpour, E. , Molotnikov, A. , Weaver, J.C. , Brechet, Y. , Estrin, Y. , 2014. Responsive

materials: a novel design for enhanced machine-augmented composites. Sci. agation. Thus, we are able to estimate characteristics of wave and Rep. 4, 5801–5821 . energy propagation in the ﬁnitely deformed 3D ﬁber composites Bertoldi, K. , Boyce, M.C. , 2008a. Mechanically triggered transformations of phononic employing these explicit relations, which are applicable for any di- band gaps in periodic elastomeric structures. Phys. Rev. B 77 (5), 052105 . rection of wave propagation and for any macroscopically applied Bertoldi, K., Boyce, M.C., 2008b. Wave propagation and instabilities in monolithic and periodically structured elastomeric materials undergoing large deforma- homogeneous pre-deformation. These important characteristics are tions. Phys. Rev. B 78, 184107 . expressed in terms of the actual microstructure parameters, such Bertoldi, K. , Boyce, M.C. , Deschanel, S. , Prange, S. , Mullin, T. , 2008. Mechanics of as volume fractions and phase material properties. This impor- deformation-triggered pattern transformations and superelastic behavior in pe- riodic elastomeric structures. J. Mech. Phys. Solids 56 (8), 2642–2668 . tant feature distinguishes our results from those derived from phe- Biot, M.A. , 1939. Non Linear Theory of Elasticity and the linearized case for a body nomenological models, where the material parameters need to be under initial stress. Philos. Mag. XXVII, 46 8–4 89 . ﬁtted, and they are not directly related to the microstructure pa- Biot, M.A. , 1940. The inﬂuence of initial stress on elastic waves. J. Appl. Phys. 11 (8), 522 . rameters and material properties of the constituents. Boulanger, P. , Hayes, M. , 1992. Finite-amplitude waves in deformed mooney-rivlin Second, we examined the shear wave propagation in the ﬁnitely materials. Q. J. Mech. Appl. Math. 45 (4), 575–593 . deformed 3D periodic FCs by application of the Bloch wave ap- Boulanger, P. , Hayes, M. , Trimarco, C. , 1994. Finite-amplitude plane waves in de- formed hadamard elastic materials. Geophys. J. Int. 118 (2), 447–458 . proach in the ﬁnite element code. This allowed us to account for Celli, P. , Gonella, S. , 2015. Manipulating waves with LEGO® bricks: a versatile exper- the interactions of the elastic waves with the material microstruc- imental platform for metamaterial architectures. Appl. Phys. Lett. 107, 081901 . ture. As a result, we found the dispersion phenomenon manifesting Chen, Q. , Elbanna, A. , 2016. Modulating elastic band gap structure in layered soft

composites using sacriﬁcial interfaces. J. Appl. Mech. 83, 1110 09. in the strongly nonlinear dependence of the wave frequencies on Currie, P. , Hayes, M. , 1969. Longitudinal and transverse waves in ﬁnite elastic strain. wavenumber. The dispersion and the corresponding wavelengths hadamard and green materials. IMA J. Appl. Math. 5 (2), 140–161 . of the shear waves in the 3D periodic FCs were found to be tun- deBotton, G. , Hariton, I. , Socolsky, E.A. , 2006. Neo-Hookean ﬁber-reinforced compos- able by the change in the shear modulus contrast between the ites in ﬁnite elasticity. J. Mech. Phys. Solids 54, 533–559. Destrade, M. , Ogden, R.W. , 2013. On stress-dependent elastic moduli and wave constituents and volume fraction of the ﬁbers. Speciﬁcally, an in- speeds. J. Appl. Math. 78 (5), 965–997 . crease in the shear modulus contrast and amount of ﬁbers leads Dorfmann, A. , Ogden, R.W. , 2010. Electroelastic waves in a ﬁnitely deformed elec- to a more pronounced dispersion of shear waves propagating in troactive material. IMA J. Appl. Math. 75 (4), 603–636. Fomenko, S.I. , Golub, M.V. , Zhang, C. , Bui, T.Q. , Wang, Y.-S. , 2014. In-plane elastic the direction of ﬁbers, i.e. the dispersion curves exhibit a signiﬁ- wave propagation and band-gaps in layered functionally graded phononic crys- cant nonlinearity. Moreover, the dispersion of shear waves is highly tals. Int. J. Solids Struct. 51, 2491–2503 . sensitive to deformation. In particular, a moderate deformation sig- Galich, P.I. , Fang, N.X. , Boyce, M.C. , Rudykh, S. , 2017. Elastic wave propagation in ﬁnitely deformed layered materials. J. Mech. Phys. Solids 98, 390–410 . niﬁcantly increases the frequency of the long waves. However, the Galich, P.I. , Rudykh, S. , 2015a. Comment on “Disentangling longitudinal and shear inﬂuence of deformation for the short waves is relatively weak. We elastic waves by neo-Hookean soft devices”. Appl. Phys. Lett. 107, 056101 . 106, found that the inﬂuence of deformation on the dispersion of shear 161903. Galich, P.I. , Rudykh, S. , 2015b. Inﬂuence of stiffening on elastic wave propagation in waves is more pronounced at the beginning of the loading due extremely deformed soft matter: from nearly incompressible to auxetic materi- to the fact that the phase velocities (28) of the long shear waves als. Extreme Mech. Lett. 4, 156–161 . change quickly up to a certain level of deformation and then the Galich, P.I. , Rudykh, S. , 2016. Manipulating pressure and shear elastic waves in di-

electric elastomers via external electric stimuli. Int. J. Solids Struct. 91, 18–25. phase velocities vary slowly with a further loading. Next, we com- Ge, Q. , Qi, H.J. , Dunn, M.L. , 2013. Active materials by four-dimension printing. Appl. pared the results of the Bloch wave analysis and the long wave Phys. Lett. 103 (13), 131901 . estimates. We found that the long wave estimates for the phase Gei, M. , 2008. Elastic waves guided by a material interface. Eur. J. Mech. 27 (3), velocities (25) of shear waves accurately describe the dispersion 328–345. Golub, M.V. , Fomenko, S.I. , Bui, T.Q. , Zhang, C. , Wang, Y.-S. , 2012. Transmission and relations for the ﬁnitely deformed FCs with low shear modulus band gaps of elastic SH waves in functionally graded periodic laminates. Int. J. μ μ ࣠ contrast between the ﬁbers and matrix (i.e. f / m 10) and small Solids Struct. 49, 344–354. Humphrey, J.D. , 2002. Cardiovascular Solid Mechanics: Cells, Tissues, and Organs. volume fractions of the ﬁbers (i.e. v ࣠ 0.25). f Springer-Verlag, New York .

Finally, we analyzed the inﬂuence of the ﬁber arrangement on John, F. , 1966. Plane elastic waves of ﬁnite amplitude. hadamard materials and har- the propagation of shear waves along the ﬁbers. In particular, by monic materials. Commun. Pure Appl. Math. 19 (3), 309–341 . comparing dispersion curves of shear waves for FCs with square Kittel, C. , 2004. Introduction to Solid State Physics. Wiley, Hoboken, N.J . Kolle, M. , Lethbridge, A. , Kreysing, M. , Baumberg, J. , Aizenberg, J. , Vukusic, P. ,2013. and rectangular arrangements of ﬁbers, we observed that (i) long Bio-inspired band-gap tunable elastic optical multilayer ﬁbers. Adv. Mater. 25 shear waves are independent of the ﬁber arrangement, (ii) shear (15), 2239–2245 . 304 P.I. Galich et al. / International Journal of Solids and Structures 110–111 (2017) 294–304

Kushwaha, M. , Halevi, P. , Dobrzynski, L. , Djafari-Rouhani, B. , 1993. Acoustic band Rudykh, S. , deBotton, G. , 2012. Instabilities of hyperelastic ﬁber composites: mi- structure of periodic elastic composites. Phys. Rev. Lett. 71 (13), 2022–2025 . cromechanical versus numerical analyses. J. Elasticity 106, 123–147 . Langenberg, K.J. , Marklein, R. , Mayer, K. , 2010. Energy vs. group velocity for elastic Rudykh, S. , Ortiz, C. , Boyce, M. , 2015. Flexibility and protection by design: imbri- waves in homogeneous anisotropic solid media. In: Proceedings of 2010 URSI cated hybrid microstructures of bio-inspired armor. Soft Matter 11, 2547–2554 . International Symposium on Electromagnetic Theory, pp. 733–736 . Saheb, D.N. , Jog, J.P. , 1999. Natural ﬁber polymer composites: a review. Adv. Polym. Li, Y. , Kaynia, N. , Rudykh, S. , Boyce, M.C. , 2013. Wrinkling of interfacial layers in Technol. 18 (4), 351–363 . stratiﬁed composites. Adv. Eng. Mater. 15 (10), 921–926 . Scott, N. , 1991. Small vibrations of prestrained constrained elastic materials: the ide- Lin, E. , Li, Y. , Ortiz, C. , Boyce, M.C. , 2014. 3D printed, bio-inspired prototypes and alized ﬁbre-reinforced material. Int. J. Solids Struct. 27 (15), 1969–1980 . analytical models for structured suture interfaces with geometrically-tuned de- Scott, N. , 1992. Waves in a homogeneously prestrained incompressible, almost in- formation and failure behavior. J. Mech. Phys. Solids 73, 166–182 . extensible, ﬁbre-reinforced elastic material. Proc. R. Irish Acad. Sect. A 92A (1), Musgrave, M.J.P. , 1970. Crystal Acoustics: Introduction to the Study of Elastic Waves 9–36 . and Vibrations in Crystals. Holden-day, San Francisco . Scott, N. , Hayes, M. , 1976. Small vibrations of a ﬁbre-reinforced composite. Q. J. Nayfeh, A.H. , 1995. Wave Propagation in Layered Anisotropic Media: With Applica- Mech. Appl. Math. 29 (4), 467–486 . tions to Composites. Elsevier Science, Amsterdam . Slesarenko, V. , Rudykh, S. , 2016. Harnessing viscoelasticity and instabilities for tun- Ogden, R. , Singh, B. , 2011. Propagation of waves in an incompressible transversely ing wavy patterns in soft layered composites. Soft Matter 12, 3677–3682 . isotropic elastic solid with initial stress: biot revisited. J. Mech. Mater. Struct. 6 Slesarenko, V., Rudykh, S., 2017. Microscopic and macroscopic instabilities in hyper- (1–4), 453–477 . elastic ﬁber composites. J. Mech. Phys. Solids doi: 10.1016/j.jmps.2016.11.002 . Ogden, R.W. , 1997. Non-linear Elastic Deformations. Dover Publications, New York . Srivastava, A. , 2016. Metamaterial properties of periodic laminates. J. Mech. Phys. Rogerson, G. , Scott, N. , 1994. Doubly constrained elastic wave propagation. Int. J. Solids 96, 252–263 . Solids Struct. 31 (20), 2769–2792 . Truesdell, C. , Noll, W. , 1965. The Non-Linear Field Theories of Mechanics. Springer . Rudykh, S. , Boyce, M. , 2014a. Transforming small localized loading into large rota- Wang, L. , Bertoldi, K. , 2012. Mechanically tunable phononic band gaps in three- tional motion in soft anisotropically-structured materials. Adv. Eng. Mater. 16 -dimensional periodic elastomeric structures. Int. J. Solids Struct. 49 (19–20), (11), 1311–1317 . 2881–2885 . Rudykh, S. , Boyce, M. , 2014b. Transforming wave propagation in layered media via instability-induced interfacial wrinkling. Phys. Rev. Lett. 112, 034301 . International Journal of Solids and Structures 135 (2018) 303–304

Contents lists available at ScienceDirect

International Journal of Solids and Structures

journal homepage: www.elsevier.com/locate/ijsolstr

Corrigendum to “Shear wave propagation in ﬁnitely deformed 3D ﬁber-reinforced composites” [Int. J. Solids Struct. 110–111 (2017) 294–304]

∗ Pavel I. Galich, Viacheslav Slesarenko, Stephan Rudykh

Department of Aerospace Engineering, Technion –Israel Institute of Technology, Haifa 320 0 0, Israel

In our paper ( Galich et al., 2017 ), Figs. 7–9 show frequencies as functions of wavenumber K 0 (in the undeformed conﬁguration); thus, in Figs. 7–9, K 0 = | K 0 | must replace k = | k | (in the deformed conﬁguration). Recall that the corresponding wave vectors in the undeformed

Fig. 1. Comparison of the long wave estimates (33) and the Bloch wave numerical analysis for the shear waves propagating in the direction of ﬁbers. Periodic FCs with = . μ /μ = , μ /μ = , = . μ /μ = , μ /μ = v f 0 25 and (a) f m 10 (b) f m 10 00 and v f 0 01 and (c) f m 10 (d) f m 1000 are subjected to the uniaxial tension along the ﬁber direction,

λ = . = ωa ρ / μ 1 25. Frequency is normalized as fn 2 π ¯0 ˜ .

DOI of original article: 10.1016/j.ijsolstr.2016.12.007 ∗ Corresponding author. E-mail address: [email protected] (S. Rudykh). https://doi.org/10.1016/j.ijsolstr.2017.12.027 0020-7683 304 P.I. Galich et al. / International Journal of Solids and Structures 135 (2018) 303–304

= . μ /μ = , μ /μ = , μ /μ = Fig. 2. Dispersion curves for the shear waves propagating in the direction of ﬁbers in FCs with v f 0 25 and (a) f m 10 (b) f m 100 and (c) f m 1000. The FCs are subjected to the uniaxial tension of the magnitude λ = 0 . 98 (dashed green curves), λ = 1 (continuous black curves), λ = 1 . 5 (dotted blue curves), and λ = 2 (dash-dotted red curves). (For interpretation of the references to colour in this ﬁgure legend, the reader is referred to the web version of this article.)

μ /μ = Fig. 3. Dispersion curves for shear waves propagating in the direction of ﬁbers in FCs with f m 1000 in the undeformed state (a) and for the FCs subjected to the uniaxial tension of magnitude λ = 1 . 5 (b) and λ = 2 (c). and deformed conﬁgurations are related via K 0 = F T · k . Here, we present frequencies as functions of wavenumber k in the deformed conﬁguration. Figs. 1 –3 correspond to Figs. 7, 8 and 9, respectively, in the original paper ( Galich et al., 2017 ). Thus, the conclusion in Galich et al. (2017) about the weak inﬂuence of the applied deformation on short shear waves (with wavelength l ࣠ 2 a ) needs to be corrected. As can be seen from Fig. 2 , the applied uniaxial deformation inﬂuence shear waves in both long and short wave ranges. All other conclusions in Galich et al. (2017) agree with the dispersion curves presented in Figs. 1 –3 .

Reference

Galich, P.I. , Slesarenko, V. , Rudykh, S. , 2017. Shear wave propagation in ﬁnitely deformed 3D ﬁber-reinforced composites. Int. J. Solids Struct. 110–111, 294–304 . Chapter 4

Conclusions and discussion

By employing rigorous analytical methods of non-linear mechanics (see Section 2.1),

I derived long wave estimates for important characteristics of elastic waves – phase and group velocities – propagating in non-linear layered [19] and ﬁbrous [25] com- posites. Next, by combining Bloch-Floquet approach (see Section 2.2) and non- linear constitutive models for each layer, I derived closed-form dispersion relations for P- and S-waves propagating perpendicularly to the layers in the non-linear pe- riodic laminates and found that BGs (forbidden frequency ranges, where waves cannot propagate) can be initiated and shifted towards desirable low frequencies in non-linear elastic laminates by mechanical loading [19]. In parallel, I explored the inﬂuence of material stiffening on elastic wave propagation in the non-linear isotropic materials [21] and laminates [19] comprised of these materials. Then, I extended my analysis to the problem of wave propagation in non-linear electroe- lastic isotropic materials [22] and laminates [23] composed of these materials.

84 4.1 Inﬂuence of stiffening on elastic wave propagation

in extremely deformed soft matter: from nearly in-

compressible to auxetic materials

In this paper, I derived closed-form expressions for phase velocities of elastic waves propagating in the ﬁnitely deformed materials with pronounced stiffening effects.

I demonstrated that ﬁnite deformation can signiﬁcantly inﬂuence elastic waves in nearly incompressible, highly compressible and auxetic (with negative Poisson’s ratio) materials. Moreover, I studied inﬂuence of propagation direction on the phase velocities of elastic waves. I found that for nearly incompressible materi- als S-wave velocities exhibit strong dependence on the direction of propagation and pre-strain, whereas the P-wave velocity is barely affected until extreme lev- els of deformation are reached. For highly compressible materials, I showed that both P- and S-wave velocities signiﬁcantly depend on applied deformation and propagation direction. Furthermore, the dependence becomes stronger when the stiffening effects become more pronounced. My ﬁndings can help to design or bet- ter understand mechanics of deformation-tunable elastic metamaterials comprised of materials with strong stiffening effects.

85 4.2 Manipulating pressure and shear waves in dielec-

tric elastomers via external electric stimuli

In this manuscript, I considered P- and S- elastic waves propagating in ﬁnitely deformed DEs in the presence of an electric ﬁeld. To allow consideration of P- waves, I utilized the ideal and enriched material models accounting for the volu- metric changes. I derived closed-form expressions for the phase velocities of elastic waves propagating in DEs subjected to an electric ﬁeld. I found that, for the ideal

DE model, the elastic wave propagation is explicitly independent of an applied electric ﬁeld, while it can be inﬂuenced through the deformation induced via an electric ﬁeld. However, characteristics of elastic waves explicitly depend on the applied electric ﬁeld in case of the proposed enriched material model. Speciﬁcally, the phase velocity of the in-plane S-wave decreases upon application of an elec- tric ﬁeld. Then, I applied my ﬁndings to explore the phenomenon of disentangling

(decoupling) P- and S-waves in DEs by an electric ﬁeld (see Fig. 1 in [22]). I showed that the divergence angle between P- and S-waves strongly depends on the value of the applied electric ﬁeld and propagation direction. Moreover, I found that an increase in the material compressibility weakens the decoupling of P- and S-waves

(see Fig. 4 in [22]). This is because the P-wave refracts in the same direction as the

S-wave from the initial propagation direction, while for nearly incompressible ma- terials the change in the P-wave direction is negligible. The phenomenon can be used to manipulate elastic waves by a bias electrostatic ﬁeld, which can be beneﬁ- cial for small length-scale devices, such as micro-electromechanical systems, where an electric ﬁeld is the preferred control parameter.

86 4.3 Elastic wave propagation in ﬁnitely deformed lay-

ered materials

In this work, I studied elastic wave propagation in ﬁnitely deformed bi-laminates.

Firstly, based on an exact analytical solution for ﬁnitely deformed laminates with alternating neo-Hookean phases, I derived closed-form expressions for the phase and group velocities of S-waves propagating in any direction in these laminates.

Secondly, I obtained long wave estimates and for the phase velocities of P- and

S-waves propagating perpendicularly to the layers in the ﬁnitely deformed com- pressible bi-laminates with neo-Hookean and Gent layers. These estimates provide the important information on elastic wave propagation with wavelengths sufﬁ- ciently larger than period of the laminate, namely l & 3d. Thirdly, I performed a detailed analysis of the BG structures for the waves propagating perpendicularly to the layers in the incompressible and compressible laminates. Speciﬁcally, I iden- tiﬁed the key parameters and mechanisms inﬂuencing the S-wave, P-wave, and complete BGs and then revealed the advantageous compositions of the laminates having the wide BGs in the low-frequency range.

Finally, I rigorously showed that SBGs in laminates comprised of layers exhibit- ing weak stiffening effects (neo-Hookean) are independent of the applied defor- mation because deformation induced changes in geometry and effective material properties fully compensate each other. However, contraction or extension of the laminate made of layers with strong stiffening effects (e.g., Gent) widens and shifts

SBGs towards higher frequencies due to the stronger effect of deformation induced changes in the material properties (as compared to the geometry changes). Fur-

87 thermore, I found that laminates with thin highly compressible layers embedded in a nearly incompressible matrix possess wide complete BGs, and the dominant mechanism inﬂuencing PBGs is the deformation induced change in the thicknesses of the layers.

4.4 Shear wave propagation and band gaps in ﬁnitely

deformed dielectric elastomer laminates: long wave

estimates and exact solution

In this article, I investigated S-wave propagation in electroelastic bi-laminates sub- jected to ﬁnite deformations and electric ﬁelds. I obtained the long wave estimates

– the exact solution for the waves with wavelength sufﬁciently larger than period of the laminate – for phase and group velocities of S-waves propagating in the bi-laminates with electroelastic ideal (neo-Hookean) layers. The derived closed- form formulas are expressed in terms of the volume fractions and electroelastic constants of the layers. Moreover, these long wave estimates can be used for any direction of wave propagation, for any applied electric ﬁeld, and for any homoge- neous ﬁnite pre-deformations. Remarkably, the S-wave propagation perpendicu- lar to the layers depends on electric ﬁeld only though the induced deformation.

Next, I derived the dispersion relations for the S-waves propagating perpendic- ular to the layers in the laminates with incompressible hyperelastic ideal dielectric layers and general elastic part (that is function of the ﬁrst strain invariant only, e.g., neo-Hookean, Gent, Arruda-Boyce, Yeoh, to name a few). Consistently with

88 the exact solution for long waves, the derived dispersion relation is independent of electric ﬁeld, and it coincides with its analogue for the purely elastic laminates.

This dispersion relation shows that SBGs in the electroelastic laminates are tunable by an electric ﬁeld only through induced deformation. In particular, the applica- tion of an electric ﬁeld to the DE laminates with electroelastic Gent phases widens and shifts SBGs towards higher frequencies. However, SBGs are independent of deformation (either it is induced by electrical or mechanical stimuli) in DE lami- nates with electroelastic neo-Hookean layers.

4.5 Shear wave propagation in ﬁnitely deformed 3D

ﬁber-reinforced composites

In this paper, I considered the S-wave propagation in the ﬁnitely deformed 3D FCs.

Based on a micromechanical approach accounting for the constituent properties and their distribution in the composite, I derived the closed-form expressions for the phase and group velocities of the S-waves propagating in the ﬁnitely deformed

3D FCs. Hence, the expressions for the phase and group velocities are presented in terms of the actual mechanical properties of composite constituents and their volume fractions. Next, I constructed the slowness and energy curves revealing the signiﬁcant inﬂuence of deformation on the propagation of S-waves. In particular, the S-wave velocities were shown to vary considerably with the deformation and propagation direction. Moreover, the energy curve of the in-plane S-wave was shown to have deformation tunable intersections, meaning that the absolute values

89 and directions of the group velocities coincide for the different directions of wave propagation. Thus, characteristics of wave and energy propagation in the ﬁnitely deformed 3D FCs can be estimated via employing the derived relations, which are applicable for any direction of wave propagation and for any macroscopically applied homogeneous pre-deformation.

Finally, I examined the S-wave propagation in the ﬁnitely deformed 3D peri- odic FCs by application of the Bloch-Floquet approach in the ﬁnite element code

(see Section 2.2). This allowed me to account for the interactions of the S-waves with the composite microstructure, i.e. to calculate dispersion relations for S- waves propagating along ﬁbers. The dispersion and the corresponding wave- lengths of the S-waves in the 3D periodic FCs were found to be tunable by the change in the shear modulus contrast between the ﬁbers and matrix and volume fraction of the ﬁbers. Speciﬁcally, an increase in the shear modulus contrast and amount of ﬁbers leads to a more pronounced dispersion of S-waves propagating in the direction of ﬁbers, i.e. the dispersion curves exhibit a signiﬁcant nonlinear- ity (highly sensitive to pre-deformation). Additionally, I analyzed the inﬂuence of the ﬁber periodicity on the propagation of S-waves along the ﬁbers. In particular, by comparing dispersion curves of S-waves for FCs with square and rectangular arrays of ﬁbers, I observed that long S-waves are independent of the ﬁber distri- bution, while S-waves with wavelengths being comparable to the characteristic lengths of the FC are signiﬁcantly affected by the spacial distribution of ﬁbers.

90 Bibliography

[1] M. Aberg and P. Gudmundson. The usage of standard ﬁnite element codes for

computation of dispersion relations in materials with periodic microstructure.

J. Acoust. Soc. Am., 102:2007–2013, 1997.

[2] M. Agoras, O. Lopez-Pamies, and P. Ponte Castaneda.˜ Onset of macroscopic

instabilities in ﬁber-reinforced elastomers at ﬁnite strain. J. Mech. Phys. Solids,

57:1828–1850, 2009.

[3] K. Bertoldi and M. C. Boyce. Wave propagation and instabilities in monolithic

and periodically structured elastomeric materials undergoing large deforma-

tions. Phys. Rev. B, 78:184107, 2008.

[4] K. Bertoldi and M. Gei. Instabilities in multilayered soft dielectrics. J. Mech.

Phys. Solids, 59:18–42, 2011.

[5] M. A. Biot. The Inﬂuence of Initial Stress on Elastic Waves. J. Appl. Phys.,

11(8):522, 1940.

[6] P. Boulanger and M. Hayes. Finite-amplitude waves in deformed mooney-

rivlin materials. Q. J. Mech. Appl. Math., 45(4):575–593, 1992.

91 [7] P. Boulanger, M. Hayes, and C. Trimarco. Finite-amplitude plane waves in

deformed hadamard elastic materials. Geophys. J. Int., 118(2):447–458, 1994.

[8] B. Cantor, H. Assender, and P. Grant. Lightweight materials, chapter 9-16, pages

89–226. Taylor & Francis Group, Boca Raton, FL, 2001.

[9] Z. Chang, H.-Y. Guo, B. Li, and X.-Q. Feng. Disentangling longitudinal

and shear elastic waves by neo-Hookean soft devices. Appl. Phys. Lett.,

106(16):161903, 2015.

[10] N. Cohen, K. Dayal, and G. deBotton. Electroelasticity of polymer networks.

J. Mech. Phys. Solids, 92:105–126, 2016.

[11] G. deBotton, I. Hariton, and E. A. Socolsky. Neo-Hookean ﬁber-reinforced

composites in ﬁnite elasticity. J. Mech. Phys. Solids, 54:533–559, 2006.

[12] G. deBotton, L. Tevet-Deree, and E. A. Socolsky. Electroactive heterogeneous

polymers: analysis and applications to laminated composites. Mech. Adv.

Mater. Struct., 14:13–22, 2007.

[13] A. Demcenko, M. Mazilu, R. Wilson, A. W. F. Volker, and J. M. Cooper. Hy-

perelastic Tuning of One-Dimensional Phononic Band Gaps Using Directional

Stress. IEEE Transactions on Ultrasonics, Ferroelectrics, and Frequency Control,

65(6):1056–1061, 2018.

[14] A. Demcenko,ˇ R. Wilson, J. M. Cooper, M. Mazilu, and A. W. F. Volker.

Ultrasonic waves in uniaxially stressed multilayered and one-dimensional

92 phononic structures: Guided and Floquet wave analysis. J. Acoust. Soc. Am.,

144(1):81–91, 2018.

[15] M. Destrade and R. W. Ogden. On stress-dependent elastic moduli and wave

speeds. J. Appl. Math., 78(5):965–997, 2013.

[16] A. Dorfmann and R. W. Ogden. Nonlinear electroelasticity. Acta. Mech.,

174:167–183, 2005.

[17] A. Dorfmann and R. W. Ogden. Electroelastic waves in a ﬁnitely deformed

electroactive material. IMA J. Appl. Math., 75(4):604–636, 2010.

[18] L. Dorfmann and R. W. Ogden. Nonlinear Theory of Electroelastic and Magnetoe-

lastic Interactions, volume 9781461495. Springer US, Boston, MA, 2014.

[19] P. I. Galich, N. X. Fang, M. C. Boyce, and S. Rudykh. Elastic wave propagation

in ﬁnitely deformed layered materials. J. Mech. Phys. Solids, 98:390–410, 2017.

[20] P. I. Galich and S. Rudykh. Comment on ”Disentangling longitudinal and

shear elastic waves by neo-Hookean soft devices” [Appl. Phys. Lett. 106,

161903 (2015)]. Appl. Phys. Lett., 107:056101, 2015.

[21] P. I. Galich and S. Rudykh. Inﬂuence of stiffening on elastic wave propaga-

tion in extremely deformed soft matter: from nearly incompressible to auxetic

materials. Extreme Mech. Lett., 4:156–161, 2015.

[22] P. I. Galich and S. Rudykh. Manipulating pressure and shear elastic waves in

dielectric elastomers via external electric stimuli. Int. J. Solids Struct., 91:18–25,

2016.

93 [23] P. I. Galich and S. Rudykh. Shear Wave Propagation and Band Gaps in Finitely

Deformed Dielectric Elastomer Laminates: Long Wave Estimates and Exact

Solution. J. Appl. Mech., 84(9):091002, 2017.

[24] P. I. Galich, V. Slesarenko, J. Li, and S. Rudykh. Elastic instabilities and shear

waves in hyperelastic composites with various periodic ﬁber arrangements.

International Journal of Engineering Science, 130:51–61, 2018.

[25] P. I. Galich, V. Slesarenko, and S. Rudykh. Shear wave propagation in ﬁnitely

deformed 3D ﬁber-reinforced composites. Int. J. Solids Struct., 110-111:294–

304, 2017.

[26] M. Gei, S. Roccabianca, and M. Bacca. Controlling bandgap in electroactive

polymer-based structures. Mechatronics, IEEE/ASME Transactions, 16(1):102–

107, 2011.

[27] A. Goshkoderia and S. Rudykh. Electromechanical macroscopic instabilities

in soft dielectric elastomer composites with periodic microstructures. Eur. J.

Mech. - A/Solids, 65:243–256, 2017.

[28] M. Jandron and D. L. Henann. A numerical simulation capability for elec-

troelastic wave propagation in dielectric elastomer composites: Application

to tunable soft phononic crystals. International Journal of Solids and Structures,

In press, 2018.

[29] D. T. Kuhnel, J. M. Rossiter, and C. F. J. Faul. 3D printing with light: towards

additive manufacturing of soft, electroactive structures. In Y. Bar-Cohen, ed-

94 itor, Electroactive Polymer Actuators and Devices (EAPAD) XX, volume 10594,

page 34. SPIE, mar 2018.

[30] M. Kushwaha, P. Halevi, L. Dobrzynski, and B. Djafari-Rouhani. Acoustic

band structure of periodic elastic composites. Phys. Rev. Lett., 71(13):2022–

2025, 1993.

[31] J. Li, V. Slesarenko, P. I. Galich, and S. Rudykh. Instabilities and pattern for-

mations in 3D-printed deformable ﬁber composites. Composites Part B: Engi-

neering, 148:114–122, 2018.

[32] J. Li, V. Slesarenko, P. I. Galich, and S. Rudykh. Oblique shear wave propaga-

tion in ﬁnitely deformed layered composites. Mech. Res. Commun., 2018.

[33] J. Li, V. Slesarenko, and S. Rudykh. Microscopic instabilities and elastic wave

propagation in ﬁnitely deformed laminates with compressible hyperelastic

phases. Eur. J. Mech. - A/Solids, 73:126–136, 2019.

[34] O. Lopez-Pamies and P. Ponte Castaneda.˜ On the overall behavior, mi-

crostructure evolution, and macroscopic stability in reinforced rubbers at

large deformations: I—theory. J. Mech. Phys. Solids, 54:807–830, 2006.

[35] O. Lopez-Pamies and P. Ponte Castaneda.˜ On the overall behavior, mi-

crostructure evolution, and macroscopic stability in reinforced rubbers at

large deformations: II—application to cylindrical ﬁbers. J. Mech. Phys. Solids,

54:831–863, 2006.

95 [36] R. M. McMeeking and C. M. Landis. Electrostatic forces and stored energy for

deformable dielectric materials. J. Appl. Mech., Trans. ASME, 72:581–590, 2005.

[37] R. Ogden and B. Singh. Propagation of waves in an incompressible trans-

versely isotropic elastic solid with initial stress: Biot revisited. J. Mech. Mater.

Struct., 6(1-4):453–477, 2011.

[38] G. Rogerson and N. Scott. Doubly constrained elastic wave propagation. Int.

J. Solids Struct., 31(20):2769–2792, 1994.

[39] J. Rossiter, P. Walters, and B. Stoimenov. Printing 3D dielectric elastomer ac-

tuators for soft robotics. volume 7287, page 72870H. International Society for

Optics and Photonics, 2009.

[40] S. Rudykh and G. deBotton. Stability of anisotropic electroactive polymers

with application to layered media. Z. Angew. Math. Phys., 62:1131–1142, 2011.

[41] S. Rudykh and G. deBotton. Instabilities of hyperelastic ﬁber composites: mi-

cromechanical versus numerical analyses. J. Elasticity, 106:123–147, 2012.

[42] S. Rudykh, A. Lewinstein, G. Uner, and G. deBotton. Analysis of microstruc-

tural induced enhancement of electromechanical coupling in soft dielectrics.

Appl. Phys. Lett., 102:151905, 2013.

[43] S. Rytov. Acoustical properties of a thinly laminated medium. Sov. Phys.

Acoust, 2:68–80, 1956.

[44] N. Scott. Small vibrations of prestrained constrained elastic materials: The

idealized ﬁbre-reinforced material. Int. J. Solids Struct., 27(15):1969–1980, 1991.

96 [45] N. Scott. Waves in a homogeneously prestrained incompressible, almost inex-

tensible, ﬁbre-reinforced elastic material. Proc. R. Irish Acad. Sect. A, 92A(1):9–

36, 1992.

[46] N. Scott and M. Hayes. Small vibrations of a ﬁbre-reinforced composite. Q. J.

Mech. Appl. Math., 29(4):467–486, 1976.

[47] G. Shmuel and R. Band. Universality of the frequency spectrum of laminates.

J. Mech. Phys. Solids, 92:127–136, 2016.

[48] G. Shmuel and G. deBotton. Band-gaps in electrostatically controlled dielec-

tric laminates subjected to incremental shear motions. J. Mech. Phys. Solids,

60(11):1970–1981, 2012.

[49] G. Shmuel and G. deBotton. Corrigendum to ”Band-gaps in electrostatically

controlled dielectric laminates subjected to incremental shear motions” [J.

Mech. Phys. Solids 60 (2012) 19701981]. J. Mech. Phys. Solids, 105:21–24, 2017.

[50] V. Slesarenko, P. I. Galich, J. Li, N. X. Fang, and S. Rudykh. Foreshadowing

elastic instabilities by negative group velocity in soft composites. Appl. Phys.

Lett., 113(3):031901, 2018.

[51] V. Slesarenko and S. Rudykh. Microscopic and macroscopic instabilities in

hyperelastic ﬁber composites. J. Mech. Phys. Solids, 99:471–482, 2017.

[52] S. A. Spinelli and O. Lopez-Pamies. Some simple explicit results for the elastic

dielectric properties and stability of layered composites. Int. J. Eng. Sci., 88:15–

28, 2015.

97 [53] A. Srivastava. Metamaterial properties of periodic laminates. J. Mech. Phys.

Solids, 96:252–263, 2016.

[54] Z. Suo, X. Zhao, and W. H. Greene. A nonlinear ﬁeld theory of deformable

dielectrics. J. Mech. Phys. Solids, 56(2):467–486, 2008.

[55] L. Tian, L. Tevet-Deree, G. deBotton, and K. Bhattacharya. Dielectric elas-

tomer composites. J. Mech. Phys. Solids, 60:181–198, 2012.

[56] R. A. Toupin. The elastic dielectric. Arch. Rational. Mech. Anal., 5(6):849–915,

1956.

[57] C. Truesdell and W. Noll. The non-linear ﬁeld theories of mechanics. Springer,

1965.

[58] K. Volokh. Mechanics of Soft Materials. Springer Singapore, Singapore, 2016.

[59] J. Willis. Negative refraction in a laminate. J. Mech. Phys. Solids, 97:10–18, 2016.

[60] B. Wu, Y. Su, W. Chen, and C. Zhang. On guided circumferential waves in

soft electroactive tubes under radially inhomogeneous biasing ﬁelds. J. Mech.

Phys. Solids, 99:116–145, 2017.

[61] W.-P. Yang and L.-W. Chen. The tunable acoustic band gaps of two-

dimensional phononic crystals with a dielectric elastomer cylindrical actua-

tor. Smart Mater. Struct., 17(1):015011, 2008.

98

מניפולציית התקדמות גל אלסטי בחומרים גמישים לא ליניאריים באמצעות גירויים חיצוניים

חיבור על מחקר

לשם מילוי חלקי של הדרישות לקבלת התואר דוקטור לפילוסופיה

פבל גליץ'

הוגש לסנט הטכניון — מכון טכנולוגי לישראל אלול תשע "ח חיפה אוגוסט 2018

מניפולציית התקדמות גל אלסטי בחומרים גמישים לא ליניאריים באמצעות גירויים חיצוניים

פבל גליץ'